# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_(Sr3N)2[Fe(CN)4]
_database_code_depnum_ccdc_archive 'CCDC 2127618'
loop_
_audit_author_name
_audit_author_address
'Franziska Jach'
;TU Dresden
Germany
;
_audit_update_record             
;
2021-12-09 deposited with the CCDC.	2022-04-01 downloaded from the CCDC.
;

#------------------ CHEMICAL DATA

_chemical_formula_structural     (Sr3N)2[Fe(CN)4]
_chemical_formula_sum            'C4 Fe1 N6 Sr6'
_chemical_formula_weight         713.7

#------------------ UNIT CELL INFORMATION 

_space_group_crystal_system      trigonal
_space_group_name_H-M            'R 3 c'
_space_group_name_Hall           'R 3 -2"c'
_space_group_IT_number           161

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -y,x-y,z
3 -x+y,-x,z
4 -y,-x,z+1/2
5 -x+y,y,z+1/2
6 x,x-y,z+1/2
7 x+2/3,y+1/3,z+1/3
8 -y+2/3,x-y+1/3,z+1/3
9 -x+y+2/3,-x+1/3,z+1/3
10 -y+2/3,-x+1/3,z+5/6
11 -x+y+2/3,y+1/3,z+5/6
12 x+2/3,x-y+1/3,z+5/6
13 x+1/3,y+2/3,z+2/3
14 -y+1/3,x-y+2/3,z+2/3
15 -x+y+1/3,-x+2/3,z+2/3
16 -y+1/3,-x+2/3,z+1/6
17 -x+y+1/3,y+2/3,z+1/6
18 x+1/3,x-y+2/3,z+1/6

_cell_length_a                   7.0212(2)
_cell_length_b                   7.0212(2)
_cell_length_c                   41.555(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     1774.09(11)
_cell_formula_units_Z            6

_cell_measurement_reflns_used    351
_cell_measurement_theta_min      1.152
_cell_measurement_theta_max      8.933
_cell_measurement_temperature    293(1)
_cell_measurement_radiation      synchrotron
_cell_measurement_wavelength     0.32641(1)
_cell_special_details            
; 
The lattice parameters of (Sr3N)2[Fe(CN)4] were refined from the 
diffraction angles of 351 reflections, extracted by full profile fitting of 
the synchrotron powder pattern (beamline BL04-MSPD at ALBA, Barcelona, λ = 0.35434 Å, 
2.304 ° < 2Θ < 17.865 °) using Jana2006. In the final runs of the crystal structure 
refinement, these cell parameters were used for the interatomic distances calculation.
;
#------------------ CRYSTAL DATA

_exptl_crystal_description       'hexagonal plate-like'
_exptl_crystal_colour            'yellow transparent'
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    4.0078
_exptl_crystal_F_000             1920
_exptl_crystal_size_max          0.04
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.01
_exptl_absorpt_coefficient_mu    28.021
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.3860
_exptl_absorpt_correction_T_max  0.7469
_exptl_absorpt_process_details   
;
Multi-scan absorption correction performed with Apex2 Software (Bruker AXS) 
using the SADABS-2014/5 program. 
;

loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
1 0.52(2) 1 0 0 0 1 0 0 0 1
2 0.143(8) -1 0 0 0 -1 0 0 0 1
3 0.33(2) -1 0 0 0 -1 0 0 0 -1
4 0.012(8) 1 0 0 0 1 0 0 0 -1


#------------------ DATA COLLECTION INFORMATION

_diffrn_ambient_temperature      293(1)
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker Kappa APEX II'
_diffrn_detector                 'CCD plate'
_diffrn_detector_type            'APEX II'
_diffrn_detector_area_resol_mean ?
_diffrn_measurement_method       ?

_diffrn_reflns_number            39012
_diffrn_reflns_theta_min         2.95
_diffrn_reflns_theta_max         35.1
_diffrn_reflns_theta_full        35.1
_diffrn_measured_fraction_theta_max 1
_diffrn_measured_fraction_theta_full 1
_diffrn_reflns_av_R_equivalents  0.077
_diffrn_reflns_av_unetI/netI     0.041
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_l_min       -66
_diffrn_reflns_limit_l_max       66
_diffrn_reflns_reduction_process ?


#------------------ REFINEMENT DATA

_refine_special_details          
;Refined as 4 component twin including obverse/revere and inversion twinnng. Stacking faults were
included in the refinement of single crystal data using a disordered structural model. Besides
the main atom positions (labelled a),further minor positions (b, c) were introduced representing 
shifted main positions along [00z]. Thus, positions labelled a correspond to the idealized model.
Constrains and restrains were applied to stabilize the refinement.
Positions: x, y coordinates were kept equal for a, b, c positions, while z coordinates are shifted,
realized by fixed distances. Occupancies: occupancy parameters of a, b, c positions sum up to 1, 
respectively. Thermal displacement parameters were kept equal for a, b, c positions.,Twin
;

_reflns_number_total             2896
_reflns_number_gt                2387
_reflns_threshold_expression     I>3σ(I)
_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0427
_refine_ls_wR_factor_gt          0.0659
_refine_ls_R_factor_all          0.0536
_refine_ls_wR_factor_ref         0.0669
_refine_ls_goodness_of_fit_ref   2.46
_refine_ls_goodness_of_fit_gt    2.67
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         2896
_refine_ls_number_parameters     57
_refine_ls_number_restraints     21
_refine_ls_number_constraints    39
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0437
_refine_ls_shift/su_mean         0.0065
_refine_diff_density_max         1.90
_refine_diff_density_min         -1.23
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_extinction_expression ?
_refine_ls_abs_structure_details 
;  870 of Friedel pairs used in the refinement
;
_refine_ls_abs_structure_Flack   0.33(2)
_refine_ls_abs_structure_Rogers  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
Sr2a . Sr2c . 13.8517 0.0001
Fe1a . Fe1b . 13.8517 0.0001
N1a . N1c . 13.8517 0.0001
N2a . N2c . 13.8517 0.0001
C1a . C1b . 13.8517 0.0001
C2a . C2c . 13.8517 0.0001
N3ac . N3bc . 13.8517 0.0001
Fe1a . Fe1c . 27.7033 0.0001
Sr2a . Sr2b . 27.7033 0.0001
N1a . N1b . 27.7033 0.0001
N2a . N2b . 27.7033 0.0001
C1a . C1c . 27.7033 0.0001
C2a . C2b . 27.7033 0.0001
N3ac . N3ab . 27.7033 0.0001
Fe1b . Fe1c . 13.8517 0.0001
Sr2b . Sr2c . 13.8517 0.0001
N1c . N1b . 13.8517 0.0001
N2c . N2b . 13.8517 0.0001
C1c . C1b . 13.8517 0.0001
C2c . C2b . 13.8517 0.0001
N3ab . N3bc . 13.8517 0.0001

# start Validation Reply Form
_vrf_PLAT021_Sr3N2FeCN4          
;
PROBLEM: Ratio Unique / Expected Reflections too High ... 3.276
RESPONSE: Refinement as 4 component twin. List of reflections 
contains all reflections for each component. Thus, some 
reflections valid for more than one component are listed
more than once yielding an unusually high number of total 
reflections.
;
# end Validation Reply Form


#------------------ COMPUTER PROGRAMS USED 

_computing_data_collection       'Apex2 (Bruker)'
_computing_data_reduction        'Apex2 (Bruker)'
_computing_cell_refinement       
;
Petřiček, V.; DušÅ?ek, M.; Palatinus, L.
Crystallographic Computing System JANA2006: General features. 
Z. Kristallogr. 2014, 229, 345-352.
;
_computing_structure_solution    
;
Petřiček, V.; DušÅ?ek, M.; Palatinus, L.
Crystallographic Computing System JANA2006: General features. 
Z. Kristallogr. 2014, 229, 345-352.
;
_computing_structure_refinement  
;
Petřiček, V.; DušÅ?ek, M.; Palatinus, L.
Crystallographic Computing System JANA2006: General features. 
Z. Kristallogr. 2014, 229, 345-352.
;
_computing_molecular_graphics    'Diamond Version 4 (Brandenburg & Putz, 2005)'



#------ ATOMIC TYPES, COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C 0.0033 0.0016 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Fe 0.3463 0.8444 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
N 0.0061 0.0033 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Sr -1.5307 3.2498 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'


loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sr1 Sr 0.31098(12) 0.98233(17) 0.93337(2) Uani 0.0107(3) 18 1 d . . .
Sr2a Sr 0.66578(11) 0.92786(11) 0.861786(17) Uani 0.0077(2) 18 0.889(2) d . . .
Fe1a Fe 0 0 0.00017(4) Uani 0.0048(3) 6 0.874(4) d . . .
C1a C 0 0 0.0453(3) Uiso 0.0045(17) 6 0.881 d . . .
C2a C 0.7575(11) 0.0024(12) 0.98492(16) Uiso 0.0079(11) 18 0.881 d . . .
N1a N 0.666667 0.333333 0.9079(3) Uiso 0.017(2) 6 0.881 d . . .
N2a N 0.6016(13) 0.0008(12) 0.9726(2) Uiso 0.0190(14) 18 0.881 d . . .
N3ac N 0 0 0.89549(19) Uiso 0.0074(12) 6 0.911 d . . .
N3ab N 0 0 0.22882(19) Uiso 0.0074(12) 6 0.97 d . . .
N3bc N 0 0 0.56215(19) Uiso 0.0074(12) 6 0.119 d . . .
Sr2b Sr 0.66578(11) 0.92786(11) 0.195120(18) Uani 0.0077(2) 18 0.081(6) d . . .
Fe1b Fe 0 0 0.33350(4) Uani 0.0048(3) 6 0.086(7) d . . .
C1b C 0 0 0.3786(3) Uiso 0.0045(17) 6 0.089 d . . .
C2b C 0.7575(11) 0.0024(12) 0.31825(16) Uiso 0.0079(11) 18 0.089 d . . .
N1b N 0.666667 0.333333 0.2412(3) Uiso 0.017(2) 6 0.089 d . . .
N2b N 0.6016(13) 0.0008(12) 0.3060(2) Uiso 0.0190(14) 18 0.089 d . . .
Sr2c Sr 0.66578(11) 0.92786(11) 0.528453(18) Uani 0.0077(2) 18 0.030(7) d . . .
Fe1c Fe 0 0 0.66683(4) Uani 0.0048(3) 6 0.039(8) d . . .
C1c C 0 0 0.7119(3) Uiso 0.0045(17) 6 0.03 d . . .
C2c C 0.7575(11) 0.0024(12) 0.65158(16) Uiso 0.0079(11) 18 0.03 d . . .
N1c N 0.666667 0.333333 0.5745(3) Uiso 0.017(2) 6 0.03 d . . .
N2c N 0.6016(13) 0.0008(12) 0.6393(2) Uiso 0.0190(14) 18 0.03 d . . .





#------------------ MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sr1 Sr1 . 2_665 3.9817(17) ?
Sr1 Sr1 . 2_675 3.894(2) ?
Sr1 Sr1 . 2_775 4.2973(13) ?
Sr1 Sr1 . 3_465 3.8937(15) ?
Sr1 Sr1 . 3_565 3.9817(19) ?
Sr1 Sr1 . 3_575 4.2973(13) ?
Sr1 Sr2a . . 4.0192(13) ?
Sr1 Sr2a . 2_665 3.4246(12) ?
Sr1 Sr2a . 3_575 3.9899(14) ?
Sr1 Sr2a . 16_665 3.9978(12) ?
Sr1 Fe1a . 1_566 3.5718(15) ?
Sr1 Sr2c . 7_455 3.5228(13) ?
Sr1 Sr2c . 8_665 4.0480(12) ?
Sr1 Sr2c . 9_465 3.8736(12) ?
Sr1 Sr2c . 5_555 3.9679(13) ?
Sr1 Sr2b . 13_445 3.8853(12) ?
Sr1 Sr2b . 14_665 4.0139(14) ?
Sr1 Sr2b . 15_565 3.5488(13) ?
Sr1 Sr2b . 12_465 3.9912(13) ?
Sr1 N3ac . 1_565 2.744(5) ?
Sr1 N1a . 1_565 2.698(5) ?
Sr1 N3bc . 7_565 2.938(4) ?
Sr1 N2a . 1_565 2.564(9) ?
Sr1 N2a . 2_555 2.960(8) ?
Sr1 C2a . 2_555 2.910(7) ?
Sr1 C2a . 3_675 2.998(9) ?
Sr1 N3ab . 13_555 2.786(5) ?
Sr1 N1c . 7_455 2.532(5) ?
Sr1 N2c . 9_565 2.385(8) ?
Sr1 N2b . 13_455 2.946(7) ?
Sr1 N2b . 14_555 2.528(11) ?
Sr1 N1b . 13_455 2.486(5) ?
Sr1 C2b . 13_455 2.901(7) ?
Sr1 C2b . 15_665 3.056(10) ?
Sr2a Sr2a . 2_665 3.6868(11) ?
Sr2a Sr2a . 2_765 3.7045(14) ?
Sr2a Sr2a . 3_565 3.6868(9) ?
Sr2a Sr2a . 3_675 3.7045(11) ?
Sr2a Fe1a . 10_565 3.0772(10) ?
Sr2a Sr2c . 7_445 4.0537(10) ?
Sr2a Sr2c . 7_455 4.0537(13) ?
Sr2a Sr2c . 7_555 4.0537(10) ?
Sr2a Sr2c . 8_665 0.8720(11) ?
Sr2a Sr2c . 9_565 3.1817(15) ?
Sr2a Sr2b . 13_445 4.0537(10) ?
Sr2a Sr2b . 13_545 4.0537(13) ?
Sr2a Sr2b . 13_555 4.0537(10) ?
Sr2a Sr2b . 14_655 3.1817(12) ?
Sr2a Sr2b . 15_565 0.8720(15) ?
Sr2a N3ac . 1_665 2.556(4) ?
Sr2a N2a . 10_564 2.698(9) ?
Sr2a C2a . 10_564 3.058(8) ?
Sr2a C2a . 12_454 3.055(10) ?
Sr2a Fe1c . 16_555 2.4316(10) ?
Sr2a Fe1b . 4_665 2.4405(11) ?
Sr2a N3ab . 13_555 2.548(4) ?
Sr2a N1c . 7_455 2.863(8) ?
Sr2a N1b . 13_555 2.870(8) ?
Sr2a C2c . 16_565 2.917(8) ?
Sr2a C2c . 17_655 2.416(8) ?
Sr2a C2b . 4_675 2.904(6) ?
Sr2a C2b . 6_555 2.437(10) ?
Sr2a C1a . 10_565 2.928(3) ?
Sr2a C1c . 16_555 2.240(4) ?
Sr2a C1b . 4_665 2.250(4) ?
Fe1a Sr2c . 4_664 2.4405(11) ?
Fe1a Sr2c . 5_544 2.4405(13) ?
Fe1a Sr2c . 6_454 2.4405(10) ?
Fe1a Sr2b . 10_554 2.4316(10) ?
Fe1a Sr2b . 11_444 2.4316(12) ?
Fe1a Sr2b . 12_454 2.4316(11) ?
Fe1a C2a . 1_454 1.825(9) ?
Fe1a C2a . 2_544 1.825(12) ?
Fe1a C2a . 3_664 1.825(7) ?
Fe1a C1a . . 1.874(12) ?
Sr2c Sr2c . 2_665 3.6868(11) ?
Sr2c Sr2c . 2_765 3.7045(14) ?
Sr2c Sr2c . 3_565 3.6868(9) ?
Sr2c Sr2c . 3_675 3.7045(11) ?
Sr2c Sr2b . 7_445 4.0537(10) ?
Sr2c Sr2b . 7_455 4.0537(13) ?
Sr2c Sr2b . 7_555 4.0537(10) ?
Sr2c Sr2b . 8_665 0.8720(11) ?
Sr2c Sr2b . 9_565 3.1817(15) ?
Sr2c N3ac . 13_554 2.548(4) ?
Sr2c N1a . 13_554 2.870(8) ?
Sr2c N3bc . 1_665 2.556(4) ?
Sr2c C2a . 4_674 2.904(6) ?
Sr2c C2a . 6_554 2.437(10) ?
Sr2c Fe1c . 10_564 3.0772(10) ?
Sr2c Fe1b . 16_555 2.4316(10) ?
Sr2c N2c . 10_564 2.698(9) ?
Sr2c N1b . 7_455 2.863(8) ?
Sr2c C2c . 10_564 3.058(8) ?
Sr2c C2c . 12_454 3.055(10) ?
Sr2c C2b . 16_565 2.917(8) ?
Sr2c C2b . 17_655 2.416(8) ?
Sr2c C1a . 4_665 2.250(4) ?
Sr2c C1c . 10_564 2.928(3) ?
Sr2c C1b . 16_555 2.240(4) ?
Sr2b Sr2b . 2_665 3.6868(11) ?
Sr2b Sr2b . 2_765 3.7045(14) ?
Sr2b Sr2b . 3_565 3.6868(9) ?
Sr2b Sr2b . 3_675 3.7045(11) ?
Sr2b N1a . 7_454 2.863(8) ?
Sr2b N3bc . 13_554 2.548(4) ?
Sr2b C2a . 16_564 2.917(8) ?
Sr2b C2a . 17_654 2.416(8) ?
Sr2b Fe1c . 4_664 2.4405(11) ?
Sr2b Fe1b . 10_564 3.0772(10) ?
Sr2b N3ab . 1_665 2.556(4) ?
Sr2b N1c . 13_554 2.870(8) ?
Sr2b N2b . 10_564 2.698(9) ?
Sr2b C2c . 4_674 2.904(6) ?
Sr2b C2c . 6_554 2.437(10) ?
Sr2b C2b . 10_564 3.058(8) ?
Sr2b C2b . 12_454 3.055(10) ?
Sr2b C1a . 16_555 2.240(4) ?
Sr2b C1c . 4_664 2.250(4) ?
Sr2b C1b . 10_564 2.928(3) ?
N3ac N1b . 13_445 0.514(15) ?
N3ac C1b . 4_555 0.702(14) ?
N1a N3bc . 7_555 0.514(15) ?
N1a C1a . 10_555 1.216(17) ?
N3bc C1a . 4_555 0.702(14) ?
N2a C2a . . 1.203(13) ?
N2a N2c . 8_545 0.796(16) ?
N2a N2b . 15_655 0.796(13) ?
N2a C2c . 8_545 0.750(11) ?
N2a C2b . 15_655 0.772(11) ?
C2a N2c . 8_545 0.772(10) ?
C2a N2b . 15_655 0.750(14) ?
C2a C2c . 8_545 1.090(16) ?
C2a C2b . 15_655 1.090(12) ?
Fe1c C2c . 1_455 1.825(9) ?
Fe1c C2c . 2_545 1.825(12) ?
Fe1c C2c . 3_665 1.825(7) ?
Fe1c C1c . . 1.874(12) ?
Fe1b C2b . 1_455 1.825(9) ?
Fe1b C2b . 2_545 1.825(12) ?
Fe1b C2b . 3_665 1.825(7) ?
Fe1b C1b . . 1.874(12) ?
N3ab N1c . 13_444 0.514(15) ?
N3ab C1c . 4_554 0.702(14) ?
N1c C1c . 10_554 1.216(17) ?
N2c N2b . 8_545 0.796(16) ?
N2c C2c . . 1.203(13) ?
N2c C2b . 8_545 0.750(11) ?
N2b C2c . 15_654 0.772(11) ?
N2b C2b . . 1.203(13) ?
N1b C1b . 10_554 1.216(17) ?
C2c C2b . 8_545 1.090(16) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Sr1 Sr1 Sr1 2_665 . 2_675 126.13(3) ?
Sr1 Sr1 Sr1 2_665 . 2_775 115.95(4) ?
Sr1 Sr1 Sr1 2_665 . 3_465 66.13(3) ?
Sr1 Sr1 Sr1 2_665 . 3_565 60.00(3) ?
Sr1 Sr1 Sr1 2_665 . 3_575 175.95(4) ?
Sr1 Sr1 Sr2a 2_665 . . 83.01(3) ?
Sr1 Sr1 Sr2a 2_665 . 2_665 65.23(3) ?
Sr1 Sr1 Sr2a 2_665 . 3_575 123.97(3) ?
Sr1 Sr1 Sr2a 2_665 . 16_665 91.11(3) ?
Sr1 Sr1 Fe1a 2_665 . 1_566 93.85(2) ?
Sr1 Sr1 Sr2c 2_665 . 7_455 119.63(3) ?
Sr1 Sr1 Sr2c 2_665 . 8_665 95.40(3) ?
Sr1 Sr1 Sr2c 2_665 . 9_465 62.02(2) ?
Sr1 Sr1 Sr2c 2_665 . 5_555 85.35(3) ?
Sr1 Sr1 Sr2b 2_665 . 13_445 53.61(2) ?
Sr1 Sr1 Sr2b 2_665 . 14_665 130.59(3) ?
Sr1 Sr1 Sr2b 2_665 . 15_565 89.97(3) ?
Sr1 Sr1 Sr2b 2_665 . 12_465 97.91(3) ?
Sr1 Sr1 N3ac 2_665 . 1_565 95.02(3) ?
Sr1 Sr1 N1a 2_665 . 1_565 139.63(13) ?
Sr1 Sr1 N3bc 2_665 . 7_565 134.40(9) ?
Sr1 Sr1 N2a 2_665 . 1_565 89.89(17) ?
Sr1 Sr1 N2a 2_665 . 2_555 40.1(2) ?
Sr1 Sr1 C2a 2_665 . 2_555 63.5(2) ?
Sr1 Sr1 C2a 2_665 . 3_675 123.64(12) ?
Sr1 Sr1 N3ab 2_665 . 13_555 44.39(9) ?
Sr1 Sr1 N1c 2_665 . 7_455 38.15(15) ?
Sr1 Sr1 N2c 2_665 . 9_565 51.9(2) ?
Sr1 Sr1 N2b 2_665 . 13_455 51.84(18) ?
Sr1 Sr1 N2b 2_665 . 14_555 134.80(19) ?
Sr1 Sr1 N1b 2_665 . 13_455 95.54(3) ?
Sr1 Sr1 C2b 2_665 . 13_455 49.73(16) ?
Sr1 Sr1 C2b 2_665 . 15_665 79.25(12) ?
Sr1 Sr1 Sr1 2_675 . 2_775 117.92(3) ?
Sr1 Sr1 Sr1 2_675 . 3_465 60.00(3) ?
Sr1 Sr1 Sr1 2_675 . 3_565 173.87(3) ?
Sr1 Sr1 Sr1 2_675 . 3_575 57.92(3) ?
Sr1 Sr1 Sr2a 2_675 . . 127.30(3) ?
Sr1 Sr1 Sr2a 2_675 . 2_665 91.92(3) ?
Sr1 Sr1 Sr2a 2_675 . 3_575 51.48(3) ?
Sr1 Sr1 Sr2a 2_675 . 16_665 96.35(3) ?
Sr1 Sr1 Fe1a 2_675 . 1_566 56.97(3) ?
Sr1 Sr1 Sr2c 2_675 . 7_455 62.74(3) ?
Sr1 Sr1 Sr2c 2_675 . 8_665 119.15(3) ?
Sr1 Sr1 Sr2c 2_675 . 9_465 85.67(3) ?
Sr1 Sr1 Sr2c 2_675 . 5_555 90.74(3) ?
Sr1 Sr1 Sr2b 2_675 . 13_445 98.57(3) ?
Sr1 Sr1 Sr2b 2_675 . 14_665 58.83(3) ?
Sr1 Sr1 Sr2b 2_675 . 15_565 116.15(4) ?
Sr1 Sr1 Sr2b 2_675 . 12_465 83.84(3) ?
Sr1 Sr1 N3ac 2_675 . 1_565 44.82(10) ?
Sr1 Sr1 N1a 2_675 . 1_565 88.09(3) ?
Sr1 Sr1 N3bc 2_675 . 7_565 88.24(3) ?
Sr1 Sr1 N2a 2_675 . 1_565 128.6(2) ?
Sr1 Sr1 N2a 2_675 . 2_555 100.5(2) ?
Sr1 Sr1 C2a 2_675 . 2_555 81.5(3) ?
Sr1 Sr1 C2a 2_675 . 3_675 47.8(2) ?
Sr1 Sr1 N3ab 2_675 . 13_555 138.98(11) ?
Sr1 Sr1 N1c 2_675 . 7_455 146.14(18) ?
Sr1 Sr1 N2c 2_675 . 9_565 92.8(3) ?
Sr1 Sr1 N2b 2_675 . 13_455 85.0(2) ?
Sr1 Sr1 N2b 2_675 . 14_555 49.2(2) ?
Sr1 Sr1 N1b 2_675 . 13_455 38.44(16) ?
Sr1 Sr1 C2b 2_675 . 13_455 103.0(2) ?
Sr1 Sr1 C2b 2_675 . 15_665 131.76(18) ?
Sr1 Sr1 Sr1 2_775 . 3_465 177.92(4) ?
Sr1 Sr1 Sr1 2_775 . 3_565 55.95(3) ?
Sr1 Sr1 Sr1 2_775 . 3_575 60.00(3) ?
Sr1 Sr1 Sr2a 2_775 . . 57.22(2) ?
Sr1 Sr1 Sr2a 2_775 . 2_665 114.90(3) ?
Sr1 Sr1 Sr2a 2_775 . 3_575 94.71(3) ?
Sr1 Sr1 Sr2a 2_775 . 16_665 81.70(2) ?
Sr1 Sr1 Fe1a 2_775 . 1_566 122.23(3) ?
Sr1 Sr1 Sr2c 2_775 . 7_455 88.23(2) ?
Sr1 Sr1 Sr2c 2_775 . 8_665 49.827(19) ?
Sr1 Sr1 Sr2c 2_775 . 9_465 126.68(3) ?
Sr1 Sr1 Sr2c 2_775 . 5_555 94.26(3) ?
Sr1 Sr1 Sr2b 2_775 . 13_445 118.90(3) ?
Sr1 Sr1 Sr2b 2_775 . 14_665 82.21(2) ?
Sr1 Sr1 Sr2b 2_775 . 15_565 60.65(2) ?
Sr1 Sr1 Sr2b 2_775 . 12_465 88.22(2) ?
Sr1 Sr1 N3ac 2_775 . 1_565 133.95(9) ?
Sr1 Sr1 N1a 2_775 . 1_565 37.22(14) ?
Sr1 Sr1 N3bc 2_775 . 7_565 43.01(9) ?
Sr1 Sr1 N2a 2_775 . 1_565 46.13(16) ?
Sr1 Sr1 N2a 2_775 . 2_555 129.36(19) ?
Sr1 Sr1 C2a 2_775 . 2_555 130.77(16) ?
Sr1 Sr1 C2a 2_775 . 3_675 98.15(18) ?
Sr1 Sr1 N3ab 2_775 . 13_555 86.66(3) ?
Sr1 Sr1 N1c 2_775 . 7_455 86.32(3) ?
Sr1 Sr1 N2c 2_775 . 9_565 128.4(3) ?
Sr1 Sr1 N2b 2_775 . 13_455 140.58(18) ?
Sr1 Sr1 N2b 2_775 . 14_555 87.53(17) ?
Sr1 Sr1 N1b 2_775 . 13_455 140.02(15) ?
Sr1 Sr1 C2b 2_775 . 13_455 117.12(16) ?
Sr1 Sr1 C2b 2_775 . 15_665 57.50(15) ?
Sr1 Sr1 Sr1 3_465 . 3_565 126.13(3) ?
Sr1 Sr1 Sr1 3_465 . 3_575 117.92(4) ?
Sr1 Sr1 Sr2a 3_465 . . 123.75(3) ?
Sr1 Sr1 Sr2a 3_465 . 2_665 65.71(2) ?
Sr1 Sr1 Sr2a 3_465 . 3_575 83.91(3) ?
Sr1 Sr1 Sr2a 3_465 . 16_665 98.39(3) ?
Sr1 Sr1 Fe1a 3_465 . 1_566 56.97(2) ?
Sr1 Sr1 Sr2c 3_465 . 7_455 90.66(3) ?
Sr1 Sr1 Sr2c 3_465 . 8_665 130.71(3) ?
Sr1 Sr1 Sr2c 3_465 . 9_465 53.94(2) ?
Sr1 Sr1 Sr2c 3_465 . 5_555 85.85(3) ?
Sr1 Sr1 Sr2b 3_465 . 13_445 62.13(2) ?
Sr1 Sr1 Sr2b 3_465 . 14_665 96.41(3) ?
Sr1 Sr1 Sr2b 3_465 . 15_565 119.90(3) ?
Sr1 Sr1 Sr2b 3_465 . 12_465 91.50(3) ?
Sr1 Sr1 N3ac 3_465 . 1_565 44.82(9) ?
Sr1 Sr1 N1a 3_465 . 1_565 141.18(14) ?
Sr1 Sr1 N3bc 3_465 . 7_565 135.68(9) ?
Sr1 Sr1 N2a 3_465 . 1_565 134.82(17) ?
Sr1 Sr1 N2a 3_465 . 2_555 52.11(19) ?
Sr1 Sr1 C2a 3_465 . 2_555 49.75(16) ?
Sr1 Sr1 C2a 3_465 . 3_675 80.41(18) ?
Sr1 Sr1 N3ab 3_465 . 13_555 95.05(3) ?
Sr1 Sr1 N1c 3_465 . 7_455 95.56(3) ?
Sr1 Sr1 N2c 3_465 . 9_565 52.7(3) ?
Sr1 Sr1 N2b 3_465 . 13_455 40.47(18) ?
Sr1 Sr1 N2b 3_465 . 14_555 90.88(17) ?
Sr1 Sr1 N1b 3_465 . 13_455 38.44(16) ?
Sr1 Sr1 C2b 3_465 . 13_455 64.06(16) ?
Sr1 Sr1 C2b 3_465 . 15_665 123.64(15) ?
Sr1 Sr1 Sr1 3_565 . 3_575 115.95(3) ?
Sr1 Sr1 Sr2a 3_565 . . 50.68(2) ?
Sr1 Sr1 Sr2a 3_565 . 2_665 91.11(3) ?
Sr1 Sr1 Sr2a 3_565 . 3_575 126.44(3) ?
Sr1 Sr1 Sr2a 3_565 . 16_665 83.04(3) ?
Sr1 Sr1 Fe1a 3_565 . 1_566 125.14(3) ?
Sr1 Sr1 Sr2c 3_565 . 7_455 115.20(3) ?
Sr1 Sr1 Sr2c 3_565 . 8_665 57.68(3) ?
Sr1 Sr1 Sr2c 3_565 . 9_465 98.22(3) ?
Sr1 Sr1 Sr2c 3_565 . 5_555 89.82(3) ?
Sr1 Sr1 Sr2b 3_565 . 13_445 85.34(3) ?
Sr1 Sr1 Sr2b 3_565 . 14_665 117.96(3) ?
Sr1 Sr1 Sr2b 3_565 . 15_565 61.80(3) ?
Sr1 Sr1 Sr2b 3_565 . 12_465 95.56(3) ?
Sr1 Sr1 N3ac 3_565 . 1_565 138.51(11) ?
Sr1 Sr1 N1a 3_565 . 1_565 86.28(3) ?
Sr1 Sr1 N3bc 3_565 . 7_565 86.58(3) ?
Sr1 Sr1 N2a 3_565 . 1_565 48.0(2) ?
Sr1 Sr1 N2a 3_565 . 2_555 84.6(2) ?
Sr1 Sr1 C2a 3_565 . 2_555 102.6(2) ?
Sr1 Sr1 C2a 3_565 . 3_675 130.3(2) ?
Sr1 Sr1 N3ab 3_565 . 13_555 44.39(9) ?
Sr1 Sr1 N1c 3_565 . 7_455 38.15(15) ?
Sr1 Sr1 N2c 3_565 . 9_565 91.7(3) ?
Sr1 Sr1 N2b 3_565 . 13_455 100.1(2) ?
Sr1 Sr1 N2b 3_565 . 14_555 127.4(2) ?
Sr1 Sr1 N1b 3_565 . 13_455 145.80(19) ?
Sr1 Sr1 C2b 3_565 . 13_455 81.0(2) ?
Sr1 Sr1 C2b 3_565 . 15_665 46.41(18) ?
Sr1 Sr1 Sr2a 3_575 . . 94.29(2) ?
Sr1 Sr1 Sr2a 3_575 . 2_665 115.89(3) ?
Sr1 Sr1 Sr2a 3_575 . 3_575 57.88(2) ?
Sr1 Sr1 Sr2a 3_575 . 16_665 88.28(2) ?
Sr1 Sr1 Fe1a 3_575 . 1_566 88.69(3) ?
Sr1 Sr1 Sr2c 3_575 . 7_455 61.41(2) ?
Sr1 Sr1 Sr2c 3_575 . 8_665 81.88(3) ?
Sr1 Sr1 Sr2c 3_575 . 9_465 119.92(3) ?
Sr1 Sr1 Sr2c 3_575 . 5_555 94.81(3) ?
Sr1 Sr1 Sr2b 3_575 . 13_445 127.54(3) ?
Sr1 Sr1 Sr2b 3_575 . 14_665 50.41(2) ?
Sr1 Sr1 Sr2b 3_575 . 15_565 87.82(3) ?
Sr1 Sr1 Sr2b 3_575 . 12_465 82.24(3) ?
Sr1 Sr1 N3ac 3_575 . 1_565 88.30(3) ?
Sr1 Sr1 N1a 3_575 . 1_565 37.22(14) ?
Sr1 Sr1 N3bc 3_575 . 7_565 43.01(9) ?
Sr1 Sr1 N2a 3_575 . 1_565 86.98(16) ?
Sr1 Sr1 N2a 3_575 . 2_555 141.9(2) ?
Sr1 Sr1 C2a 3_575 . 2_555 118.7(2) ?
Sr1 Sr1 C2a 3_575 . 3_675 58.50(12) ?
Sr1 Sr1 N3ab 3_575 . 13_555 133.13(9) ?
Sr1 Sr1 N1c 3_575 . 7_455 138.80(14) ?
Sr1 Sr1 N2c 3_575 . 9_565 130.0(2) ?
Sr1 Sr1 N2b 3_575 . 13_455 130.98(18) ?
Sr1 Sr1 N2b 3_575 . 14_555 46.99(18) ?
Sr1 Sr1 N1b 3_575 . 13_455 88.12(4) ?
Sr1 Sr1 C2b 3_575 . 13_455 131.17(15) ?
Sr1 Sr1 C2b 3_575 . 15_665 97.90(12) ?
Sr2a Sr1 Sr2a . . 2_665 58.73(2) ?
Sr2a Sr1 Sr2a . . 3_575 75.90(3) ?
Sr2a Sr1 Sr2a . . 16_665 129.34(3) ?
Sr2a Sr1 Fe1a . . 1_566 175.71(4) ?
Sr2a Sr1 Sr2c . . 7_455 64.63(2) ?
Sr2a Sr1 Sr2c . . 8_665 12.404(17) ?
Sr2a Sr1 Sr2c . . 9_465 70.30(2) ?
Sr2a Sr1 Sr2c . . 5_555 139.09(4) ?
Sr2a Sr1 Sr2b . . 13_445 61.68(2) ?
Sr2a Sr1 Sr2b . . 14_665 68.92(2) ?
Sr2a Sr1 Sr2b . . 15_565 11.16(2) ?
Sr2a Sr1 Sr2b . . 12_465 140.43(3) ?
Sr2a Sr1 N3ac . . 1_565 97.16(13) ?
Sr2a Sr1 N1a . . 1_565 57.41(17) ?
Sr2a Sr1 N3bc . . 7_565 51.39(8) ?
Sr2a Sr1 N2a . . 1_565 87.7(2) ?
Sr2a Sr1 N2a . . 2_555 122.3(2) ?
Sr2a Sr1 C2a . . 2_555 145.8(2) ?
Sr2a Sr1 C2a . . 3_675 151.51(14) ?
Sr2a Sr1 N3ab . . 13_555 38.92(8) ?
Sr2a Sr1 N1c . . 7_455 45.09(18) ?
Sr2a Sr1 N2c . . 9_565 133.5(3) ?
Sr2a Sr1 N2b . . 13_455 134.73(18) ?
Sr2a Sr1 N2b . . 14_555 139.33(16) ?
Sr2a Sr1 N1b . . 13_455 106.9(3) ?
Sr2a Sr1 C2b . . 13_455 126.52(19) ?
Sr2a Sr1 C2b . . 15_665 92.34(19) ?
Sr2a Sr1 Sr2a 2_665 . 3_575 59.37(3) ?
Sr2a Sr1 Sr2a 2_665 . 16_665 155.03(3) ?
Sr2a Sr1 Fe1a 2_665 . 1_566 122.53(3) ?
Sr2a Sr1 Sr2c 2_665 . 7_455 54.49(2) ?
Sr2a Sr1 Sr2c 2_665 . 8_665 65.08(2) ?
Sr2a Sr1 Sr2c 2_665 . 9_465 11.781(19) ?
Sr2a Sr1 Sr2c 2_665 . 5_555 145.04(3) ?
Sr2a Sr1 Sr2b 2_665 . 13_445 11.65(2) ?
Sr2a Sr1 Sr2b 2_665 . 14_665 65.49(3) ?
Sr2a Sr1 Sr2b 2_665 . 15_565 54.26(2) ?
Sr2a Sr1 Sr2b 2_665 . 12_465 155.37(2) ?
Sr2a Sr1 N3ac 2_665 . 1_565 47.40(11) ?
Sr2a Sr1 N1a 2_665 . 1_565 96.5(2) ?
Sr2a Sr1 N3bc 2_665 . 7_565 87.29(13) ?
Sr2a Sr1 N2a 2_665 . 1_565 139.1(2) ?
Sr2a Sr1 N2a 2_665 . 2_555 94.01(16) ?
Sr2a Sr1 C2a 2_665 . 2_555 108.55(14) ?
Sr2a Sr1 C2a 2_665 . 3_675 137.7(2) ?
Sr2a Sr1 N3ab 2_665 . 13_555 47.07(11) ?
Sr2a Sr1 N1c 2_665 . 7_455 55.0(2) ?
Sr2a Sr1 N2c 2_665 . 9_565 103.44(19) ?
Sr2a Sr1 N2b 2_665 . 13_455 94.26(15) ?
Sr2a Sr1 N2b 2_665 . 14_555 141.1(2) ?
Sr2a Sr1 N1b 2_665 . 13_455 55.4(2) ?
Sr2a Sr1 C2b 2_665 . 13_455 108.64(13) ?
Sr2a Sr1 C2b 2_665 . 15_665 135.45(17) ?
Sr2a Sr1 Sr2a 3_575 . 16_665 141.35(4) ?
Sr2a Sr1 Fe1a 3_575 . 1_566 108.33(4) ?
Sr2a Sr1 Sr2c 3_575 . 7_455 11.27(2) ?
Sr2a Sr1 Sr2c 3_575 . 8_665 69.12(3) ?
Sr2a Sr1 Sr2c 3_575 . 9_465 62.04(2) ?
Sr2a Sr1 Sr2c 3_575 . 5_555 140.53(4) ?
Sr2a Sr1 Sr2b 3_575 . 13_445 70.75(2) ?
Sr2a Sr1 Sr2b 3_575 . 14_665 12.505(17) ?
Sr2a Sr1 Sr2b 3_575 . 15_565 64.75(3) ?
Sr2a Sr1 Sr2b 3_575 . 12_465 130.50(4) ?
Sr2a Sr1 N3ac 3_575 . 1_565 39.43(8) ?
Sr2a Sr1 N1a 3_575 . 1_565 57.88(17) ?
Sr2a Sr1 N3bc 3_575 . 7_565 51.79(8) ?
Sr2a Sr1 N2a 3_575 . 1_565 139.07(15) ?
Sr2a Sr1 N2a 3_575 . 2_555 135.84(19) ?
Sr2a Sr1 C2a 3_575 . 2_555 127.8(2) ?
Sr2a Sr1 C2a 3_575 . 3_675 93.90(17) ?
Sr2a Sr1 N3ab 3_575 . 13_555 97.34(13) ?
Sr2a Sr1 N1c 3_575 . 7_455 107.0(3) ?
Sr2a Sr1 N2c 3_575 . 9_565 135.5(3) ?
Sr2a Sr1 N2b 3_575 . 13_455 123.71(19) ?
Sr2a Sr1 N2b 3_575 . 14_555 88.9(2) ?
Sr2a Sr1 N1b 3_575 . 13_455 45.68(18) ?
Sr2a Sr1 C2b 3_575 . 13_455 147.33(17) ?
Sr2a Sr1 C2b 3_575 . 15_665 151.27(13) ?
Sr2a Sr1 Fe1a 16_665 . 1_566 47.56(2) ?
Sr2a Sr1 Sr2c 16_665 . 7_455 148.89(4) ?
Sr2a Sr1 Sr2c 16_665 . 8_665 128.53(3) ?
Sr2a Sr1 Sr2c 16_665 . 9_465 146.50(2) ?
Sr2a Sr1 Sr2c 16_665 . 5_555 12.563(17) ?
Sr2a Sr1 Sr2b 16_665 . 13_445 143.68(3) ?
Sr2a Sr1 Sr2b 16_665 . 14_665 138.15(3) ?
Sr2a Sr1 Sr2b 16_665 . 15_565 138.25(3) ?
Sr2a Sr1 Sr2b 16_665 . 12_465 12.53(2) ?
Sr2a Sr1 N3ac 16_665 . 1_565 133.50(14) ?
Sr2a Sr1 N1a 16_665 . 1_565 107.2(2) ?
Sr2a Sr1 N3bc 16_665 . 7_565 116.40(13) ?
Sr2a Sr1 N2a 16_665 . 1_565 41.8(2) ?
Sr2a Sr1 N2a 16_665 . 2_555 61.35(16) ?
Sr2a Sr1 C2a 16_665 . 2_555 50.06(14) ?
Sr2a Sr1 C2a 16_665 . 3_675 49.28(19) ?
Sr2a Sr1 N3ab 16_665 . 13_555 120.66(13) ?
Sr2a Sr1 N1c 16_665 . 7_455 111.1(3) ?
Sr2a Sr1 N2c 16_665 . 9_565 52.8(2) ?
Sr2a Sr1 N2b 16_665 . 13_455 63.21(16) ?
Sr2a Sr1 N2b 16_665 . 14_555 52.6(2) ?
Sr2a Sr1 N1b 16_665 . 13_455 123.8(3) ?
Sr2a Sr1 C2b 16_665 . 13_455 46.51(12) ?
Sr2a Sr1 C2b 16_665 . 15_665 37.52(19) ?
Fe1a Sr1 Sr2c 1_566 . 7_455 119.60(4) ?
Fe1a Sr1 Sr2c 1_566 . 8_665 170.08(3) ?
Fe1a Sr1 Sr2c 1_566 . 9_465 110.82(3) ?
Fe1a Sr1 Sr2c 1_566 . 5_555 37.31(2) ?
Fe1a Sr1 Sr2b 1_566 . 13_445 118.63(2) ?
Fe1a Sr1 Sr2b 1_566 . 14_665 115.37(4) ?
Fe1a Sr1 Sr2b 1_566 . 15_565 173.06(4) ?
Fe1a Sr1 Sr2b 1_566 . 12_465 36.98(2) ?
Fe1a Sr1 N3ac 1_566 . 1_565 86.00(13) ?
Fe1a Sr1 N1a 1_566 . 1_565 125.20(18) ?
Fe1a Sr1 N3bc 1_566 . 7_565 131.70(9) ?
Fe1a Sr1 N2a 1_566 . 1_565 89.4(2) ?
Fe1a Sr1 N2a 1_566 . 2_555 54.2(2) ?
Fe1a Sr1 C2a 1_566 . 2_555 30.6(2) ?
Fe1a Sr1 C2a 1_566 . 3_675 30.70(13) ?
Fe1a Sr1 N3ab 1_566 . 13_555 138.18(9) ?
Fe1a Sr1 N1c 1_566 . 7_455 131.49(19) ?
Fe1a Sr1 N2c 1_566 . 9_565 42.8(3) ?
Fe1a Sr1 N2b 1_566 . 13_455 42.43(17) ?
Fe1a Sr1 N2b 1_566 . 14_555 42.83(16) ?
Fe1a Sr1 N1b 1_566 . 13_455 76.3(3) ?
Fe1a Sr1 C2b 1_566 . 13_455 49.40(19) ?
Fe1a Sr1 C2b 1_566 . 15_665 84.18(19) ?
Sr2c Sr1 Sr2c 7_455 . 8_665 58.10(2) ?
Sr2c Sr1 Sr2c 7_455 . 9_465 59.57(2) ?
Sr2c Sr1 Sr2c 7_455 . 5_555 150.69(4) ?
Sr2c Sr1 Sr2b 7_455 . 13_445 66.14(2) ?
Sr2c Sr1 Sr2b 7_455 . 14_665 10.995(16) ?
Sr2c Sr1 Sr2b 7_455 . 15_565 53.48(3) ?
Sr2c Sr1 Sr2b 7_455 . 12_465 139.57(4) ?
Sr2c Sr1 N3ac 7_455 . 1_565 45.93(10) ?
Sr2c Sr1 N1a 7_455 . 1_565 53.0(2) ?
Sr2c Sr1 N3bc 7_455 . 7_565 45.51(10) ?
Sr2c Sr1 N2a 7_455 . 1_565 134.20(16) ?
Sr2c Sr1 N2a 7_455 . 2_555 140.80(17) ?
Sr2c Sr1 C2a 7_455 . 2_555 137.5(2) ?
Sr2c Sr1 C2a 7_455 . 3_675 103.97(16) ?
Sr2c Sr1 N3ab 7_455 . 13_555 87.78(13) ?
Sr2c Sr1 N1c 7_455 . 7_455 97.4(3) ?
Sr2c Sr1 N2c 7_455 . 9_565 143.3(3) ?
Sr2c Sr1 N2b 7_455 . 13_455 131.13(19) ?
Sr2c Sr1 N2b 7_455 . 14_555 97.8(2) ?
Sr2c Sr1 N1b 7_455 . 13_455 53.6(2) ?
Sr2c Sr1 C2b 7_455 . 13_455 154.61(15) ?
Sr2c Sr1 C2b 7_455 . 15_665 145.70(15) ?
Sr2c Sr1 Sr2c 8_665 . 9_465 76.86(2) ?
Sr2c Sr1 Sr2c 8_665 . 5_555 140.21(3) ?
Sr2c Sr1 Sr2b 8_665 . 13_445 70.13(2) ?
Sr2c Sr1 Sr2b 8_665 . 14_665 60.37(2) ?
Sr2c Sr1 Sr2b 8_665 . 15_565 10.824(17) ?
Sr2c Sr1 Sr2b 8_665 . 12_465 137.41(3) ?
Sr2c Sr1 N3ac 8_665 . 1_565 96.74(13) ?
Sr2c Sr1 N1a 8_665 . 1_565 45.07(17) ?
Sr2c Sr1 N3bc 8_665 . 7_565 39.01(8) ?
Sr2c Sr1 N2a 8_665 . 1_565 87.1(2) ?
Sr2c Sr1 N2a 8_665 . 2_555 134.5(2) ?
Sr2c Sr1 C2a 8_665 . 2_555 157.7(2) ?
Sr2c Sr1 C2a 8_665 . 3_675 139.46(14) ?
Sr2c Sr1 N3ab 8_665 . 13_555 51.31(8) ?
Sr2c Sr1 N1c 8_665 . 7_455 57.40(17) ?
Sr2c Sr1 N2c 8_665 . 9_565 145.3(3) ?
Sr2c Sr1 N2b 8_665 . 13_455 147.14(18) ?
Sr2c Sr1 N2b 8_665 . 14_555 127.31(16) ?
Sr2c Sr1 N1b 8_665 . 13_455 106.3(3) ?
Sr2c Sr1 C2b 8_665 . 13_455 137.1(2) ?
Sr2c Sr1 C2b 8_665 . 15_665 94.03(18) ?
Sr2c Sr1 Sr2c 9_465 . 5_555 135.06(2) ?
Sr2c Sr1 Sr2b 9_465 . 13_445 12.91(2) ?
Sr2c Sr1 Sr2b 9_465 . 14_665 70.36(2) ?
Sr2c Sr1 Sr2b 9_465 . 15_565 66.04(3) ?
Sr2c Sr1 Sr2b 9_465 . 12_465 144.16(2) ?
Sr2c Sr1 N3ac 9_465 . 1_565 41.01(8) ?
Sr2c Sr1 N1a 9_465 . 1_565 106.3(2) ?
Sr2c Sr1 N3bc 9_465 . 7_565 97.06(13) ?
Sr2c Sr1 N2a 9_465 . 1_565 145.5(2) ?
Sr2c Sr1 N2a 9_465 . 2_555 85.35(16) ?
Sr2c Sr1 C2a 9_465 . 2_555 97.71(13) ?
Sr2c Sr1 C2a 9_465 . 3_675 128.5(2) ?
Sr2c Sr1 N3ab 9_465 . 13_555 53.90(9) ?
Sr2c Sr1 N1c 9_465 . 7_455 60.49(19) ?
Sr2c Sr1 N2c 9_465 . 9_565 93.8(2) ?
Sr2c Sr1 N2b 9_465 . 13_455 83.78(16) ?
Sr2c Sr1 N2b 9_465 . 14_555 134.2(2) ?
Sr2c Sr1 N1b 9_465 . 13_455 47.59(19) ?
Sr2c Sr1 C2b 9_465 . 13_455 100.37(12) ?
Sr2c Sr1 C2b 9_465 . 15_665 138.67(15) ?
Sr2c Sr1 Sr2b 5_555 . 13_445 134.71(3) ?
Sr2c Sr1 Sr2b 5_555 . 14_665 141.59(4) ?
Sr2c Sr1 Sr2b 5_555 . 15_565 149.12(4) ?
Sr2c Sr1 Sr2b 5_555 . 12_465 12.576(17) ?
Sr2c Sr1 N3ac 5_555 . 1_565 122.90(14) ?
Sr2c Sr1 N1a 5_555 . 1_565 118.4(2) ?
Sr2c Sr1 N3bc 5_555 . 7_565 127.64(13) ?
Sr2c Sr1 N2a 5_555 . 1_565 53.1(2) ?
Sr2c Sr1 N2a 5_555 . 2_555 51.32(16) ?
Sr2c Sr1 C2a 5_555 . 2_555 37.70(14) ?
Sr2c Sr1 C2a 5_555 . 3_675 46.76(16) ?
Sr2c Sr1 N3ab 5_555 . 13_555 121.50(14) ?
Sr2c Sr1 N1c 5_555 . 7_455 111.9(3) ?
Sr2c Sr1 N2c 5_555 . 9_565 41.61(19) ?
Sr2c Sr1 N2b 5_555 . 13_455 51.29(16) ?
Sr2c Sr1 N2b 5_555 . 14_555 53.3(2) ?
Sr2c Sr1 N1b 5_555 . 13_455 113.2(3) ?
Sr2c Sr1 C2b 5_555 . 13_455 37.25(13) ?
Sr2c Sr1 C2b 5_555 . 15_665 46.89(19) ?
Sr2b Sr1 Sr2b 13_445 . 14_665 77.13(2) ?
Sr2b Sr1 Sr2b 13_445 . 15_565 59.57(2) ?
Sr2b Sr1 Sr2b 13_445 . 12_465 146.26(3) ?
Sr2b Sr1 N3ac 13_445 . 1_565 53.85(9) ?
Sr2b Sr1 N1a 13_445 . 1_565 106.2(2) ?
Sr2b Sr1 N3bc 13_445 . 7_565 97.03(13) ?
Sr2b Sr1 N2a 13_445 . 1_565 132.7(2) ?
Sr2b Sr1 N2a 13_445 . 2_555 83.40(17) ?
Sr2b Sr1 C2a 13_445 . 2_555 99.94(15) ?
Sr2b Sr1 C2a 13_445 . 3_675 140.3(2) ?
Sr2b Sr1 N3ab 13_445 . 13_555 41.07(8) ?
Sr2b Sr1 N1c 13_445 . 7_455 47.60(19) ?
Sr2b Sr1 N2c 13_445 . 9_565 93.47(19) ?
Sr2b Sr1 N2b 13_445 . 13_455 85.32(15) ?
Sr2b Sr1 N2b 13_445 . 14_555 147.0(2) ?
Sr2b Sr1 N1b 13_445 . 13_455 60.46(19) ?
Sr2b Sr1 C2b 13_445 . 13_455 97.70(13) ?
Sr2b Sr1 C2b 13_445 . 15_665 126.67(15) ?
Sr2b Sr1 Sr2b 14_665 . 15_565 57.96(3) ?
Sr2b Sr1 Sr2b 14_665 . 12_465 129.70(4) ?
Sr2b Sr1 N3ac 14_665 . 1_565 51.90(8) ?
Sr2b Sr1 N1a 14_665 . 1_565 45.45(18) ?
Sr2b Sr1 N3bc 14_665 . 7_565 39.30(8) ?
Sr2b Sr1 N2a 14_665 . 1_565 126.91(15) ?
Sr2b Sr1 N2a 14_665 . 2_555 148.32(18) ?
Sr2b Sr1 C2a 14_665 . 2_555 138.7(2) ?
Sr2b Sr1 C2a 14_665 . 3_675 95.64(15) ?
Sr2b Sr1 N3ab 14_665 . 13_555 96.58(13) ?
Sr2b Sr1 N1c 14_665 . 7_455 106.1(3) ?
Sr2b Sr1 N2c 14_665 . 9_565 147.5(3) ?
Sr2b Sr1 N2b 14_665 . 13_455 136.0(2) ?
Sr2b Sr1 N2b 14_665 . 14_555 88.3(2) ?
Sr2b Sr1 N1b 14_665 . 13_455 58.12(18) ?
Sr2b Sr1 C2b 14_665 . 13_455 159.36(18) ?
Sr2b Sr1 C2b 14_665 . 15_665 139.03(13) ?
Sr2b Sr1 Sr2b 15_565 . 12_465 147.94(3) ?
Sr2b Sr1 N3ac 15_565 . 1_565 87.90(13) ?
Sr2b Sr1 N1a 15_565 . 1_565 52.4(2) ?
Sr2b Sr1 N3bc 15_565 . 7_565 45.04(10) ?
Sr2b Sr1 N2a 15_565 . 1_565 96.4(2) ?
Sr2b Sr1 N2a 15_565 . 2_555 130.0(2) ?
Sr2b Sr1 C2a 15_565 . 2_555 153.5(2) ?
Sr2b Sr1 C2a 15_565 . 3_675 146.32(13) ?
Sr2b Sr1 N3ab 15_565 . 13_555 45.66(10) ?
Sr2b Sr1 N1c 15_565 . 7_455 53.2(2) ?
Sr2b Sr1 N2c 15_565 . 9_565 141.8(2) ?
Sr2b Sr1 N2b 15_565 . 13_455 140.20(17) ?
Sr2b Sr1 N2b 15_565 . 14_555 134.60(18) ?
Sr2b Sr1 N1b 15_565 . 13_455 97.6(3) ?
Sr2b Sr1 C2b 15_565 . 13_455 136.35(19) ?
Sr2b Sr1 C2b 15_565 . 15_665 102.24(19) ?
Sr2b Sr1 N3ac 12_465 . 1_565 121.97(13) ?
Sr2b Sr1 N1a 12_465 . 1_565 107.5(2) ?
Sr2b Sr1 N3bc 12_465 . 7_565 116.71(13) ?
Sr2b Sr1 N2a 12_465 . 1_565 52.8(2) ?
Sr2b Sr1 N2a 12_465 . 2_555 63.20(17) ?
Sr2b Sr1 C2a 12_465 . 2_555 46.85(14) ?
Sr2b Sr1 C2a 12_465 . 3_675 37.12(18) ?
Sr2b Sr1 N3ab 12_465 . 13_555 132.15(14) ?
Sr2b Sr1 N1c 12_465 . 7_455 122.5(3) ?
Sr2b Sr1 N2c 12_465 . 9_565 52.80(19) ?
Sr2b Sr1 N2b 12_465 . 13_455 61.25(15) ?
Sr2b Sr1 N2b 12_465 . 14_555 41.8(2) ?
Sr2b Sr1 N1b 12_465 . 13_455 112.3(3) ?
Sr2b Sr1 C2b 12_465 . 13_455 49.59(14) ?
Sr2b Sr1 C2b 12_465 . 15_665 49.76(19) ?
N3ac Sr1 N1a 1_565 . 1_565 97.31(19) ?
N3ac Sr1 N3bc 1_565 . 7_565 90.95(13) ?
N3ac Sr1 N2a 1_565 . 1_565 173.5(2) ?
N3ac Sr1 N2a 1_565 . 2_555 96.4(2) ?
N3ac Sr1 C2a 1_565 . 2_555 92.7(2) ?
N3ac Sr1 C2a 1_565 . 3_675 90.8(2) ?
N3ac Sr1 N3ab 1_565 . 13_555 94.26(14) ?
N3ac Sr1 N1c 1_565 . 7_455 101.4(2) ?
N3ac Sr1 N2c 1_565 . 9_565 97.4(3) ?
N3ac Sr1 N2b 1_565 . 13_455 85.2(2) ?
N3ac Sr1 N2b 1_565 . 14_555 93.9(3) ?
N3ac Sr1 N1b 1_565 . 13_455 9.7(3) ?
N3ac Sr1 C2b 1_565 . 13_455 108.87(18) ?
N3ac Sr1 C2b 1_565 . 15_665 168.2(2) ?
N1a Sr1 N3bc 1_565 . 7_565 9.3(3) ?
N1a Sr1 N2a 1_565 . 1_565 81.6(2) ?
N1a Sr1 N2a 1_565 . 2_555 166.2(3) ?
N1a Sr1 C2a 1_565 . 2_555 153.0(3) ?
N1a Sr1 C2a 1_565 . 3_675 94.5(2) ?
N1a Sr1 N3ab 1_565 . 13_555 96.31(18) ?
N1a Sr1 N1c 1_565 . 7_455 101.6(2) ?
N1a Sr1 N2c 1_565 . 9_565 160.0(3) ?
N1a Sr1 N2b 1_565 . 13_455 167.4(3) ?
N1a Sr1 N2b 1_565 . 14_555 82.5(3) ?
N1a Sr1 N1b 1_565 . 13_455 102.8(2) ?
N1a Sr1 C2b 1_565 . 13_455 151.8(3) ?
N1a Sr1 C2b 1_565 . 15_665 93.6(2) ?
N3bc Sr1 N2a 7_565 . 1_565 88.69(18) ?
N3bc Sr1 N2a 7_565 . 2_555 171.1(2) ?
N3bc Sr1 C2a 7_565 . 2_555 161.3(2) ?
N3bc Sr1 C2a 7_565 . 3_675 101.38(16) ?
N3bc Sr1 N3ab 7_565 . 13_555 90.12(12) ?
N3bc Sr1 N1c 7_565 . 7_455 96.38(18) ?
N3bc Sr1 N2c 7_565 . 9_565 169.2(2) ?
N3bc Sr1 N2b 7_565 . 13_455 173.1(2) ?
N3bc Sr1 N2b 7_565 . 14_555 89.6(2) ?
N3bc Sr1 N1b 7_565 . 13_455 97.41(19) ?
N3bc Sr1 C2b 7_565 . 13_455 159.84(18) ?
N3bc Sr1 C2b 7_565 . 15_665 100.41(17) ?
N2a Sr1 N2a 1_565 . 2_555 84.6(2) ?
N2a Sr1 C2a 1_565 . 2_555 85.6(2) ?
N2a Sr1 C2a 1_565 . 3_675 82.9(3) ?
N2a Sr1 N3ab 1_565 . 13_555 92.3(2) ?
N2a Sr1 N1c 1_565 . 7_455 85.1(3) ?
N2a Sr1 N2c 1_565 . 9_565 82.2(3) ?
N2a Sr1 N2b 1_565 . 13_455 94.5(2) ?
N2a Sr1 N2b 1_565 . 14_555 79.5(3) ?
N2a Sr1 N1b 1_565 . 13_455 164.9(3) ?
N2a Sr1 C2b 1_565 . 13_455 71.2(2) ?
N2a Sr1 C2b 1_565 . 15_665 12.22(19) ?
N2a Sr1 C2a 2_555 . 2_555 23.6(3) ?
N2a Sr1 C2a 2_555 . 3_675 83.6(2) ?
N2a Sr1 N3ab 2_555 . 13_555 84.4(2) ?
N2a Sr1 N1c 2_555 . 7_455 77.3(3) ?
N2a Sr1 N2c 2_555 . 9_565 11.9(3) ?
N2a Sr1 N2b 2_555 . 13_455 15.5(3) ?
N2a Sr1 N2b 2_555 . 14_555 94.9(3) ?
N2a Sr1 N1b 2_555 . 13_455 90.6(3) ?
N2a Sr1 C2b 2_555 . 13_455 15.1(2) ?
N2a Sr1 C2b 2_555 . 15_665 72.6(2) ?
C2a Sr1 C2a 2_555 . 3_675 60.2(2) ?
C2a Sr1 N3ab 2_555 . 13_555 107.9(2) ?
C2a Sr1 N1c 2_555 . 7_455 100.9(3) ?
C2a Sr1 N2c 2_555 . 9_565 12.4(4) ?
C2a Sr1 N2b 2_555 . 13_455 14.7(2) ?
C2a Sr1 N2b 2_555 . 14_555 71.9(3) ?
C2a Sr1 N1b 2_555 . 13_455 84.2(3) ?
C2a Sr1 C2b 2_555 . 13_455 21.6(3) ?
C2a Sr1 C2b 2_555 . 15_665 75.6(3) ?
C2a Sr1 N3ab 3_675 . 13_555 167.38(18) ?
C2a Sr1 N1c 3_675 . 7_455 158.3(3) ?
C2a Sr1 N2c 3_675 . 9_565 71.7(3) ?
C2a Sr1 N2b 3_675 . 13_455 73.0(2) ?
C2a Sr1 N2b 3_675 . 14_555 12.2(2) ?
C2a Sr1 N1b 3_675 . 13_455 82.4(3) ?
C2a Sr1 C2b 3_675 . 13_455 75.4(2) ?
C2a Sr1 C2b 3_675 . 15_665 84.1(3) ?
N3ab Sr1 N1c 13_555 . 7_455 9.6(3) ?
N3ab Sr1 N2c 13_555 . 9_565 96.1(3) ?
N3ab Sr1 N2b 13_555 . 13_455 95.83(19) ?
N3ab Sr1 N2b 13_555 . 14_555 171.8(3) ?
N3ab Sr1 N1b 13_555 . 13_455 101.5(2) ?
N3ab Sr1 C2b 13_555 . 13_455 92.0(2) ?
N3ab Sr1 C2b 13_555 . 15_665 88.8(2) ?
N1c Sr1 N2c 7_455 . 9_565 88.8(3) ?
N1c Sr1 N2b 7_455 . 13_455 90.0(2) ?
N1c Sr1 N2b 7_455 . 14_555 163.4(3) ?
N1c Sr1 N1b 7_455 . 13_455 107.8(2) ?
N1c Sr1 C2b 7_455 . 13_455 83.6(3) ?
N1c Sr1 C2b 7_455 . 15_665 80.5(3) ?
N2c Sr1 N2b 9_565 . 13_455 12.2(3) ?
N2c Sr1 N2b 9_565 . 14_555 83.0(3) ?
N2c Sr1 N1b 9_565 . 13_455 90.0(4) ?
N2c Sr1 C2b 9_565 . 13_455 11.9(4) ?
N2c Sr1 C2b 9_565 . 15_665 71.0(3) ?
N2b Sr1 N2b 13_455 . 14_555 85.0(2) ?
N2b Sr1 N1b 13_455 . 13_455 78.1(3) ?
N2b Sr1 C2b 13_455 . 13_455 23.7(2) ?
N2b Sr1 C2b 13_455 . 15_665 83.2(2) ?
N2b Sr1 N1b 14_555 . 13_455 86.7(3) ?
N2b Sr1 C2b 14_555 . 13_455 85.5(3) ?
N2b Sr1 C2b 14_555 . 15_665 83.2(3) ?
N1b Sr1 C2b 13_455 . 13_455 101.8(3) ?
N1b Sr1 C2b 13_455 . 15_665 159.4(3) ?
C2b Sr1 C2b 13_455 . 15_665 59.6(2) ?
Sr1 Sr2a Sr1 . . 2_775 64.90(2) ?
Sr1 Sr2a Sr1 . . 3_565 64.09(3) ?
Sr1 Sr2a Sr1 . . 10_664 133.31(3) ?
Sr1 Sr2a Sr2a . . 2_665 52.56(2) ?
Sr1 Sr2a Sr2a . . 2_765 131.29(3) ?
Sr1 Sr2a Sr2a . . 3_565 86.84(2) ?
Sr1 Sr2a Sr2a . . 3_675 116.25(2) ?
Sr1 Sr2a Fe1a . . 10_565 84.80(3) ?
Sr1 Sr2a Sr2c . . 7_445 94.73(2) ?
Sr1 Sr2a Sr2c . . 7_455 51.74(2) ?
Sr1 Sr2a Sr2c . . 7_555 122.46(2) ?
Sr1 Sr2a Sr2c . . 8_665 85.68(8) ?
Sr1 Sr2a Sr2c . . 9_565 128.31(3) ?
Sr1 Sr2a Sr2b . . 13_445 57.535(18) ?
Sr1 Sr2a Sr2b . . 13_545 128.26(3) ?
Sr1 Sr2a Sr2b . . 13_555 85.27(2) ?
Sr1 Sr2a Sr2b . . 14_655 94.84(3) ?
Sr1 Sr2a Sr2b . . 15_565 51.95(7) ?
Sr1 Sr2a N3ac . . 1_665 97.29(14) ?
Sr1 Sr2a N2a . . 10_564 147.49(15) ?
Sr1 Sr2a C2a . . 10_564 139.71(12) ?
Sr1 Sr2a C2a . . 12_454 85.31(16) ?
Sr1 Sr2a Fe1c . . 16_555 91.30(3) ?
Sr1 Sr2a Fe1b . . 4_665 156.08(4) ?
Sr1 Sr2a N3ab . . 13_555 43.39(9) ?
Sr1 Sr2a N1c . . 7_455 38.78(9) ?
Sr1 Sr2a N1b . . 13_555 88.88(18) ?
Sr1 Sr2a C2c . . 16_565 86.52(16) ?
Sr1 Sr2a C2c . . 17_655 133.6(2) ?
Sr1 Sr2a C2b . . 4_675 133.49(18) ?
Sr1 Sr2a C2b . . 6_555 158.02(16) ?
Sr1 Sr2a C1a . . 10_565 55.32(17) ?
Sr1 Sr2a C1c . . 16_555 53.5(2) ?
Sr1 Sr2a C1b . . 4_665 112.0(3) ?
Sr1 Sr2a Sr1 2_775 . 3_565 62.81(2) ?
Sr1 Sr2a Sr1 2_775 . 10_664 131.49(2) ?
Sr1 Sr2a Sr2a 2_775 . 2_665 116.39(3) ?
Sr1 Sr2a Sr2a 2_775 . 2_765 86.39(3) ?
Sr1 Sr2a Sr2a 2_775 . 3_565 130.71(3) ?
Sr1 Sr2a Sr2a 2_775 . 3_675 52.70(2) ?
Sr1 Sr2a Fe1a 2_775 . 10_565 85.31(3) ?
Sr1 Sr2a Sr2c 2_775 . 7_445 127.65(3) ?
Sr1 Sr2a Sr2c 2_775 . 7_455 85.73(3) ?
Sr1 Sr2a Sr2c 2_775 . 7_555 57.57(2) ?
Sr1 Sr2a Sr2c 2_775 . 8_665 52.15(7) ?
Sr1 Sr2a Sr2c 2_775 . 9_565 94.16(3) ?
Sr1 Sr2a Sr2b 2_775 . 13_445 122.43(3) ?
Sr1 Sr2a Sr2b 2_775 . 13_545 94.27(3) ?
Sr1 Sr2a Sr2b 2_775 . 13_555 52.35(2) ?
Sr1 Sr2a Sr2b 2_775 . 14_655 127.59(3) ?
Sr1 Sr2a Sr2b 2_775 . 15_565 85.32(7) ?
Sr1 Sr2a N3ac 2_775 . 1_665 42.99(9) ?
Sr1 Sr2a N2a 2_775 . 10_564 147.46(16) ?
Sr1 Sr2a C2a 2_775 . 10_564 139.61(16) ?
Sr1 Sr2a C2a 2_775 . 12_454 116.33(18) ?
Sr1 Sr2a Fe1c 2_775 . 16_555 156.17(4) ?
Sr1 Sr2a Fe1b 2_775 . 4_665 91.18(4) ?
Sr1 Sr2a N3ab 2_775 . 13_555 96.85(14) ?
Sr1 Sr2a N1c 2_775 . 7_455 88.41(19) ?
Sr1 Sr2a N1b 2_775 . 13_555 38.28(9) ?
Sr1 Sr2a C2c 2_775 . 16_565 134.03(17) ?
Sr1 Sr2a C2c 2_775 . 17_655 157.5(3) ?
Sr1 Sr2a C2b 2_775 . 4_675 87.11(13) ?
Sr1 Sr2a C2b 2_775 . 6_555 132.84(17) ?
Sr1 Sr2a C1a 2_775 . 10_565 55.73(17) ?
Sr1 Sr2a C1c 2_775 . 16_555 111.7(3) ?
Sr1 Sr2a C1b 2_775 . 4_665 53.2(2) ?
Sr1 Sr2a Sr1 3_565 . 10_664 158.81(4) ?
Sr1 Sr2a Sr2a 3_565 . 2_665 96.35(3) ?
Sr1 Sr2a Sr2a 3_565 . 2_765 67.93(3) ?
Sr1 Sr2a Sr2a 3_565 . 3_565 68.71(2) ?
Sr1 Sr2a Sr2a 3_565 . 3_675 95.27(3) ?
Sr1 Sr2a Fe1a 3_565 . 10_565 142.15(4) ?
Sr1 Sr2a Sr2c 3_565 . 7_445 64.91(2) ?
Sr1 Sr2a Sr2c 3_565 . 7_455 115.72(3) ?
Sr1 Sr2a Sr2c 3_565 . 7_555 89.43(3) ?
Sr1 Sr2a Sr2c 3_565 . 8_665 114.92(7) ?
Sr1 Sr2a Sr2c 3_565 . 9_565 64.33(3) ?
Sr1 Sr2a Sr2b 3_565 . 13_445 90.57(3) ?
Sr1 Sr2a Sr2b 3_565 . 13_545 64.28(3) ?
Sr1 Sr2a Sr2b 3_565 . 13_555 115.09(2) ?
Sr1 Sr2a Sr2b 3_565 . 14_655 64.86(2) ?
Sr1 Sr2a Sr2b 3_565 . 15_565 115.88(8) ?
Sr1 Sr2a N3ac 3_565 . 1_665 52.20(12) ?
Sr1 Sr2a N2a 3_565 . 10_564 119.6(2) ?
Sr1 Sr2a C2a 3_565 . 10_564 96.57(14) ?
Sr1 Sr2a C2a 3_565 . 12_454 147.08(14) ?
Sr1 Sr2a Fe1c 3_565 . 16_555 107.00(4) ?
Sr1 Sr2a Fe1b 3_565 . 4_665 105.95(5) ?
Sr1 Sr2a N3ab 3_565 . 13_555 53.19(12) ?
Sr1 Sr2a N1c 3_565 . 7_455 46.43(14) ?
Sr1 Sr2a N1b 3_565 . 13_555 45.46(14) ?
Sr1 Sr2a C2c 3_565 . 16_565 136.30(13) ?
Sr1 Sr2a C2c 3_565 . 17_655 110.1(2) ?
Sr1 Sr2a C2b 3_565 . 4_675 135.43(17) ?
Sr1 Sr2a C2b 3_565 . 6_555 109.3(2) ?
Sr1 Sr2a C1a 3_565 . 10_565 105.9(2) ?
Sr1 Sr2a C1c 3_565 . 16_555 65.8(2) ?
Sr1 Sr2a C1b 3_565 . 4_665 64.8(2) ?
Sr1 Sr2a Sr2a 10_664 . 2_665 89.84(3) ?
Sr1 Sr2a Sr2a 10_664 . 2_765 95.32(3) ?
Sr1 Sr2a Sr2a 10_664 . 3_565 97.50(2) ?
Sr1 Sr2a Sr2a 10_664 . 3_675 86.66(2) ?
Sr1 Sr2a Fe1a 10_664 . 10_565 58.94(3) ?
Sr1 Sr2a Sr2c 10_664 . 7_445 98.26(2) ?
Sr1 Sr2a Sr2c 10_664 . 7_455 83.37(3) ?
Sr1 Sr2a Sr2c 10_664 . 7_555 88.38(2) ?
Sr1 Sr2a Sr2c 10_664 . 8_665 81.77(7) ?
Sr1 Sr2a Sr2c 10_664 . 9_565 96.62(3) ?
Sr1 Sr2a Sr2b 10_664 . 13_445 91.62(2) ?
Sr1 Sr2a Sr2b 10_664 . 13_545 96.63(3) ?
Sr1 Sr2a Sr2b 10_664 . 13_555 81.736(19) ?
Sr1 Sr2a Sr2b 10_664 . 14_655 98.27(2) ?
Sr1 Sr2a Sr2b 10_664 . 15_565 83.31(7) ?
Sr1 Sr2a N3ac 10_664 . 1_665 123.92(14) ?
Sr1 Sr2a N2a 10_664 . 10_564 39.3(2) ?
Sr1 Sr2a C2a 10_664 . 10_564 62.36(14) ?
Sr1 Sr2a C2a 10_664 . 12_454 48.05(16) ?
Sr1 Sr2a Fe1c 10_664 . 16_555 65.59(4) ?
Sr1 Sr2a Fe1b 10_664 . 4_665 62.70(4) ?
Sr1 Sr2a N3ab 10_664 . 13_555 127.21(14) ?
Sr1 Sr2a N1c 10_664 . 7_455 135.70(19) ?
Sr1 Sr2a N1b 10_664 . 13_555 132.37(19) ?
Sr1 Sr2a C2c 10_664 . 16_565 49.70(15) ?
Sr1 Sr2a C2c 10_664 . 17_655 50.17(19) ?
Sr1 Sr2a C2b 10_664 . 4_675 46.44(13) ?
Sr1 Sr2a C2b 10_664 . 6_555 49.8(2) ?
Sr1 Sr2a C1a 10_664 . 10_565 95.2(2) ?
Sr1 Sr2a C1c 10_664 . 16_555 112.2(3) ?
Sr1 Sr2a C1b 10_664 . 4_665 109.0(3) ?
Sr2a Sr2a Sr2a 2_665 . 2_765 143.58(3) ?
Sr2a Sr2a Sr2a 2_665 . 3_565 60.00(3) ?
Sr2a Sr2a Sr2a 2_665 . 3_675 156.42(3) ?
Sr2a Sr2a Fe1a 2_665 . 10_565 79.26(3) ?
Sr2a Sr2a Sr2c 2_665 . 7_445 71.75(2) ?
Sr2a Sr2a Sr2c 2_665 . 7_455 48.25(2) ?
Sr2a Sr2a Sr2c 2_665 . 7_555 168.25(3) ?
Sr2a Sr2a Sr2c 2_665 . 8_665 108.87(9) ?
Sr2a Sr2a Sr2c 2_665 . 9_565 131.91(3) ?
Sr2a Sr2a Sr2b 2_665 . 13_445 11.75(2) ?
Sr2a Sr2a Sr2b 2_665 . 13_545 131.75(3) ?
Sr2a Sr2a Sr2b 2_665 . 13_555 108.25(3) ?
Sr2a Sr2a Sr2b 2_665 . 14_655 71.91(3) ?
Sr2a Sr2a Sr2b 2_665 . 15_565 48.87(6) ?
Sr2a Sr2a N3ac 2_665 . 1_665 146.24(14) ?
Sr2a Sr2a N2a 2_665 . 10_564 95.98(16) ?
Sr2a Sr2a C2a 2_665 . 10_564 99.27(15) ?
Sr2a Sr2a C2a 2_665 . 12_454 52.95(12) ?
Sr2a Sr2a Fe1c 2_665 . 16_555 40.70(3) ?
Sr2a Sr2a Fe1b 2_665 . 4_665 150.56(4) ?
Sr2a Sr2a N3ab 2_665 . 13_555 43.66(10) ?
Sr2a Sr2a N1c 2_665 . 7_455 49.91(14) ?
Sr2a Sr2a N1b 2_665 . 13_555 137.77(19) ?
Sr2a Sr2a C2c 2_665 . 16_565 40.86(13) ?
Sr2a Sr2a C2c 2_665 . 17_655 84.9(3) ?
Sr2a Sr2a C2b 2_665 . 4_675 127.37(18) ?
Sr2a Sr2a C2b 2_665 . 6_555 110.62(16) ?
Sr2a Sr2a C1a 2_665 . 10_565 78.70(3) ?
Sr2a Sr2a C1c 2_665 . 16_555 34.63(14) ?
Sr2a Sr2a C1b 2_665 . 4_665 160.8(3) ?
Sr2a Sr2a Sr2a 2_765 . 3_565 83.58(3) ?
Sr2a Sr2a Sr2a 2_765 . 3_675 60.00(2) ?
Sr2a Sr2a Fe1a 2_765 . 10_565 133.42(2) ?
Sr2a Sr2a Sr2c 2_765 . 7_445 71.84(2) ?
Sr2a Sr2a Sr2c 2_765 . 7_455 168.16(2) ?
Sr2a Sr2a Sr2c 2_765 . 7_555 48.16(2) ?
Sr2a Sr2a Sr2c 2_765 . 8_665 107.55(9) ?
Sr2a Sr2a Sr2c 2_765 . 9_565 11.668(17) ?
Sr2a Sr2a Sr2b 2_765 . 13_445 131.84(3) ?
Sr2a Sr2a Sr2b 2_765 . 13_545 11.836(14) ?
Sr2a Sr2a Sr2b 2_765 . 13_555 108.16(2) ?
Sr2a Sr2a Sr2b 2_765 . 14_655 71.67(3) ?
Sr2a Sr2a Sr2b 2_765 . 15_565 167.55(6) ?
Sr2a Sr2a N3ac 2_765 . 1_665 43.57(10) ?
Sr2a Sr2a N2a 2_765 . 10_564 67.6(2) ?
Sr2a Sr2a C2a 2_765 . 10_564 53.23(16) ?
Sr2a Sr2a C2a 2_765 . 12_454 143.37(16) ?
Sr2a Sr2a Fe1c 2_765 . 16_555 110.50(3) ?
Sr2a Sr2a Fe1b 2_765 . 4_665 40.63(3) ?
Sr2a Sr2a N3ab 2_765 . 13_555 109.52(4) ?
Sr2a Sr2a N1c 2_765 . 7_455 107.30(6) ?
Sr2a Sr2a N1b 2_765 . 13_555 49.81(14) ?
Sr2a Sr2a C2c 2_765 . 16_565 137.08(17) ?
Sr2a Sr2a C2c 2_765 . 17_655 71.4(3) ?
Sr2a Sr2a C2b 2_765 . 4_675 78.7(2) ?
Sr2a Sr2a C2b 2_765 . 6_555 51.5(2) ?
Sr2a Sr2a C1a 2_765 . 10_565 136.25(6) ?
Sr2a Sr2a C1c 2_765 . 16_555 112.34(5) ?
Sr2a Sr2a C1b 2_765 . 4_665 34.59(13) ?
Sr2a Sr2a Sr2a 3_565 . 3_675 143.58(4) ?
Sr2a Sr2a Fe1a 3_565 . 10_565 133.69(3) ?
Sr2a Sr2a Sr2c 3_565 . 7_445 11.75(2) ?
Sr2a Sr2a Sr2c 3_565 . 7_455 108.25(3) ?
Sr2a Sr2a Sr2c 3_565 . 7_555 131.75(3) ?
Sr2a Sr2a Sr2c 3_565 . 8_665 168.87(10) ?
Sr2a Sr2a Sr2c 3_565 . 9_565 71.91(3) ?
Sr2a Sr2a Sr2b 3_565 . 13_445 48.25(2) ?
Sr2a Sr2a Sr2b 3_565 . 13_545 71.75(2) ?
Sr2a Sr2a Sr2b 3_565 . 13_555 168.25(3) ?
Sr2a Sr2a Sr2b 3_565 . 14_655 11.91(3) ?
Sr2a Sr2a Sr2b 3_565 . 15_565 108.87(6) ?
Sr2a Sr2a N3ac 3_565 . 1_665 109.55(5) ?
Sr2a Sr2a N2a 3_565 . 10_564 67.62(14) ?
Sr2a Sr2a C2a 3_565 . 10_564 52.87(12) ?
Sr2a Sr2a C2a 3_565 . 12_454 99.33(15) ?
Sr2a Sr2a Fe1c 3_565 . 16_555 40.70(3) ?
Sr2a Sr2a Fe1b 3_565 . 4_665 110.52(3) ?
Sr2a Sr2a N3ab 3_565 . 13_555 43.66(10) ?
Sr2a Sr2a N1c 3_565 . 7_455 49.91(14) ?
Sr2a Sr2a N1b 3_565 . 13_555 107.34(6) ?
Sr2a Sr2a C2c 3_565 . 16_565 78.60(13) ?
Sr2a Sr2a C2c 3_565 . 17_655 52.20(16) ?
Sr2a Sr2a C2b 3_565 . 4_675 136.96(14) ?
Sr2a Sr2a C2b 3_565 . 6_555 71.48(18) ?
Sr2a Sr2a C1a 3_565 . 10_565 136.53(7) ?
Sr2a Sr2a C1c 3_565 . 16_555 34.63(14) ?
Sr2a Sr2a C1b 3_565 . 4_665 112.35(5) ?
Sr2a Sr2a Fe1a 3_675 . 10_565 78.97(2) ?
Sr2a Sr2a Sr2c 3_675 . 7_445 131.84(3) ?
Sr2a Sr2a Sr2c 3_675 . 7_455 108.16(2) ?
Sr2a Sr2a Sr2c 3_675 . 7_555 11.84(2) ?
Sr2a Sr2a Sr2c 3_675 . 8_665 47.55(8) ?
Sr2a Sr2a Sr2c 3_675 . 9_565 71.67(3) ?
Sr2a Sr2a Sr2b 3_675 . 13_445 168.16(3) ?
Sr2a Sr2a Sr2b 3_675 . 13_545 71.84(2) ?
Sr2a Sr2a Sr2b 3_675 . 13_555 48.16(2) ?
Sr2a Sr2a Sr2b 3_675 . 14_655 131.67(4) ?
Sr2a Sr2a Sr2b 3_675 . 15_565 107.55(6) ?
Sr2a Sr2a N3ac 3_675 . 1_665 43.57(10) ?
Sr2a Sr2a N2a 3_675 . 10_564 96.00(14) ?
Sr2a Sr2a C2a 3_675 . 10_564 99.69(14) ?
Sr2a Sr2a C2a 3_675 . 12_454 109.76(13) ?
Sr2a Sr2a Fe1c 3_675 . 16_555 150.45(4) ?
Sr2a Sr2a Fe1b 3_675 . 4_665 40.63(3) ?
Sr2a Sr2a N3ab 3_675 . 13_555 146.12(14) ?
Sr2a Sr2a N1c 3_675 . 7_455 137.64(19) ?
Sr2a Sr2a N1b 3_675 . 13_555 49.81(14) ?
Sr2a Sr2a C2c 3_675 . 16_565 127.57(12) ?
Sr2a Sr2a C2c 3_675 . 17_655 110.1(2) ?
Sr2a Sr2a C2b 3_675 . 4_675 41.09(15) ?
Sr2a Sr2a C2b 3_675 . 6_555 84.57(15) ?
Sr2a Sr2a C1a 3_675 . 10_565 78.41(2) ?
Sr2a Sr2a C1c 3_675 . 16_555 160.8(3) ?
Sr2a Sr2a C1b 3_675 . 4_665 34.59(13) ?
Fe1a Sr2a Sr2c 10_565 . 7_445 143.25(3) ?
Fe1a Sr2a Sr2c 10_565 . 7_455 36.92(2) ?
Fe1a Sr2a Sr2c 10_565 . 7_555 89.900(18) ?
Fe1a Sr2a Sr2c 10_565 . 8_665 37.23(7) ?
Fe1a Sr2a Sr2c 10_565 . 9_565 142.95(3) ?
Fe1a Sr2a Sr2b 10_565 . 13_445 90.10(2) ?
Fe1a Sr2a Sr2b 10_565 . 13_545 143.08(3) ?
Fe1a Sr2a Sr2b 10_565 . 13_555 36.75(2) ?
Fe1a Sr2a Sr2b 10_565 . 14_655 143.38(3) ?
Fe1a Sr2a Sr2b 10_565 . 15_565 36.45(6) ?
Fe1a Sr2a N3ac 10_565 . 1_665 116.67(3) ?
Fe1a Sr2a N2a 10_565 . 10_564 98.2(2) ?
Fe1a Sr2a C2a 10_565 . 10_564 121.28(15) ?
Fe1a Sr2a C2a 10_565 . 12_454 34.62(16) ?
Fe1a Sr2a Fe1c 10_565 . 16_555 94.03(3) ?
Fe1a Sr2a Fe1b 10_565 . 4_665 93.84(3) ?
Fe1a Sr2a N3ab 10_565 . 13_555 116.95(4) ?
Fe1a Sr2a N1c 10_565 . 7_455 118.16(4) ?
Fe1a Sr2a N1b 10_565 . 13_555 117.92(3) ?
Fe1a Sr2a C2c 10_565 . 16_565 55.49(13) ?
Fe1a Sr2a C2c 10_565 . 17_655 107.0(2) ?
Fe1a Sr2a C2b 10_565 . 4_675 55.1(2) ?
Fe1a Sr2a C2b 10_565 . 6_555 107.3(2) ?
Fe1a Sr2a C1a 10_565 . 10_565 36.3(2) ?
Fe1a Sr2a C1c 10_565 . 16_555 113.31(9) ?
Fe1a Sr2a C1b 10_565 . 4_665 113.01(9) ?
Sr2c Sr2a Sr2c 7_445 . 7_455 120.00(2) ?
Sr2c Sr2a Sr2c 7_445 . 7_555 120.00(3) ?
Sr2c Sr2a Sr2c 7_445 . 8_665 179.39(9) ?
Sr2c Sr2a Sr2c 7_445 . 9_565 60.17(2) ?
Sr2c Sr2a Sr2b 7_445 . 13_445 60.000(19) ?
Sr2c Sr2a Sr2b 7_445 . 13_545 60.000(19) ?
Sr2c Sr2a Sr2b 7_445 . 13_555 180 ?
Sr2c Sr2a Sr2b 7_445 . 14_655 0.17(2) ?
Sr2c Sr2a Sr2b 7_445 . 15_565 120.61(6) ?
Sr2c Sr2a N3ac 7_445 . 1_665 99.88(3) ?
Sr2c Sr2a N2a 7_445 . 10_564 63.77(16) ?
Sr2c Sr2a C2a 7_445 . 10_564 45.59(12) ?
Sr2c Sr2a C2a 7_445 . 12_454 108.63(16) ?
Sr2c Sr2a Fe1c 7_445 . 16_555 49.22(2) ?
Sr2c Sr2a Fe1b 7_445 . 4_665 100.36(3) ?
Sr2c Sr2a N3ab 7_445 . 13_555 51.44(8) ?
Sr2c Sr2a N1c 7_445 . 7_455 56.30(11) ?
Sr2c Sr2a N1b 7_445 . 13_555 98.79(4) ?
Sr2c Sr2a C2c 7_445 . 16_565 87.77(14) ?
Sr2c Sr2a C2c 7_445 . 17_655 49.36(16) ?
Sr2c Sr2a C2b 7_445 . 4_675 131.21(16) ?
Sr2c Sr2a C2b 7_445 . 6_555 64.46(19) ?
Sr2c Sr2a C1a 7_445 . 10_565 147.35(9) ?
Sr2c Sr2a C1c 7_445 . 16_555 44.85(10) ?
Sr2c Sr2a C1b 7_445 . 4_665 101.24(4) ?
Sr2c Sr2a Sr2c 7_455 . 7_555 120.00(2) ?
Sr2c Sr2a Sr2c 7_455 . 8_665 60.61(8) ?
Sr2c Sr2a Sr2c 7_455 . 9_565 179.83(2) ?
Sr2c Sr2a Sr2b 7_455 . 13_445 60.000(19) ?
Sr2c Sr2a Sr2b 7_455 . 13_545 180 ?
Sr2c Sr2a Sr2b 7_455 . 13_555 60.000(19) ?
Sr2c Sr2a Sr2b 7_455 . 14_655 120.17(3) ?
Sr2c Sr2a Sr2b 7_455 . 15_565 0.61(5) ?
Sr2c Sr2a N3ac 7_455 . 1_665 128.56(8) ?
Sr2c Sr2a N2a 7_455 . 10_564 116.2(2) ?
Sr2c Sr2a C2a 7_455 . 10_564 134.16(16) ?
Sr2c Sr2a C2a 7_455 . 12_454 36.83(17) ?
Sr2c Sr2a Fe1c 7_455 . 16_555 79.74(2) ?
Sr2c Sr2a Fe1b 7_455 . 4_665 130.76(3) ?
Sr2c Sr2a N3ab 7_455 . 13_555 80.21(3) ?
Sr2c Sr2a N1c 7_455 . 7_455 81.29(3) ?
Sr2c Sr2a N1b 7_455 . 13_555 123.72(11) ?
Sr2c Sr2a C2c 7_455 . 16_565 48.77(17) ?
Sr2c Sr2a C2c 7_455 . 17_655 115.5(3) ?
Sr2c Sr2a C2b 7_455 . 4_675 92.1(2) ?
Sr2c Sr2a C2b 7_455 . 6_555 131.3(2) ?
Sr2c Sr2a C1a 7_455 . 10_565 32.85(9) ?
Sr2c Sr2a C1c 7_455 . 16_555 78.85(3) ?
Sr2c Sr2a C1b 7_455 . 4_665 135.09(10) ?
Sr2c Sr2a Sr2c 7_555 . 8_665 59.39(8) ?
Sr2c Sr2a Sr2c 7_555 . 9_565 59.83(2) ?
Sr2c Sr2a Sr2b 7_555 . 13_445 180 ?
Sr2c Sr2a Sr2b 7_555 . 13_545 60.000(19) ?
Sr2c Sr2a Sr2b 7_555 . 13_555 60.000(19) ?
Sr2c Sr2a Sr2b 7_555 . 14_655 119.83(3) ?
Sr2c Sr2a Sr2b 7_555 . 15_565 119.39(6) ?
Sr2c Sr2a N3ac 7_555 . 1_665 37.35(12) ?
Sr2c Sr2a N2a 7_555 . 10_564 89.99(15) ?
Sr2c Sr2a C2a 7_555 . 10_564 90.18(14) ?
Sr2c Sr2a C2a 7_555 . 12_454 118.75(12) ?
Sr2c Sr2a Fe1c 7_555 . 16_555 146.24(4) ?
Sr2c Sr2a Fe1b 7_555 . 4_665 33.62(3) ?
Sr2c Sr2a N3ab 7_555 . 13_555 142.50(13) ?
Sr2c Sr2a N1c 7_555 . 7_455 134.92(17) ?
Sr2c Sr2a N1b 7_555 . 13_555 44.93(17) ?
Sr2c Sr2a C2c 7_555 . 16_565 134.27(12) ?
Sr2c Sr2a C2c 7_555 . 17_655 102.7(3) ?
Sr2c Sr2a C2b 7_555 . 4_675 46.00(17) ?
Sr2c Sr2a C2b 7_555 . 6_555 76.78(15) ?
Sr2c Sr2a C1a 7_555 . 10_565 89.895(18) ?
Sr2c Sr2a C1c 7_555 . 16_555 154.5(2) ?
Sr2c Sr2a C1b 7_555 . 4_665 25.42(19) ?
Sr2c Sr2a Sr2c 8_665 . 9_565 119.22(9) ?
Sr2c Sr2a Sr2b 8_665 . 13_445 120.61(9) ?
Sr2c Sr2a Sr2b 8_665 . 13_545 119.39(9) ?
Sr2c Sr2a Sr2b 8_665 . 13_555 0.61(8) ?
Sr2c Sr2a Sr2b 8_665 . 14_655 179.22(10) ?
Sr2c Sr2a Sr2b 8_665 . 15_565 60.00(9) ?
Sr2c Sr2a N3ac 8_665 . 1_665 79.61(8) ?
Sr2c Sr2a N2a 8_665 . 10_564 116.06(17) ?
Sr2c Sr2a C2a 8_665 . 10_564 134.07(14) ?
Sr2c Sr2a C2a 8_665 . 12_454 71.85(18) ?
Sr2c Sr2a Fe1c 8_665 . 16_555 131.25(9) ?
Sr2c Sr2a Fe1b 8_665 . 4_665 79.11(8) ?
Sr2c Sr2a N3ab 8_665 . 13_555 128.99(12) ?
Sr2c Sr2a N1c 8_665 . 7_455 124.06(14) ?
Sr2c Sr2a N1b 8_665 . 13_555 80.76(8) ?
Sr2c Sr2a C2c 8_665 . 16_565 92.71(16) ?
Sr2c Sr2a C2c 8_665 . 17_655 130.54(18) ?
Sr2c Sr2a C2b 8_665 . 4_675 48.45(17) ?
Sr2c Sr2a C2b 8_665 . 6_555 115.2(2) ?
Sr2c Sr2a C1a 8_665 . 10_565 33.21(11) ?
Sr2c Sr2a C1c 8_665 . 16_555 135.69(14) ?
Sr2c Sr2a C1b 8_665 . 4_665 78.18(8) ?
Sr2c Sr2a Sr2b 9_565 . 13_445 120.17(2) ?
Sr2c Sr2a Sr2b 9_565 . 13_545 0.168(14) ?
Sr2c Sr2a Sr2b 9_565 . 13_555 119.83(3) ?
Sr2c Sr2a Sr2b 9_565 . 14_655 60.00(3) ?
Sr2c Sr2a Sr2b 9_565 . 15_565 179.22(6) ?
Sr2c Sr2a N3ac 9_565 . 1_665 51.32(8) ?
Sr2c Sr2a N2a 9_565 . 10_564 63.8(2) ?
Sr2c Sr2a C2a 9_565 . 10_564 45.93(16) ?
Sr2c Sr2a C2a 9_565 . 12_454 143.19(18) ?
Sr2c Sr2a Fe1c 9_565 . 16_555 100.41(3) ?
Sr2c Sr2a Fe1b 9_565 . 4_665 49.11(3) ?
Sr2c Sr2a N3ab 9_565 . 13_555 99.93(3) ?
Sr2c Sr2a N1c 9_565 . 7_455 98.83(4) ?
Sr2c Sr2a N1b 9_565 . 13_555 56.18(11) ?
Sr2c Sr2a C2c 9_565 . 16_565 131.33(17) ?
Sr2c Sr2a C2c 9_565 . 17_655 64.6(3) ?
Sr2c Sr2a C2b 9_565 . 4_675 87.8(2) ?
Sr2c Sr2a C2b 9_565 . 6_555 48.7(2) ?
Sr2c Sr2a C1a 9_565 . 10_565 147.00(9) ?
Sr2c Sr2a C1c 9_565 . 16_555 101.31(3) ?
Sr2c Sr2a C1b 9_565 . 4_665 44.76(10) ?
Sr2b Sr2a Sr2b 13_445 . 13_545 120.00(2) ?
Sr2b Sr2a Sr2b 13_445 . 13_555 120.00(3) ?
Sr2b Sr2a Sr2b 13_445 . 14_655 60.17(2) ?
Sr2b Sr2a Sr2b 13_445 . 15_565 60.61(6) ?
Sr2b Sr2a N3ac 13_445 . 1_665 142.65(13) ?
Sr2b Sr2a N2a 13_445 . 10_564 90.01(15) ?
Sr2b Sr2a C2a 13_445 . 10_564 89.82(14) ?
Sr2b Sr2a C2a 13_445 . 12_454 61.25(12) ?
Sr2b Sr2a Fe1c 13_445 . 16_555 33.76(3) ?
Sr2b Sr2a Fe1b 13_445 . 4_665 146.38(4) ?
Sr2b Sr2a N3ab 13_445 . 13_555 37.50(12) ?
Sr2b Sr2a N1c 13_445 . 7_455 45.08(17) ?
Sr2b Sr2a N1b 13_445 . 13_555 135.07(17) ?
Sr2b Sr2a C2c 13_445 . 16_565 45.73(12) ?
Sr2b Sr2a C2c 13_445 . 17_655 77.3(3) ?
Sr2b Sr2a C2b 13_445 . 4_675 134.00(17) ?
Sr2b Sr2a C2b 13_445 . 6_555 103.22(15) ?
Sr2b Sr2a C1a 13_445 . 10_565 90.11(2) ?
Sr2b Sr2a C1c 13_445 . 16_555 25.54(19) ?
Sr2b Sr2a C1b 13_445 . 4_665 154.6(2) ?
Sr2b Sr2a Sr2b 13_545 . 13_555 120.00(2) ?
Sr2b Sr2a Sr2b 13_545 . 14_655 59.83(2) ?
Sr2b Sr2a Sr2b 13_545 . 15_565 179.39(6) ?
Sr2b Sr2a N3ac 13_545 . 1_665 51.44(8) ?
Sr2b Sr2a N2a 13_545 . 10_564 63.8(2) ?
Sr2b Sr2a C2a 13_545 . 10_564 45.84(16) ?
Sr2b Sr2a C2a 13_545 . 12_454 143.17(18) ?
Sr2b Sr2a Fe1c 13_545 . 16_555 100.26(3) ?
Sr2b Sr2a Fe1b 13_545 . 4_665 49.24(2) ?
Sr2b Sr2a N3ab 13_545 . 13_555 99.79(3) ?
Sr2b Sr2a N1c 13_545 . 7_455 98.71(3) ?
Sr2b Sr2a N1b 13_545 . 13_555 56.28(11) ?
Sr2b Sr2a C2c 13_545 . 16_565 131.23(17) ?
Sr2b Sr2a C2c 13_545 . 17_655 64.5(3) ?
Sr2b Sr2a C2b 13_545 . 4_675 87.9(2) ?
Sr2b Sr2a C2b 13_545 . 6_555 48.7(2) ?
Sr2b Sr2a C1a 13_545 . 10_565 147.15(9) ?
Sr2b Sr2a C1c 13_545 . 16_555 101.15(3) ?
Sr2b Sr2a C1b 13_545 . 4_665 44.91(9) ?
Sr2b Sr2a Sr2b 13_555 . 14_655 179.83(3) ?
Sr2b Sr2a Sr2b 13_555 . 15_565 59.39(6) ?
Sr2b Sr2a N3ac 13_555 . 1_665 80.12(2) ?
Sr2b Sr2a N2a 13_555 . 10_564 116.23(16) ?
Sr2b Sr2a C2a 13_555 . 10_564 134.41(12) ?
Sr2b Sr2a C2a 13_555 . 12_454 71.37(16) ?
Sr2b Sr2a Fe1c 13_555 . 16_555 130.78(4) ?
Sr2b Sr2a Fe1b 13_555 . 4_665 79.645(19) ?
Sr2b Sr2a N3ab 13_555 . 13_555 128.56(8) ?
Sr2b Sr2a N1c 13_555 . 7_455 123.69(12) ?
Sr2b Sr2a N1b 13_555 . 13_555 81.21(3) ?
Sr2b Sr2a C2c 13_555 . 16_565 92.23(14) ?
Sr2b Sr2a C2c 13_555 . 17_655 130.64(16) ?
Sr2b Sr2a C2b 13_555 . 4_675 48.79(16) ?
Sr2b Sr2a C2b 13_555 . 6_555 115.54(19) ?
Sr2b Sr2a C1a 13_555 . 10_565 32.65(9) ?
Sr2b Sr2a C1c 13_555 . 16_555 135.15(10) ?
Sr2b Sr2a C1b 13_555 . 4_665 78.76(3) ?
Sr2b Sr2a Sr2b 14_655 . 15_565 120.78(6) ?
Sr2b Sr2a N3ac 14_655 . 1_665 99.74(4) ?
Sr2b Sr2a N2a 14_655 . 10_564 63.72(16) ?
Sr2b Sr2a C2a 14_655 . 10_564 45.49(12) ?
Sr2b Sr2a C2a 14_655 . 12_454 108.76(16) ?
Sr2b Sr2a Fe1c 14_655 . 16_555 49.35(2) ?
Sr2b Sr2a Fe1b 14_655 . 4_665 100.21(3) ?
Sr2b Sr2a N3ab 14_655 . 13_555 51.56(8) ?
Sr2b Sr2a N1c 14_655 . 7_455 56.40(11) ?
Sr2b Sr2a N1b 14_655 . 13_555 98.67(4) ?
Sr2b Sr2a C2c 14_655 . 16_565 87.90(14) ?
Sr2b Sr2a C2c 14_655 . 17_655 49.33(16) ?
Sr2b Sr2a C2b 14_655 . 4_675 131.12(16) ?
Sr2b Sr2a C2b 14_655 . 6_555 64.37(19) ?
Sr2b Sr2a C1a 14_655 . 10_565 147.50(9) ?
Sr2b Sr2a C1c 14_655 . 16_555 45.00(9) ?
Sr2b Sr2a C1b 14_655 . 4_665 101.08(4) ?
Sr2b Sr2a N3ac 15_565 . 1_665 128.12(10) ?
Sr2b Sr2a N2a 15_565 . 10_564 116.4(2) ?
Sr2b Sr2a C2a 15_565 . 10_564 134.51(18) ?
Sr2b Sr2a C2a 15_565 . 12_454 36.93(19) ?
Sr2b Sr2a Fe1c 15_565 . 16_555 80.27(6) ?
Sr2b Sr2a Fe1b 15_565 . 4_665 130.29(7) ?
Sr2b Sr2a N3ab 15_565 . 13_555 80.72(7) ?
Sr2b Sr2a N1c 15_565 . 7_455 81.74(7) ?
Sr2b Sr2a N1b 15_565 . 13_555 123.35(13) ?
Sr2b Sr2a C2c 15_565 . 16_565 49.12(18) ?
Sr2b Sr2a C2c 15_565 . 17_655 115.9(3) ?
Sr2b Sr2a C2b 15_565 . 4_675 91.6(2) ?
Sr2b Sr2a C2b 15_565 . 6_555 131.4(2) ?
Sr2b Sr2a C1a 15_565 . 10_565 32.30(10) ?
Sr2b Sr2a C1c 15_565 . 16_555 79.43(6) ?
Sr2b Sr2a C1b 15_565 . 4_665 134.54(11) ?
N3ac Sr2a N2a 1_665 . 10_564 109.7(2) ?
N3ac Sr2a C2a 1_665 . 10_564 96.67(19) ?
N3ac Sr2a C2a 1_665 . 12_454 151.08(15) ?
N3ac Sr2a Fe1c 1_665 . 16_555 148.66(4) ?
N3ac Sr2a Fe1b 1_665 . 4_665 62.01(15) ?
N3ac Sr2a N3ab 1_665 . 13_555 105.15(18) ?
N3ac Sr2a N1c 1_665 . 7_455 97.7(2) ?
N3ac Sr2a N1b 1_665 . 13_555 8.6(2) ?
N3ac Sr2a C2c 1_665 . 16_565 171.10(15) ?
N3ac Sr2a C2c 1_665 . 17_655 115.0(3) ?
N3ac Sr2a C2b 1_665 . 4_675 83.3(2) ?
N3ac Sr2a C2b 1_665 . 6_555 93.5(2) ?
N3ac Sr2a C1a 1_665 . 10_565 96.96(14) ?
N3ac Sr2a C1c 1_665 . 16_555 118.0(3) ?
N3ac Sr2a C1b 1_665 . 4_665 15.1(3) ?
N2a Sr2a C2a 10_564 . 10_564 23.0(2) ?
N2a Sr2a C2a 10_564 . 12_454 79.7(3) ?
N2a Sr2a Fe1c 10_564 . 16_555 56.25(15) ?
N2a Sr2a Fe1b 10_564 . 4_665 56.37(15) ?
N2a Sr2a N3ab 10_564 . 13_555 109.83(18) ?
N2a Sr2a N1c 10_564 . 7_455 117.1(2) ?
N2a Sr2a N1b 10_564 . 13_555 117.0(3) ?
N2a Sr2a C2c 10_564 . 16_565 69.5(3) ?
N2a Sr2a C2c 10_564 . 17_655 15.6(2) ?
N2a Sr2a C2b 10_564 . 4_675 69.4(2) ?
N2a Sr2a C2b 10_564 . 6_555 16.3(3) ?
N2a Sr2a C1a 10_564 . 10_565 134.5(3) ?
N2a Sr2a C1c 10_564 . 16_555 96.7(3) ?
N2a Sr2a C1b 10_564 . 4_665 96.6(3) ?
C2a Sr2a C2a 10_564 . 12_454 99.8(2) ?
C2a Sr2a Fe1c 10_564 . 16_555 59.36(15) ?
C2a Sr2a Fe1b 10_564 . 4_665 59.83(13) ?
C2a Sr2a N3ab 10_564 . 13_555 96.41(15) ?
C2a Sr2a N1c 10_564 . 7_455 101.86(16) ?
C2a Sr2a N1b 10_564 . 13_555 102.1(2) ?
C2a Sr2a C2c 10_564 . 16_565 85.4(2) ?
C2a Sr2a C2c 10_564 . 17_655 18.6(3) ?
C2a Sr2a C2b 10_564 . 4_675 85.6(2) ?
C2a Sr2a C2b 10_564 . 6_555 18.9(2) ?
C2a Sr2a C1a 10_564 . 10_565 157.5(3) ?
C2a Sr2a C1c 10_564 . 16_555 86.7(2) ?
C2a Sr2a C1b 10_564 . 4_665 87.0(2) ?
C2a Sr2a Fe1c 12_454 . 16_555 59.42(16) ?
C2a Sr2a Fe1b 12_454 . 4_665 106.97(14) ?
C2a Sr2a N3ab 12_454 . 13_555 96.50(15) ?
C2a Sr2a N1c 12_454 . 7_455 101.94(17) ?
C2a Sr2a N1b 12_454 . 13_555 152.33(17) ?
C2a Sr2a C2c 12_454 . 16_565 20.9(2) ?
C2a Sr2a C2c 12_454 . 17_655 81.6(3) ?
C2a Sr2a C2b 12_454 . 4_675 74.5(2) ?
C2a Sr2a C2b 12_454 . 6_555 94.5(3) ?
C2a Sr2a C1a 12_454 . 10_565 60.9(3) ?
C2a Sr2a C1c 12_454 . 16_555 86.7(2) ?
C2a Sr2a C1b 12_454 . 4_665 144.1(2) ?
Fe1c Sr2a Fe1b 16_555 . 4_665 112.61(5) ?
Fe1c Sr2a N3ab 16_555 . 13_555 62.25(15) ?
Fe1c Sr2a N1c 16_555 . 7_455 70.87(19) ?
Fe1c Sr2a N1b 16_555 . 13_555 147.92(5) ?
Fe1c Sr2a C2c 16_555 . 16_565 38.57(14) ?
Fe1c Sr2a C2c 16_555 . 17_655 44.2(3) ?
Fe1c Sr2a C2b 16_555 . 4_675 112.02(14) ?
Fe1c Sr2a C2b 16_555 . 6_555 70.04(16) ?
Fe1c Sr2a C1a 16_555 . 10_565 112.53(10) ?
Fe1c Sr2a C1c 16_555 . 16_555 47.1(3) ?
Fe1c Sr2a C1b 16_555 . 4_665 145.06(13) ?
Fe1b Sr2a N3ab 4_665 . 13_555 148.63(4) ?
Fe1b Sr2a N1c 4_665 . 7_455 147.82(6) ?
Fe1b Sr2a N1b 4_665 . 13_555 70.62(19) ?
Fe1b Sr2a C2c 4_665 . 16_565 112.36(15) ?
Fe1b Sr2a C2c 4_665 . 17_655 69.6(2) ?
Fe1b Sr2a C2b 4_665 . 4_675 38.7(2) ?
Fe1b Sr2a C2b 4_665 . 6_555 43.94(15) ?
Fe1b Sr2a C1a 4_665 . 10_565 112.25(10) ?
Fe1b Sr2a C1c 4_665 . 16_555 145.11(12) ?
Fe1b Sr2a C1b 4_665 . 4_665 46.9(3) ?
N3ab Sr2a N1c 13_555 . 7_455 8.6(2) ?
N3ab Sr2a N1b 13_555 . 13_555 97.7(2) ?
N3ab Sr2a C2c 13_555 . 16_565 83.15(17) ?
N3ab Sr2a C2c 13_555 . 17_655 94.2(2) ?
N3ab Sr2a C2b 13_555 . 4_675 171.0(2) ?
N3ab Sr2a C2b 13_555 . 6_555 115.1(2) ?
N3ab Sr2a C1a 13_555 . 10_565 97.15(15) ?
N3ab Sr2a C1c 13_555 . 16_555 15.2(3) ?
N3ab Sr2a C1b 13_555 . 4_665 117.9(3) ?
N1c Sr2a N1b 7_455 . 13_555 90.0(2) ?
N1c Sr2a C2c 7_455 . 16_565 90.3(2) ?
N1c Sr2a C2c 7_455 . 17_655 101.5(2) ?
N1c Sr2a C2b 7_455 . 4_675 172.2(2) ?
N1c Sr2a C2b 7_455 . 6_555 120.7(2) ?
N1c Sr2a C1a 7_455 . 10_565 93.90(17) ?
N1c Sr2a C1c 7_455 . 16_555 23.8(3) ?
N1c Sr2a C1b 7_455 . 4_665 111.2(3) ?
N1b Sr2a C2c 13_555 . 16_565 172.28(18) ?
N1b Sr2a C2c 13_555 . 17_655 120.7(3) ?
N1b Sr2a C2b 13_555 . 4_675 90.4(2) ?
N1b Sr2a C2b 13_555 . 6_555 100.8(3) ?
N1b Sr2a C1a 13_555 . 10_565 93.74(17) ?
N1b Sr2a C1c 13_555 . 16_555 111.2(3) ?
N1b Sr2a C1b 13_555 . 4_665 23.7(3) ?
C2c Sr2a C2c 16_565 . 17_655 66.8(3) ?
C2c Sr2a C2b 16_565 . 4_675 88.3(2) ?
C2c Sr2a C2b 16_565 . 6_555 85.7(3) ?
C2c Sr2a C1a 16_565 . 10_565 78.6(2) ?
C2c Sr2a C1c 16_565 . 16_555 70.7(3) ?
C2c Sr2a C1b 16_565 . 4_665 158.3(3) ?
C2c Sr2a C2b 17_655 . 4_675 84.9(2) ?
C2c Sr2a C2b 17_655 . 6_555 26.0(3) ?
C2c Sr2a C1a 17_655 . 10_565 141.8(3) ?
C2c Sr2a C1c 17_655 . 16_555 81.3(3) ?
C2c Sr2a C1b 17_655 . 4_665 104.3(4) ?
C2b Sr2a C2b 4_675 . 6_555 66.8(3) ?
C2b Sr2a C1a 4_675 . 10_565 78.3(2) ?
C2b Sr2a C1c 4_675 . 16_555 158.1(3) ?
C2b Sr2a C1b 4_675 . 4_665 70.9(3) ?
C2b Sr2a C1a 6_555 . 10_565 142.0(3) ?
C2b Sr2a C1c 6_555 . 16_555 104.5(3) ?
C2b Sr2a C1b 6_555 . 4_665 80.6(3) ?
C1a Sr2a C1c 10_565 . 16_555 102.49(13) ?
C1a Sr2a C1b 10_565 . 4_665 102.24(13) ?
C1c Sr2a C1b 16_555 . 4_665 129.0(3) ?
Sr1 Fe1a Sr1 1_544 . 2_664 66.06(4) ?
Sr1 Fe1a Sr1 1_544 . 3_454 66.06(3) ?
Sr1 Fe1a Sr2a 1_544 . 16_654 73.50(2) ?
Sr1 Fe1a Sr2a 1_544 . 17_434 124.21(3) ?
Sr1 Fe1a Sr2a 1_544 . 18_454 127.76(3) ?
Sr1 Fe1a Sr2c 1_544 . 4_664 124.83(3) ?
Sr1 Fe1a Sr2c 1_544 . 5_544 80.19(3) ?
Sr1 Fe1a Sr2c 1_544 . 6_454 136.23(4) ?
Sr1 Fe1a Sr2b 1_544 . 10_554 121.54(3) ?
Sr1 Fe1a Sr2b 1_544 . 11_444 139.62(4) ?
Sr1 Fe1a Sr2b 1_544 . 12_454 80.92(3) ?
Sr1 Fe1a C2a 1_544 . 1_454 108.7(2) ?
Sr1 Fe1a C2a 1_544 . 2_544 54.2(2) ?
Sr1 Fe1a C2a 1_544 . 3_664 57.0(3) ?
Sr1 Fe1a C1a 1_544 . . 141.00(2) ?
Sr1 Fe1a Sr1 2_664 . 3_454 66.06(3) ?
Sr1 Fe1a Sr2a 2_664 . 16_654 124.21(3) ?
Sr1 Fe1a Sr2a 2_664 . 17_434 127.76(3) ?
Sr1 Fe1a Sr2a 2_664 . 18_454 73.50(3) ?
Sr1 Fe1a Sr2c 2_664 . 4_664 80.19(3) ?
Sr1 Fe1a Sr2c 2_664 . 5_544 136.23(4) ?
Sr1 Fe1a Sr2c 2_664 . 6_454 124.83(4) ?
Sr1 Fe1a Sr2b 2_664 . 10_554 139.62(4) ?
Sr1 Fe1a Sr2b 2_664 . 11_444 80.92(3) ?
Sr1 Fe1a Sr2b 2_664 . 12_454 121.54(3) ?
Sr1 Fe1a C2a 2_664 . 1_454 57.0(2) ?
Sr1 Fe1a C2a 2_664 . 2_544 108.7(2) ?
Sr1 Fe1a C2a 2_664 . 3_664 54.2(3) ?
Sr1 Fe1a C1a 2_664 . . 141.00(3) ?
Sr1 Fe1a Sr2a 3_454 . 16_654 127.76(4) ?
Sr1 Fe1a Sr2a 3_454 . 17_434 73.50(2) ?
Sr1 Fe1a Sr2a 3_454 . 18_454 124.21(3) ?
Sr1 Fe1a Sr2c 3_454 . 4_664 136.23(4) ?
Sr1 Fe1a Sr2c 3_454 . 5_544 124.83(3) ?
Sr1 Fe1a Sr2c 3_454 . 6_454 80.19(3) ?
Sr1 Fe1a Sr2b 3_454 . 10_554 80.92(3) ?
Sr1 Fe1a Sr2b 3_454 . 11_444 121.54(4) ?
Sr1 Fe1a Sr2b 3_454 . 12_454 139.62(4) ?
Sr1 Fe1a C2a 3_454 . 1_454 54.2(3) ?
Sr1 Fe1a C2a 3_454 . 2_544 57.0(3) ?
Sr1 Fe1a C2a 3_454 . 3_664 108.7(2) ?
Sr1 Fe1a C1a 3_454 . . 141.00(2) ?
Sr2a Fe1a Sr2a 16_654 . 17_434 106.33(4) ?
Sr2a Fe1a Sr2a 16_654 . 18_454 106.33(3) ?
Sr2a Fe1a Sr2c 16_654 . 4_664 93.84(4) ?
Sr2a Fe1a Sr2c 16_654 . 5_544 12.484(19) ?
Sr2a Fe1a Sr2c 16_654 . 6_454 110.94(5) ?
Sr2a Fe1a Sr2b 16_654 . 10_554 94.03(4) ?
Sr2a Fe1a Sr2b 16_654 . 11_444 110.66(5) ?
Sr2a Fe1a Sr2b 16_654 . 12_454 12.30(3) ?
Sr2a Fe1a C2a 16_654 . 1_454 177.8(2) ?
Sr2a Fe1a C2a 16_654 . 2_544 73.0(3) ?
Sr2a Fe1a C2a 16_654 . 3_664 72.0(4) ?
Sr2a Fe1a C1a 16_654 . . 67.54(3) ?
Sr2a Fe1a Sr2a 17_434 . 18_454 106.33(4) ?
Sr2a Fe1a Sr2c 17_434 . 4_664 110.94(5) ?
Sr2a Fe1a Sr2c 17_434 . 5_544 93.84(4) ?
Sr2a Fe1a Sr2c 17_434 . 6_454 12.48(3) ?
Sr2a Fe1a Sr2b 17_434 . 10_554 12.30(3) ?
Sr2a Fe1a Sr2b 17_434 . 11_444 94.03(4) ?
Sr2a Fe1a Sr2b 17_434 . 12_454 110.66(5) ?
Sr2a Fe1a C2a 17_434 . 1_454 73.0(2) ?
Sr2a Fe1a C2a 17_434 . 2_544 72.0(2) ?
Sr2a Fe1a C2a 17_434 . 3_664 177.8(2) ?
Sr2a Fe1a C1a 17_434 . . 67.54(3) ?
Sr2a Fe1a Sr2c 18_454 . 4_664 12.48(2) ?
Sr2a Fe1a Sr2c 18_454 . 5_544 110.94(5) ?
Sr2a Fe1a Sr2c 18_454 . 6_454 93.84(4) ?
Sr2a Fe1a Sr2b 18_454 . 10_554 110.66(5) ?
Sr2a Fe1a Sr2b 18_454 . 11_444 12.30(2) ?
Sr2a Fe1a Sr2b 18_454 . 12_454 94.03(4) ?
Sr2a Fe1a C2a 18_454 . 1_454 72.0(3) ?
Sr2a Fe1a C2a 18_454 . 2_544 177.8(2) ?
Sr2a Fe1a C2a 18_454 . 3_664 73.0(3) ?
Sr2a Fe1a C1a 18_454 . . 67.54(3) ?
Sr2c Fe1a Sr2c 4_664 . 5_544 98.74(5) ?
Sr2c Fe1a Sr2c 4_664 . 6_454 98.74(5) ?
Sr2c Fe1a Sr2b 4_664 . 10_554 112.61(6) ?
Sr2c Fe1a Sr2b 4_664 . 11_444 20.62(3) ?
Sr2c Fe1a Sr2b 4_664 . 12_454 81.54(4) ?
Sr2c Fe1a C2a 4_664 . 1_454 84.5(3) ?
Sr2c Fe1a C2a 4_664 . 2_544 166.7(3) ?
Sr2c Fe1a C2a 4_664 . 3_664 67.9(3) ?
Sr2c Fe1a C1a 4_664 . . 61.21(4) ?
Sr2c Fe1a Sr2c 5_544 . 6_454 98.74(5) ?
Sr2c Fe1a Sr2b 5_544 . 10_554 81.54(4) ?
Sr2c Fe1a Sr2b 5_544 . 11_444 112.61(6) ?
Sr2c Fe1a Sr2b 5_544 . 12_454 20.62(3) ?
Sr2c Fe1a C2a 5_544 . 1_454 166.7(2) ?
Sr2c Fe1a C2a 5_544 . 2_544 67.9(3) ?
Sr2c Fe1a C2a 5_544 . 3_664 84.5(4) ?
Sr2c Fe1a C1a 5_544 . . 61.21(4) ?
Sr2c Fe1a Sr2b 6_454 . 10_554 20.62(4) ?
Sr2c Fe1a Sr2b 6_454 . 11_444 81.54(4) ?
Sr2c Fe1a Sr2b 6_454 . 12_454 112.61(6) ?
Sr2c Fe1a C2a 6_454 . 1_454 67.9(2) ?
Sr2c Fe1a C2a 6_454 . 2_544 84.5(2) ?
Sr2c Fe1a C2a 6_454 . 3_664 166.7(3) ?
Sr2c Fe1a C1a 6_454 . . 61.21(4) ?
Sr2b Fe1a Sr2b 10_554 . 11_444 98.60(5) ?
Sr2b Fe1a Sr2b 10_554 . 12_454 98.60(5) ?
Sr2b Fe1a C2a 10_554 . 1_454 85.3(2) ?
Sr2b Fe1a C2a 10_554 . 2_544 67.4(2) ?
Sr2b Fe1a C2a 10_554 . 3_664 166.0(3) ?
Sr2b Fe1a C1a 10_554 . . 61.09(4) ?
Sr2b Fe1a Sr2b 11_444 . 12_454 98.60(5) ?
Sr2b Fe1a C2a 11_444 . 1_454 67.4(3) ?
Sr2b Fe1a C2a 11_444 . 2_544 166.0(2) ?
Sr2b Fe1a C2a 11_444 . 3_664 85.3(3) ?
Sr2b Fe1a C1a 11_444 . . 61.09(4) ?
Sr2b Fe1a C2a 12_454 . 1_454 166.0(3) ?
Sr2b Fe1a C2a 12_454 . 2_544 85.3(3) ?
Sr2b Fe1a C2a 12_454 . 3_664 67.4(3) ?
Sr2b Fe1a C1a 12_454 . . 61.09(4) ?
C2a Fe1a C2a 1_454 . 2_544 108.6(4) ?
C2a Fe1a C2a 1_454 . 3_664 108.6(4) ?
C2a Fe1a C1a 1_454 . . 110.3(2) ?
C2a Fe1a C2a 2_544 . 3_664 108.6(4) ?
C2a Fe1a C1a 2_544 . . 110.3(2) ?
C2a Fe1a C1a 3_664 . . 110.3(2) ?
Sr1 Sr2c Sr1 13_544 . 14_664 63.32(3) ?
Sr1 Sr2c Sr1 13_544 . 15_564 68.77(2) ?
Sr1 Sr2c Sr1 13_544 . 5_554 152.88(4) ?
Sr1 Sr2c Sr2a 13_544 . 13_444 87.88(2) ?
Sr1 Sr2c Sr2a 13_544 . 13_544 63.62(3) ?
Sr1 Sr2c Sr2a 13_544 . 13_554 118.77(3) ?
Sr1 Sr2c Sr2a 13_544 . 14_654 61.18(2) ?
Sr1 Sr2c Sr2a 13_544 . 15_564 116.58(7) ?
Sr1 Sr2c Fe1a 13_544 . 4_665 106.95(4) ?
Sr1 Sr2c Sr2c 13_544 . 2_665 94.16(2) ?
Sr1 Sr2c Sr2c 13_544 . 2_765 68.07(3) ?
Sr1 Sr2c Sr2c 13_544 . 3_565 64.95(2) ?
Sr1 Sr2c Sr2c 13_544 . 3_675 98.39(3) ?
Sr1 Sr2c Sr2b 13_544 . 7_445 61.23(2) ?
Sr1 Sr2c Sr2b 13_544 . 7_455 116.38(3) ?
Sr1 Sr2c Sr2b 13_544 . 7_555 92.12(2) ?
Sr1 Sr2c Sr2b 13_544 . 8_665 118.60(8) ?
Sr1 Sr2c Sr2b 13_544 . 9_565 63.68(3) ?
Sr1 Sr2c N3ac 13_544 . 13_554 50.70(11) ?
Sr1 Sr2c N1a 13_544 . 13_554 48.62(14) ?
Sr1 Sr2c N3bc 13_544 . 1_665 55.08(11) ?
Sr1 Sr2c C2a 13_544 . 4_674 138.07(17) ?
Sr1 Sr2c C2a 13_544 . 6_554 107.4(2) ?
Sr1 Sr2c Fe1c 13_544 . 10_564 144.74(4) ?
Sr1 Sr2c Fe1b 13_544 . 16_555 103.35(3) ?
Sr1 Sr2c N2c 13_544 . 10_564 117.0(2) ?
Sr1 Sr2c N1b 13_544 . 7_455 44.33(13) ?
Sr1 Sr2c C2c 13_544 . 10_564 93.93(14) ?
Sr1 Sr2c C2c 13_544 . 12_454 145.87(13) ?
Sr1 Sr2c C2b 13_544 . 16_565 133.56(12) ?
Sr1 Sr2c C2b 13_544 . 17_655 106.9(2) ?
Sr1 Sr2c C1a 13_544 . 4_665 67.2(2) ?
Sr1 Sr2c C1c 13_544 . 10_564 108.5(2) ?
Sr1 Sr2c C1b 13_544 . 16_555 62.9(2) ?
Sr1 Sr2c Sr1 14_664 . 15_564 60.30(3) ?
Sr1 Sr2c Sr1 14_664 . 5_554 137.02(4) ?
Sr1 Sr2c Sr2a 14_664 . 13_444 60.39(2) ?
Sr1 Sr2c Sr2a 14_664 . 13_544 126.87(3) ?
Sr1 Sr2c Sr2a 14_664 . 13_554 83.92(3) ?
Sr1 Sr2c Sr2a 14_664 . 14_654 96.19(3) ?
Sr1 Sr2c Sr2a 14_664 . 15_564 53.30(7) ?
Sr1 Sr2c Fe1a 14_664 . 4_665 153.21(4) ?
Sr1 Sr2c Sr2c 14_664 . 2_665 55.48(2) ?
Sr1 Sr2c Sr2c 14_664 . 2_765 129.29(3) ?
Sr1 Sr2c Sr2c 14_664 . 3_565 88.57(3) ?
Sr1 Sr2c Sr2c 14_664 . 3_675 113.58(3) ?
Sr1 Sr2c Sr2b 14_664 . 7_445 96.08(2) ?
Sr1 Sr2c Sr2b 14_664 . 7_455 53.13(3) ?
Sr1 Sr2c Sr2b 14_664 . 7_555 119.61(2) ?
Sr1 Sr2c Sr2b 14_664 . 8_665 84.31(8) ?
Sr1 Sr2c Sr2b 14_664 . 9_565 126.92(3) ?
Sr1 Sr2c N3ac 14_664 . 13_554 44.97(10) ?
Sr1 Sr2c N1a 14_664 . 13_554 86.12(18) ?
Sr1 Sr2c N3bc 14_664 . 1_665 94.50(14) ?
Sr1 Sr2c C2a 14_664 . 4_674 132.46(17) ?
Sr1 Sr2c C2a 14_664 . 6_554 160.01(17) ?
Sr1 Sr2c Fe1c 14_664 . 10_564 85.27(4) ?
Sr1 Sr2c Fe1b 14_664 . 16_555 94.14(4) ?
Sr1 Sr2c N2c 14_664 . 10_564 150.28(15) ?
Sr1 Sr2c N1b 14_664 . 7_455 39.87(10) ?
Sr1 Sr2c C2c 14_664 . 10_564 141.38(12) ?
Sr1 Sr2c C2c 14_664 . 12_454 87.34(16) ?
Sr1 Sr2c C2b 14_664 . 16_565 89.16(16) ?
Sr1 Sr2c C2b 14_664 . 17_655 136.1(2) ?
Sr1 Sr2c C1a 14_664 . 4_665 109.2(3) ?
Sr1 Sr2c C1c 14_664 . 10_564 54.68(18) ?
Sr1 Sr2c C1b 14_664 . 16_555 55.7(2) ?
Sr1 Sr2c Sr1 15_564 . 5_554 133.35(2) ?
Sr1 Sr2c Sr2a 15_564 . 13_444 120.60(3) ?
Sr1 Sr2c Sr2a 15_564 . 13_544 97.68(3) ?
Sr1 Sr2c Sr2a 15_564 . 13_554 50.011(18) ?
Sr1 Sr2c Sr2a 15_564 . 14_654 129.94(3) ?
Sr1 Sr2c Sr2a 15_564 . 15_564 81.91(7) ?
Sr1 Sr2c Fe1a 15_564 . 4_665 93.01(4) ?
Sr1 Sr2c Sr2c 15_564 . 2_665 114.03(3) ?
Sr1 Sr2c Sr2c 15_564 . 2_765 89.68(3) ?
Sr1 Sr2c Sr2c 15_564 . 3_565 132.32(3) ?
Sr1 Sr2c Sr2c 15_564 . 3_675 53.83(2) ?
Sr1 Sr2c Sr2b 15_564 . 7_445 129.99(3) ?
Sr1 Sr2c Sr2b 15_564 . 7_455 82.32(3) ?
Sr1 Sr2c Sr2b 15_564 . 7_555 59.40(2) ?
Sr1 Sr2c Sr2b 15_564 . 8_665 49.84(7) ?
Sr1 Sr2c Sr2b 15_564 . 9_565 97.56(3) ?
Sr1 Sr2c N3ac 15_564 . 13_554 96.73(14) ?
Sr1 Sr2c N1a 15_564 . 13_554 41.72(9) ?
Sr1 Sr2c N3bc 15_564 . 1_665 46.34(9) ?
Sr1 Sr2c C2a 15_564 . 4_674 86.73(13) ?
Sr1 Sr2c C2a 15_564 . 6_554 135.34(16) ?
Sr1 Sr2c Fe1c 15_564 . 10_564 82.28(3) ?
Sr1 Sr2c Fe1b 15_564 . 16_555 154.33(4) ?
Sr1 Sr2c N2c 15_564 . 10_564 149.38(15) ?
Sr1 Sr2c N1b 15_564 . 7_455 88.42(18) ?
Sr1 Sr2c C2c 15_564 . 10_564 142.90(16) ?
Sr1 Sr2c C2c 15_564 . 12_454 112.97(18) ?
Sr1 Sr2c C2b 15_564 . 16_565 130.59(17) ?
Sr1 Sr2c C2b 15_564 . 17_655 160.5(3) ?
Sr1 Sr2c C1a 15_564 . 4_665 56.3(2) ?
Sr1 Sr2c C1c 15_564 . 10_564 52.31(17) ?
Sr1 Sr2c C1b 15_564 . 16_555 111.3(3) ?
Sr1 Sr2c Sr2a 5_554 . 13_444 90.49(3) ?
Sr1 Sr2c Sr2a 5_554 . 13_544 94.30(3) ?
Sr1 Sr2c Sr2a 5_554 . 13_554 85.21(2) ?
Sr1 Sr2c Sr2a 5_554 . 14_654 94.80(3) ?
Sr1 Sr2c Sr2a 5_554 . 15_564 85.67(7) ?
Sr1 Sr2c Fe1a 5_554 . 4_665 62.50(4) ?
Sr1 Sr2c Sr2c 5_554 . 2_665 89.41(3) ?
Sr1 Sr2c Sr2c 5_554 . 2_765 93.58(3) ?
Sr1 Sr2c Sr2c 5_554 . 3_565 94.24(2) ?
Sr1 Sr2c Sr2c 5_554 . 3_675 88.45(2) ?
Sr1 Sr2c Sr2b 5_554 . 7_445 94.79(2) ?
Sr1 Sr2c Sr2b 5_554 . 7_455 85.70(3) ?
Sr1 Sr2c Sr2b 5_554 . 7_555 89.51(3) ?
Sr1 Sr2c Sr2b 5_554 . 8_665 85.24(7) ?
Sr1 Sr2c Sr2b 5_554 . 9_565 94.29(3) ?
Sr1 Sr2c N3ac 5_554 . 13_554 125.31(15) ?
Sr1 Sr2c N1a 5_554 . 13_554 132.79(19) ?
Sr1 Sr2c N3bc 5_554 . 1_665 124.23(15) ?
Sr1 Sr2c C2a 5_554 . 4_674 48.76(13) ?
Sr1 Sr2c C2a 5_554 . 6_554 46.9(2) ?
Sr1 Sr2c Fe1c 5_554 . 10_564 62.30(4) ?
Sr1 Sr2c Fe1b 5_554 . 16_555 63.31(4) ?
Sr1 Sr2c N2c 5_554 . 10_564 35.9(2) ?
Sr1 Sr2c N1b 5_554 . 7_455 133.88(19) ?
Sr1 Sr2c C2c 5_554 . 10_564 58.99(14) ?
Sr1 Sr2c C2c 5_554 . 12_454 49.86(16) ?
Sr1 Sr2c C2b 5_554 . 16_565 49.89(15) ?
Sr1 Sr2c C2b 5_554 . 17_655 46.63(19) ?
Sr1 Sr2c C1a 5_554 . 4_665 109.2(3) ?
Sr1 Sr2c C1c 5_554 . 10_564 98.6(2) ?
Sr1 Sr2c C1b 5_554 . 16_555 110.2(3) ?
Sr2a Sr2c Sr2a 13_444 . 13_544 120.00(2) ?
Sr2a Sr2c Sr2a 13_444 . 13_554 120.00(3) ?
Sr2a Sr2c Sr2a 13_444 . 14_654 60.17(2) ?
Sr2a Sr2c Sr2a 13_444 . 15_564 60.61(6) ?
Sr2a Sr2c Fe1a 13_444 . 4_665 146.38(4) ?
Sr2a Sr2c Sr2c 13_444 . 2_665 11.75(2) ?
Sr2a Sr2c Sr2c 13_444 . 2_765 131.84(3) ?
Sr2a Sr2c Sr2c 13_444 . 3_565 48.25(2) ?
Sr2a Sr2c Sr2c 13_444 . 3_675 168.16(3) ?
Sr2a Sr2c Sr2b 13_444 . 7_445 60.000(19) ?
Sr2a Sr2c Sr2b 13_444 . 7_455 60.000(19) ?
Sr2a Sr2c Sr2b 13_444 . 7_555 180 ?
Sr2a Sr2c Sr2b 13_444 . 8_665 120.61(9) ?
Sr2a Sr2c Sr2b 13_444 . 9_565 120.17(2) ?
Sr2a Sr2c N3ac 13_444 . 13_554 37.50(12) ?
Sr2a Sr2c N1a 13_444 . 13_554 135.07(17) ?
Sr2a Sr2c N3bc 13_444 . 1_665 142.65(13) ?
Sr2a Sr2c C2a 13_444 . 4_674 134.00(17) ?
Sr2a Sr2c C2a 13_444 . 6_554 103.22(15) ?
Sr2a Sr2c Fe1c 13_444 . 10_564 90.10(2) ?
Sr2a Sr2c Fe1b 13_444 . 16_555 33.76(3) ?
Sr2a Sr2c N2c 13_444 . 10_564 90.01(15) ?
Sr2a Sr2c N1b 13_444 . 7_455 45.08(17) ?
Sr2a Sr2c C2c 13_444 . 10_564 89.82(14) ?
Sr2a Sr2c C2c 13_444 . 12_454 61.25(12) ?
Sr2a Sr2c C2b 13_444 . 16_565 45.73(12) ?
Sr2a Sr2c C2b 13_444 . 17_655 77.3(3) ?
Sr2a Sr2c C1a 13_444 . 4_665 154.6(2) ?
Sr2a Sr2c C1c 13_444 . 10_564 90.11(2) ?
Sr2a Sr2c C1b 13_444 . 16_555 25.54(19) ?
Sr2a Sr2c Sr2a 13_544 . 13_554 120.00(2) ?
Sr2a Sr2c Sr2a 13_544 . 14_654 59.83(2) ?
Sr2a Sr2c Sr2a 13_544 . 15_564 179.39(6) ?
Sr2a Sr2c Fe1a 13_544 . 4_665 49.24(2) ?
Sr2a Sr2c Sr2c 13_544 . 2_665 131.75(3) ?
Sr2a Sr2c Sr2c 13_544 . 2_765 11.836(14) ?
Sr2a Sr2c Sr2c 13_544 . 3_565 71.75(2) ?
Sr2a Sr2c Sr2c 13_544 . 3_675 71.84(2) ?
Sr2a Sr2c Sr2b 13_544 . 7_445 60.000(19) ?
Sr2a Sr2c Sr2b 13_544 . 7_455 180 ?
Sr2a Sr2c Sr2b 13_544 . 7_555 60.000(19) ?
Sr2a Sr2c Sr2b 13_544 . 8_665 119.39(9) ?
Sr2a Sr2c Sr2b 13_544 . 9_565 0.168(15) ?
Sr2a Sr2c N3ac 13_544 . 13_554 99.79(3) ?
Sr2a Sr2c N1a 13_544 . 13_554 56.28(11) ?
Sr2a Sr2c N3bc 13_544 . 1_665 51.44(8) ?
Sr2a Sr2c C2a 13_544 . 4_674 87.9(2) ?
Sr2a Sr2c C2a 13_544 . 6_554 48.7(2) ?
Sr2a Sr2c Fe1c 13_544 . 10_564 143.08(3) ?
Sr2a Sr2c Fe1b 13_544 . 16_555 100.26(3) ?
Sr2a Sr2c N2c 13_544 . 10_564 63.8(2) ?
Sr2a Sr2c N1b 13_544 . 7_455 98.71(3) ?
Sr2a Sr2c C2c 13_544 . 10_564 45.84(16) ?
Sr2a Sr2c C2c 13_544 . 12_454 143.17(18) ?
Sr2a Sr2c C2b 13_544 . 16_565 131.23(17) ?
Sr2a Sr2c C2b 13_544 . 17_655 64.5(3) ?
Sr2a Sr2c C1a 13_544 . 4_665 44.91(9) ?
Sr2a Sr2c C1c 13_544 . 10_564 147.15(9) ?
Sr2a Sr2c C1b 13_544 . 16_555 101.15(3) ?
Sr2a Sr2c Sr2a 13_554 . 14_654 179.83(3) ?
Sr2a Sr2c Sr2a 13_554 . 15_564 59.39(6) ?
Sr2a Sr2c Fe1a 13_554 . 4_665 79.645(19) ?
Sr2a Sr2c Sr2c 13_554 . 2_665 108.25(3) ?
Sr2a Sr2c Sr2c 13_554 . 2_765 108.16(2) ?
Sr2a Sr2c Sr2c 13_554 . 3_565 168.25(3) ?
Sr2a Sr2c Sr2c 13_554 . 3_675 48.16(2) ?
Sr2a Sr2c Sr2b 13_554 . 7_445 180 ?
Sr2a Sr2c Sr2b 13_554 . 7_455 60.000(19) ?
Sr2a Sr2c Sr2b 13_554 . 7_555 60.000(19) ?
Sr2a Sr2c Sr2b 13_554 . 8_665 0.61(8) ?
Sr2a Sr2c Sr2b 13_554 . 9_565 119.83(3) ?
Sr2a Sr2c N3ac 13_554 . 13_554 128.56(8) ?
Sr2a Sr2c N1a 13_554 . 13_554 81.21(3) ?
Sr2a Sr2c N3bc 13_554 . 1_665 80.12(2) ?
Sr2a Sr2c C2a 13_554 . 4_674 48.79(16) ?
Sr2a Sr2c C2a 13_554 . 6_554 115.54(19) ?
Sr2a Sr2c Fe1c 13_554 . 10_564 36.75(2) ?
Sr2a Sr2c Fe1b 13_554 . 16_555 130.78(4) ?
Sr2a Sr2c N2c 13_554 . 10_564 116.23(16) ?
Sr2a Sr2c N1b 13_554 . 7_455 123.70(12) ?
Sr2a Sr2c C2c 13_554 . 10_564 134.41(12) ?
Sr2a Sr2c C2c 13_554 . 12_454 71.37(16) ?
Sr2a Sr2c C2b 13_554 . 16_565 92.23(14) ?
Sr2a Sr2c C2b 13_554 . 17_655 130.64(17) ?
Sr2a Sr2c C1a 13_554 . 4_665 78.76(3) ?
Sr2a Sr2c C1c 13_554 . 10_564 32.65(9) ?
Sr2a Sr2c C1b 13_554 . 16_555 135.15(10) ?
Sr2a Sr2c Sr2a 14_654 . 15_564 120.78(6) ?
Sr2a Sr2c Fe1a 14_654 . 4_665 100.21(3) ?
Sr2a Sr2c Sr2c 14_654 . 2_665 71.91(3) ?
Sr2a Sr2c Sr2c 14_654 . 2_765 71.67(3) ?
Sr2a Sr2c Sr2c 14_654 . 3_565 11.91(3) ?
Sr2a Sr2c Sr2c 14_654 . 3_675 131.67(4) ?
Sr2a Sr2c Sr2b 14_654 . 7_445 0.17(2) ?
Sr2a Sr2c Sr2b 14_654 . 7_455 120.17(3) ?
Sr2a Sr2c Sr2b 14_654 . 7_555 119.83(3) ?
Sr2a Sr2c Sr2b 14_654 . 8_665 179.22(10) ?
Sr2a Sr2c Sr2b 14_654 . 9_565 60.00(3) ?
Sr2a Sr2c N3ac 14_654 . 13_554 51.56(8) ?
Sr2a Sr2c N1a 14_654 . 13_554 98.67(4) ?
Sr2a Sr2c N3bc 14_654 . 1_665 99.74(4) ?
Sr2a Sr2c C2a 14_654 . 4_674 131.12(16) ?
Sr2a Sr2c C2a 14_654 . 6_554 64.37(19) ?
Sr2a Sr2c Fe1c 14_654 . 10_564 143.38(3) ?
Sr2a Sr2c Fe1b 14_654 . 16_555 49.35(2) ?
Sr2a Sr2c N2c 14_654 . 10_564 63.72(16) ?
Sr2a Sr2c N1b 14_654 . 7_455 56.41(11) ?
Sr2a Sr2c C2c 14_654 . 10_564 45.49(12) ?
Sr2a Sr2c C2c 14_654 . 12_454 108.76(16) ?
Sr2a Sr2c C2b 14_654 . 16_565 87.90(14) ?
Sr2a Sr2c C2b 14_654 . 17_655 49.33(16) ?
Sr2a Sr2c C1a 14_654 . 4_665 101.08(4) ?
Sr2a Sr2c C1c 14_654 . 10_564 147.50(9) ?
Sr2a Sr2c C1b 14_654 . 16_555 45.00(9) ?
Sr2a Sr2c Fe1a 15_564 . 4_665 130.29(7) ?
Sr2a Sr2c Sr2c 15_564 . 2_665 48.87(6) ?
Sr2a Sr2c Sr2c 15_564 . 2_765 167.55(6) ?
Sr2a Sr2c Sr2c 15_564 . 3_565 108.87(6) ?
Sr2a Sr2c Sr2c 15_564 . 3_675 107.55(6) ?
Sr2a Sr2c Sr2b 15_564 . 7_445 120.61(6) ?
Sr2a Sr2c Sr2b 15_564 . 7_455 0.61(5) ?
Sr2a Sr2c Sr2b 15_564 . 7_555 119.39(6) ?
Sr2a Sr2c Sr2b 15_564 . 8_665 60.00(9) ?
Sr2a Sr2c Sr2b 15_564 . 9_565 179.22(6) ?
Sr2a Sr2c N3ac 15_564 . 13_554 80.72(7) ?
Sr2a Sr2c N1a 15_564 . 13_554 123.36(13) ?
Sr2a Sr2c N3bc 15_564 . 1_665 128.12(10) ?
Sr2a Sr2c C2a 15_564 . 4_674 91.6(2) ?
Sr2a Sr2c C2a 15_564 . 6_554 131.4(2) ?
Sr2a Sr2c Fe1c 15_564 . 10_564 36.45(6) ?
Sr2a Sr2c Fe1b 15_564 . 16_555 80.27(6) ?
Sr2a Sr2c N2c 15_564 . 10_564 116.4(2) ?
Sr2a Sr2c N1b 15_564 . 7_455 81.75(7) ?
Sr2a Sr2c C2c 15_564 . 10_564 134.51(18) ?
Sr2a Sr2c C2c 15_564 . 12_454 36.93(18) ?
Sr2a Sr2c C2b 15_564 . 16_565 49.12(18) ?
Sr2a Sr2c C2b 15_564 . 17_655 115.9(3) ?
Sr2a Sr2c C1a 15_564 . 4_665 134.54(11) ?
Sr2a Sr2c C1c 15_564 . 10_564 32.30(10) ?
Sr2a Sr2c C1b 15_564 . 16_555 79.43(6) ?
Fe1a Sr2c Sr2c 4_665 . 2_665 150.56(4) ?
Fe1a Sr2c Sr2c 4_665 . 2_765 40.63(3) ?
Fe1a Sr2c Sr2c 4_665 . 3_565 110.52(3) ?
Fe1a Sr2c Sr2c 4_665 . 3_675 40.63(3) ?
Fe1a Sr2c Sr2b 4_665 . 7_445 100.36(3) ?
Fe1a Sr2c Sr2b 4_665 . 7_455 130.76(3) ?
Fe1a Sr2c Sr2b 4_665 . 7_555 33.62(3) ?
Fe1a Sr2c Sr2b 4_665 . 8_665 79.11(8) ?
Fe1a Sr2c Sr2b 4_665 . 9_565 49.11(3) ?
Fe1a Sr2c N3ac 4_665 . 13_554 148.63(4) ?
Fe1a Sr2c N1a 4_665 . 13_554 70.62(19) ?
Fe1a Sr2c N3bc 4_665 . 1_665 62.01(15) ?
Fe1a Sr2c C2a 4_665 . 4_674 38.7(2) ?
Fe1a Sr2c C2a 4_665 . 6_554 43.94(15) ?
Fe1a Sr2c Fe1c 4_665 . 10_564 93.84(3) ?
Fe1a Sr2c Fe1b 4_665 . 16_555 112.61(5) ?
Fe1a Sr2c N2c 4_665 . 10_564 56.37(15) ?
Fe1a Sr2c N1b 4_665 . 7_455 147.82(6) ?
Fe1a Sr2c C2c 4_665 . 10_564 59.83(13) ?
Fe1a Sr2c C2c 4_665 . 12_454 106.97(14) ?
Fe1a Sr2c C2b 4_665 . 16_565 112.36(15) ?
Fe1a Sr2c C2b 4_665 . 17_655 69.6(2) ?
Fe1a Sr2c C1a 4_665 . 4_665 46.9(3) ?
Fe1a Sr2c C1c 4_665 . 10_564 112.25(10) ?
Fe1a Sr2c C1b 4_665 . 16_555 145.11(12) ?
Sr2c Sr2c Sr2c 2_665 . 2_765 143.58(3) ?
Sr2c Sr2c Sr2c 2_665 . 3_565 60.00(3) ?
Sr2c Sr2c Sr2c 2_665 . 3_675 156.42(3) ?
Sr2c Sr2c Sr2b 2_665 . 7_445 71.75(2) ?
Sr2c Sr2c Sr2b 2_665 . 7_455 48.25(2) ?
Sr2c Sr2c Sr2b 2_665 . 7_555 168.25(3) ?
Sr2c Sr2c Sr2b 2_665 . 8_665 108.87(9) ?
Sr2c Sr2c Sr2b 2_665 . 9_565 131.91(3) ?
Sr2c Sr2c N3ac 2_665 . 13_554 43.66(10) ?
Sr2c Sr2c N1a 2_665 . 13_554 137.77(19) ?
Sr2c Sr2c N3bc 2_665 . 1_665 146.24(14) ?
Sr2c Sr2c C2a 2_665 . 4_674 127.37(18) ?
Sr2c Sr2c C2a 2_665 . 6_554 110.62(16) ?
Sr2c Sr2c Fe1c 2_665 . 10_564 79.26(3) ?
Sr2c Sr2c Fe1b 2_665 . 16_555 40.70(3) ?
Sr2c Sr2c N2c 2_665 . 10_564 95.98(16) ?
Sr2c Sr2c N1b 2_665 . 7_455 49.91(14) ?
Sr2c Sr2c C2c 2_665 . 10_564 99.27(15) ?
Sr2c Sr2c C2c 2_665 . 12_454 52.95(12) ?
Sr2c Sr2c C2b 2_665 . 16_565 40.86(13) ?
Sr2c Sr2c C2b 2_665 . 17_655 84.9(3) ?
Sr2c Sr2c C1a 2_665 . 4_665 160.8(3) ?
Sr2c Sr2c C1c 2_665 . 10_564 78.70(3) ?
Sr2c Sr2c C1b 2_665 . 16_555 34.63(14) ?
Sr2c Sr2c Sr2c 2_765 . 3_565 83.58(3) ?
Sr2c Sr2c Sr2c 2_765 . 3_675 60.00(2) ?
Sr2c Sr2c Sr2b 2_765 . 7_445 71.84(2) ?
Sr2c Sr2c Sr2b 2_765 . 7_455 168.16(2) ?
Sr2c Sr2c Sr2b 2_765 . 7_555 48.16(2) ?
Sr2c Sr2c Sr2b 2_765 . 8_665 107.55(9) ?
Sr2c Sr2c Sr2b 2_765 . 9_565 11.668(17) ?
Sr2c Sr2c N3ac 2_765 . 13_554 109.52(4) ?
Sr2c Sr2c N1a 2_765 . 13_554 49.81(14) ?
Sr2c Sr2c N3bc 2_765 . 1_665 43.57(10) ?
Sr2c Sr2c C2a 2_765 . 4_674 78.7(2) ?
Sr2c Sr2c C2a 2_765 . 6_554 51.5(2) ?
Sr2c Sr2c Fe1c 2_765 . 10_564 133.42(3) ?
Sr2c Sr2c Fe1b 2_765 . 16_555 110.50(3) ?
Sr2c Sr2c N2c 2_765 . 10_564 67.6(2) ?
Sr2c Sr2c N1b 2_765 . 7_455 107.30(6) ?
Sr2c Sr2c C2c 2_765 . 10_564 53.23(16) ?
Sr2c Sr2c C2c 2_765 . 12_454 143.37(16) ?
Sr2c Sr2c C2b 2_765 . 16_565 137.08(17) ?
Sr2c Sr2c C2b 2_765 . 17_655 71.4(3) ?
Sr2c Sr2c C1a 2_765 . 4_665 34.59(13) ?
Sr2c Sr2c C1c 2_765 . 10_564 136.25(6) ?
Sr2c Sr2c C1b 2_765 . 16_555 112.34(5) ?
Sr2c Sr2c Sr2c 3_565 . 3_675 143.58(4) ?
Sr2c Sr2c Sr2b 3_565 . 7_445 11.75(2) ?
Sr2c Sr2c Sr2b 3_565 . 7_455 108.25(3) ?
Sr2c Sr2c Sr2b 3_565 . 7_555 131.75(3) ?
Sr2c Sr2c Sr2b 3_565 . 8_665 168.87(10) ?
Sr2c Sr2c Sr2b 3_565 . 9_565 71.91(3) ?
Sr2c Sr2c N3ac 3_565 . 13_554 43.66(10) ?
Sr2c Sr2c N1a 3_565 . 13_554 107.34(6) ?
Sr2c Sr2c N3bc 3_565 . 1_665 109.55(5) ?
Sr2c Sr2c C2a 3_565 . 4_674 136.96(15) ?
Sr2c Sr2c C2a 3_565 . 6_554 71.48(18) ?
Sr2c Sr2c Fe1c 3_565 . 10_564 133.69(3) ?
Sr2c Sr2c Fe1b 3_565 . 16_555 40.70(3) ?
Sr2c Sr2c N2c 3_565 . 10_564 67.62(14) ?
Sr2c Sr2c N1b 3_565 . 7_455 49.91(14) ?
Sr2c Sr2c C2c 3_565 . 10_564 52.87(12) ?
Sr2c Sr2c C2c 3_565 . 12_454 99.33(15) ?
Sr2c Sr2c C2b 3_565 . 16_565 78.60(13) ?
Sr2c Sr2c C2b 3_565 . 17_655 52.20(16) ?
Sr2c Sr2c C1a 3_565 . 4_665 112.35(5) ?
Sr2c Sr2c C1c 3_565 . 10_564 136.53(7) ?
Sr2c Sr2c C1b 3_565 . 16_555 34.63(14) ?
Sr2c Sr2c Sr2b 3_675 . 7_445 131.84(3) ?
Sr2c Sr2c Sr2b 3_675 . 7_455 108.16(2) ?
Sr2c Sr2c Sr2b 3_675 . 7_555 11.84(2) ?
Sr2c Sr2c Sr2b 3_675 . 8_665 47.55(8) ?
Sr2c Sr2c Sr2b 3_675 . 9_565 71.67(3) ?
Sr2c Sr2c N3ac 3_675 . 13_554 146.12(14) ?
Sr2c Sr2c N1a 3_675 . 13_554 49.81(14) ?
Sr2c Sr2c N3bc 3_675 . 1_665 43.57(10) ?
Sr2c Sr2c C2a 3_675 . 4_674 41.09(15) ?
Sr2c Sr2c C2a 3_675 . 6_554 84.57(15) ?
Sr2c Sr2c Fe1c 3_675 . 10_564 78.97(2) ?
Sr2c Sr2c Fe1b 3_675 . 16_555 150.45(4) ?
Sr2c Sr2c N2c 3_675 . 10_564 96.00(14) ?
Sr2c Sr2c N1b 3_675 . 7_455 137.64(19) ?
Sr2c Sr2c C2c 3_675 . 10_564 99.69(14) ?
Sr2c Sr2c C2c 3_675 . 12_454 109.76(13) ?
Sr2c Sr2c C2b 3_675 . 16_565 127.57(12) ?
Sr2c Sr2c C2b 3_675 . 17_655 110.1(2) ?
Sr2c Sr2c C1a 3_675 . 4_665 34.59(13) ?
Sr2c Sr2c C1c 3_675 . 10_564 78.41(2) ?
Sr2c Sr2c C1b 3_675 . 16_555 160.8(3) ?
Sr2b Sr2c Sr2b 7_445 . 7_455 120.00(2) ?
Sr2b Sr2c Sr2b 7_445 . 7_555 120.00(3) ?
Sr2b Sr2c Sr2b 7_445 . 8_665 179.39(9) ?
Sr2b Sr2c Sr2b 7_445 . 9_565 60.17(2) ?
Sr2b Sr2c N3ac 7_445 . 13_554 51.44(8) ?
Sr2b Sr2c N1a 7_445 . 13_554 98.79(4) ?
Sr2b Sr2c N3bc 7_445 . 1_665 99.88(3) ?
Sr2b Sr2c C2a 7_445 . 4_674 131.21(16) ?
Sr2b Sr2c C2a 7_445 . 6_554 64.46(19) ?
Sr2b Sr2c Fe1c 7_445 . 10_564 143.25(3) ?
Sr2b Sr2c Fe1b 7_445 . 16_555 49.22(2) ?
Sr2b Sr2c N2c 7_445 . 10_564 63.77(16) ?
Sr2b Sr2c N1b 7_445 . 7_455 56.30(11) ?
Sr2b Sr2c C2c 7_445 . 10_564 45.59(12) ?
Sr2b Sr2c C2c 7_445 . 12_454 108.63(16) ?
Sr2b Sr2c C2b 7_445 . 16_565 87.77(14) ?
Sr2b Sr2c C2b 7_445 . 17_655 49.36(16) ?
Sr2b Sr2c C1a 7_445 . 4_665 101.24(4) ?
Sr2b Sr2c C1c 7_445 . 10_564 147.35(9) ?
Sr2b Sr2c C1b 7_445 . 16_555 44.85(10) ?
Sr2b Sr2c Sr2b 7_455 . 7_555 120.00(2) ?
Sr2b Sr2c Sr2b 7_455 . 8_665 60.61(8) ?
Sr2b Sr2c Sr2b 7_455 . 9_565 179.83(2) ?
Sr2b Sr2c N3ac 7_455 . 13_554 80.21(3) ?
Sr2b Sr2c N1a 7_455 . 13_554 123.72(11) ?
Sr2b Sr2c N3bc 7_455 . 1_665 128.56(8) ?
Sr2b Sr2c C2a 7_455 . 4_674 92.1(2) ?
Sr2b Sr2c C2a 7_455 . 6_554 131.3(2) ?
Sr2b Sr2c Fe1c 7_455 . 10_564 36.92(2) ?
Sr2b Sr2c Fe1b 7_455 . 16_555 79.74(2) ?
Sr2b Sr2c N2c 7_455 . 10_564 116.2(2) ?
Sr2b Sr2c N1b 7_455 . 7_455 81.29(3) ?
Sr2b Sr2c C2c 7_455 . 10_564 134.16(16) ?
Sr2b Sr2c C2c 7_455 . 12_454 36.83(17) ?
Sr2b Sr2c C2b 7_455 . 16_565 48.77(17) ?
Sr2b Sr2c C2b 7_455 . 17_655 115.5(3) ?
Sr2b Sr2c C1a 7_455 . 4_665 135.09(10) ?
Sr2b Sr2c C1c 7_455 . 10_564 32.85(9) ?
Sr2b Sr2c C1b 7_455 . 16_555 78.85(3) ?
Sr2b Sr2c Sr2b 7_555 . 8_665 59.39(8) ?
Sr2b Sr2c Sr2b 7_555 . 9_565 59.83(2) ?
Sr2b Sr2c N3ac 7_555 . 13_554 142.50(13) ?
Sr2b Sr2c N1a 7_555 . 13_554 44.93(17) ?
Sr2b Sr2c N3bc 7_555 . 1_665 37.35(12) ?
Sr2b Sr2c C2a 7_555 . 4_674 46.00(17) ?
Sr2b Sr2c C2a 7_555 . 6_554 76.78(15) ?
Sr2b Sr2c Fe1c 7_555 . 10_564 89.900(18) ?
Sr2b Sr2c Fe1b 7_555 . 16_555 146.24(4) ?
Sr2b Sr2c N2c 7_555 . 10_564 89.99(15) ?
Sr2b Sr2c N1b 7_555 . 7_455 134.92(17) ?
Sr2b Sr2c C2c 7_555 . 10_564 90.18(14) ?
Sr2b Sr2c C2c 7_555 . 12_454 118.75(12) ?
Sr2b Sr2c C2b 7_555 . 16_565 134.27(12) ?
Sr2b Sr2c C2b 7_555 . 17_655 102.7(3) ?
Sr2b Sr2c C1a 7_555 . 4_665 25.42(19) ?
Sr2b Sr2c C1c 7_555 . 10_564 89.895(18) ?
Sr2b Sr2c C1b 7_555 . 16_555 154.5(2) ?
Sr2b Sr2c Sr2b 8_665 . 9_565 119.22(9) ?
Sr2b Sr2c N3ac 8_665 . 13_554 128.99(12) ?
Sr2b Sr2c N1a 8_665 . 13_554 80.76(8) ?
Sr2b Sr2c N3bc 8_665 . 1_665 79.61(8) ?
Sr2b Sr2c C2a 8_665 . 4_674 48.45(17) ?
Sr2b Sr2c C2a 8_665 . 6_554 115.2(2) ?
Sr2b Sr2c Fe1c 8_665 . 10_564 37.23(7) ?
Sr2b Sr2c Fe1b 8_665 . 16_555 131.25(9) ?
Sr2b Sr2c N2c 8_665 . 10_564 116.06(17) ?
Sr2b Sr2c N1b 8_665 . 7_455 124.06(14) ?
Sr2b Sr2c C2c 8_665 . 10_564 134.07(14) ?
Sr2b Sr2c C2c 8_665 . 12_454 71.85(18) ?
Sr2b Sr2c C2b 8_665 . 16_565 92.71(16) ?
Sr2b Sr2c C2b 8_665 . 17_655 130.54(18) ?
Sr2b Sr2c C1a 8_665 . 4_665 78.18(8) ?
Sr2b Sr2c C1c 8_665 . 10_564 33.20(11) ?
Sr2b Sr2c C1b 8_665 . 16_555 135.69(14) ?
Sr2b Sr2c N3ac 9_565 . 13_554 99.93(3) ?
Sr2b Sr2c N1a 9_565 . 13_554 56.18(11) ?
Sr2b Sr2c N3bc 9_565 . 1_665 51.32(8) ?
Sr2b Sr2c C2a 9_565 . 4_674 87.8(2) ?
Sr2b Sr2c C2a 9_565 . 6_554 48.7(2) ?
Sr2b Sr2c Fe1c 9_565 . 10_564 142.95(3) ?
Sr2b Sr2c Fe1b 9_565 . 16_555 100.41(3) ?
Sr2b Sr2c N2c 9_565 . 10_564 63.8(2) ?
Sr2b Sr2c N1b 9_565 . 7_455 98.83(4) ?
Sr2b Sr2c C2c 9_565 . 10_564 45.93(16) ?
Sr2b Sr2c C2c 9_565 . 12_454 143.19(18) ?
Sr2b Sr2c C2b 9_565 . 16_565 131.33(17) ?
Sr2b Sr2c C2b 9_565 . 17_655 64.6(3) ?
Sr2b Sr2c C1a 9_565 . 4_665 44.76(10) ?
Sr2b Sr2c C1c 9_565 . 10_564 147.00(9) ?
Sr2b Sr2c C1b 9_565 . 16_555 101.31(3) ?
N3ac Sr2c N1a 13_554 . 13_554 97.7(2) ?
N3ac Sr2c N3bc 13_554 . 1_665 105.15(18) ?
N3ac Sr2c C2a 13_554 . 4_674 171.0(2) ?
N3ac Sr2c C2a 13_554 . 6_554 115.1(2) ?
N3ac Sr2c Fe1c 13_554 . 10_564 116.95(4) ?
N3ac Sr2c Fe1b 13_554 . 16_555 62.25(15) ?
N3ac Sr2c N2c 13_554 . 10_564 109.83(18) ?
N3ac Sr2c N1b 13_554 . 7_455 8.6(2) ?
N3ac Sr2c C2c 13_554 . 10_564 96.41(15) ?
N3ac Sr2c C2c 13_554 . 12_454 96.50(15) ?
N3ac Sr2c C2b 13_554 . 16_565 83.15(17) ?
N3ac Sr2c C2b 13_554 . 17_655 94.2(2) ?
N3ac Sr2c C1a 13_554 . 4_665 117.9(3) ?
N3ac Sr2c C1c 13_554 . 10_564 97.15(15) ?
N3ac Sr2c C1b 13_554 . 16_555 15.2(3) ?
N1a Sr2c N3bc 13_554 . 1_665 8.6(2) ?
N1a Sr2c C2a 13_554 . 4_674 90.4(2) ?
N1a Sr2c C2a 13_554 . 6_554 100.8(3) ?
N1a Sr2c Fe1c 13_554 . 10_564 117.92(3) ?
N1a Sr2c Fe1b 13_554 . 16_555 147.92(5) ?
N1a Sr2c N2c 13_554 . 10_564 117.0(3) ?
N1a Sr2c N1b 13_554 . 7_455 90.0(2) ?
N1a Sr2c C2c 13_554 . 10_564 102.1(2) ?
N1a Sr2c C2c 13_554 . 12_454 152.33(17) ?
N1a Sr2c C2b 13_554 . 16_565 172.28(18) ?
N1a Sr2c C2b 13_554 . 17_655 120.7(3) ?
N1a Sr2c C1a 13_554 . 4_665 23.7(3) ?
N1a Sr2c C1c 13_554 . 10_564 93.74(17) ?
N1a Sr2c C1b 13_554 . 16_555 111.2(3) ?
N3bc Sr2c C2a 1_665 . 4_674 83.3(2) ?
N3bc Sr2c C2a 1_665 . 6_554 93.5(2) ?
N3bc Sr2c Fe1c 1_665 . 10_564 116.67(3) ?
N3bc Sr2c Fe1b 1_665 . 16_555 148.66(4) ?
N3bc Sr2c N2c 1_665 . 10_564 109.7(2) ?
N3bc Sr2c N1b 1_665 . 7_455 97.7(2) ?
N3bc Sr2c C2c 1_665 . 10_564 96.67(19) ?
N3bc Sr2c C2c 1_665 . 12_454 151.08(15) ?
N3bc Sr2c C2b 1_665 . 16_565 171.10(15) ?
N3bc Sr2c C2b 1_665 . 17_655 115.0(3) ?
N3bc Sr2c C1a 1_665 . 4_665 15.1(3) ?
N3bc Sr2c C1c 1_665 . 10_564 96.96(14) ?
N3bc Sr2c C1b 1_665 . 16_555 118.0(3) ?
C2a Sr2c C2a 4_674 . 6_554 66.8(3) ?
C2a Sr2c Fe1c 4_674 . 10_564 55.1(2) ?
C2a Sr2c Fe1b 4_674 . 16_555 112.02(14) ?
C2a Sr2c N2c 4_674 . 10_564 69.4(2) ?
C2a Sr2c N1b 4_674 . 7_455 172.2(2) ?
C2a Sr2c C2c 4_674 . 10_564 85.6(2) ?
C2a Sr2c C2c 4_674 . 12_454 74.5(2) ?
C2a Sr2c C2b 4_674 . 16_565 88.3(2) ?
C2a Sr2c C2b 4_674 . 17_655 84.9(2) ?
C2a Sr2c C1a 4_674 . 4_665 70.9(3) ?
C2a Sr2c C1c 4_674 . 10_564 78.3(2) ?
C2a Sr2c C1b 4_674 . 16_555 158.1(3) ?
C2a Sr2c Fe1c 6_554 . 10_564 107.3(2) ?
C2a Sr2c Fe1b 6_554 . 16_555 70.04(16) ?
C2a Sr2c N2c 6_554 . 10_564 16.3(3) ?
C2a Sr2c N1b 6_554 . 7_455 120.7(2) ?
C2a Sr2c C2c 6_554 . 10_564 18.9(2) ?
C2a Sr2c C2c 6_554 . 12_454 94.5(3) ?
C2a Sr2c C2b 6_554 . 16_565 85.7(3) ?
C2a Sr2c C2b 6_554 . 17_655 26.0(3) ?
C2a Sr2c C1a 6_554 . 4_665 80.6(3) ?
C2a Sr2c C1c 6_554 . 10_564 142.0(3) ?
C2a Sr2c C1b 6_554 . 16_555 104.5(3) ?
Fe1c Sr2c Fe1b 10_564 . 16_555 94.03(3) ?
Fe1c Sr2c N2c 10_564 . 10_564 98.2(2) ?
Fe1c Sr2c N1b 10_564 . 7_455 118.16(4) ?
Fe1c Sr2c C2c 10_564 . 10_564 121.28(15) ?
Fe1c Sr2c C2c 10_564 . 12_454 34.62(16) ?
Fe1c Sr2c C2b 10_564 . 16_565 55.49(13) ?
Fe1c Sr2c C2b 10_564 . 17_655 107.0(2) ?
Fe1c Sr2c C1a 10_564 . 4_665 113.01(9) ?
Fe1c Sr2c C1c 10_564 . 10_564 36.3(2) ?
Fe1c Sr2c C1b 10_564 . 16_555 113.31(9) ?
Fe1b Sr2c N2c 16_555 . 10_564 56.25(15) ?
Fe1b Sr2c N1b 16_555 . 7_455 70.87(19) ?
Fe1b Sr2c C2c 16_555 . 10_564 59.36(15) ?
Fe1b Sr2c C2c 16_555 . 12_454 59.42(16) ?
Fe1b Sr2c C2b 16_555 . 16_565 38.57(14) ?
Fe1b Sr2c C2b 16_555 . 17_655 44.2(3) ?
Fe1b Sr2c C1a 16_555 . 4_665 145.06(13) ?
Fe1b Sr2c C1c 16_555 . 10_564 112.53(10) ?
Fe1b Sr2c C1b 16_555 . 16_555 47.1(3) ?
N2c Sr2c N1b 10_564 . 7_455 117.1(2) ?
N2c Sr2c C2c 10_564 . 10_564 23.0(2) ?
N2c Sr2c C2c 10_564 . 12_454 79.7(3) ?
N2c Sr2c C2b 10_564 . 16_565 69.5(3) ?
N2c Sr2c C2b 10_564 . 17_655 15.6(2) ?
N2c Sr2c C1a 10_564 . 4_665 96.6(3) ?
N2c Sr2c C1c 10_564 . 10_564 134.5(3) ?
N2c Sr2c C1b 10_564 . 16_555 96.7(3) ?
N1b Sr2c C2c 7_455 . 10_564 101.86(16) ?
N1b Sr2c C2c 7_455 . 12_454 101.95(17) ?
N1b Sr2c C2b 7_455 . 16_565 90.3(2) ?
N1b Sr2c C2b 7_455 . 17_655 101.5(2) ?
N1b Sr2c C1a 7_455 . 4_665 111.2(3) ?
N1b Sr2c C1c 7_455 . 10_564 93.90(17) ?
N1b Sr2c C1b 7_455 . 16_555 23.8(3) ?
C2c Sr2c C2c 10_564 . 12_454 99.8(2) ?
C2c Sr2c C2b 10_564 . 16_565 85.4(2) ?
C2c Sr2c C2b 10_564 . 17_655 18.6(3) ?
C2c Sr2c C1a 10_564 . 4_665 87.0(2) ?
C2c Sr2c C1c 10_564 . 10_564 157.5(3) ?
C2c Sr2c C1b 10_564 . 16_555 86.7(2) ?
C2c Sr2c C2b 12_454 . 16_565 20.9(2) ?
C2c Sr2c C2b 12_454 . 17_655 81.6(3) ?
C2c Sr2c C1a 12_454 . 4_665 144.1(2) ?
C2c Sr2c C1c 12_454 . 10_564 60.9(3) ?
C2c Sr2c C1b 12_454 . 16_555 86.7(2) ?
C2b Sr2c C2b 16_565 . 17_655 66.8(3) ?
C2b Sr2c C1a 16_565 . 4_665 158.3(3) ?
C2b Sr2c C1c 16_565 . 10_564 78.6(2) ?
C2b Sr2c C1b 16_565 . 16_555 70.7(3) ?
C2b Sr2c C1a 17_655 . 4_665 104.3(4) ?
C2b Sr2c C1c 17_655 . 10_564 141.8(3) ?
C2b Sr2c C1b 17_655 . 16_555 81.3(3) ?
C1a Sr2c C1c 4_665 . 10_564 102.24(13) ?
C1a Sr2c C1b 4_665 . 16_555 129.0(3) ?
C1c Sr2c C1b 10_564 . 16_555 102.49(13) ?
Sr1 Sr2b Sr1 7_554 . 8_664 64.58(3) ?
Sr1 Sr2b Sr1 7_554 . 9_464 59.04(2) ?
Sr1 Sr2b Sr1 7_554 . 18_564 135.75(3) ?
Sr1 Sr2b Sr2a 7_554 . 7_444 127.37(3) ?
Sr1 Sr2b Sr2a 7_554 . 7_454 83.17(3) ?
Sr1 Sr2b Sr2a 7_554 . 7_554 60.786(19) ?
Sr1 Sr2b Sr2a 7_554 . 8_664 52.47(7) ?
Sr1 Sr2b Sr2a 7_554 . 9_564 96.72(3) ?
Sr1 Sr2b Fe1a 7_554 . 16_555 152.97(4) ?
Sr1 Sr2b Sr2c 7_554 . 13_444 119.21(3) ?
Sr1 Sr2b Sr2c 7_554 . 13_544 96.83(3) ?
Sr1 Sr2b Sr2c 7_554 . 13_554 52.63(2) ?
Sr1 Sr2b Sr2c 7_554 . 14_654 127.32(3) ?
Sr1 Sr2b Sr2c 7_554 . 15_564 82.78(7) ?
Sr1 Sr2b Sr2b 7_554 . 2_665 113.11(3) ?
Sr1 Sr2b Sr2b 7_554 . 2_765 89.24(3) ?
Sr1 Sr2b Sr2b 7_554 . 3_565 129.61(3) ?
Sr1 Sr2b Sr2b 7_554 . 3_675 55.692(19) ?
Sr1 Sr2b N1a 7_554 . 7_454 86.00(18) ?
Sr1 Sr2b N3bc 7_554 . 13_554 94.36(14) ?
Sr1 Sr2b C2a 7_554 . 16_564 131.72(17) ?
Sr1 Sr2b C2a 7_554 . 17_654 160.5(3) ?
Sr1 Sr2b Fe1c 7_554 . 4_664 94.41(3) ?
Sr1 Sr2b Fe1b 7_554 . 10_564 84.51(3) ?
Sr1 Sr2b N3ab 7_554 . 1_665 45.73(9) ?
Sr1 Sr2b N1c 7_554 . 13_554 40.64(10) ?
Sr1 Sr2b N2b 7_554 . 10_564 150.71(16) ?
Sr1 Sr2b C2c 7_554 . 4_674 89.27(13) ?
Sr1 Sr2b C2c 7_554 . 6_554 136.10(17) ?
Sr1 Sr2b C2b 7_554 . 10_564 142.40(16) ?
Sr1 Sr2b C2b 7_554 . 12_454 114.66(18) ?
Sr1 Sr2b C1a 7_554 . 16_555 109.0(3) ?
Sr1 Sr2b C1c 7_554 . 4_664 56.3(2) ?
Sr1 Sr2b C1b 7_554 . 10_564 53.81(18) ?
Sr1 Sr2b Sr1 8_664 . 9_464 68.94(3) ?
Sr1 Sr2b Sr1 8_664 . 18_564 154.92(4) ?
Sr1 Sr2b Sr2a 8_664 . 7_444 62.90(2) ?
Sr1 Sr2b Sr2a 8_664 . 7_454 119.17(3) ?
Sr1 Sr2b Sr2a 8_664 . 7_554 88.18(3) ?
Sr1 Sr2b Sr2a 8_664 . 8_664 116.89(8) ?
Sr1 Sr2b Sr2a 8_664 . 9_564 60.88(3) ?
Sr1 Sr2b Fe1a 8_664 . 16_555 106.40(4) ?
Sr1 Sr2b Sr2c 8_664 . 13_444 91.82(2) ?
Sr1 Sr2b Sr2c 8_664 . 13_544 60.83(3) ?
Sr1 Sr2b Sr2c 8_664 . 13_554 117.10(3) ?
Sr1 Sr2b Sr2c 8_664 . 14_654 62.84(3) ?
Sr1 Sr2b Sr2c 8_664 . 15_564 119.34(8) ?
Sr1 Sr2b Sr2b 8_664 . 2_665 98.16(3) ?
Sr1 Sr2b Sr2b 8_664 . 2_765 64.74(3) ?
Sr1 Sr2b Sr2b 8_664 . 3_565 67.36(2) ?
Sr1 Sr2b Sr2b 8_664 . 3_675 94.62(3) ?
Sr1 Sr2b N1a 8_664 . 7_454 48.33(13) ?
Sr1 Sr2b N3bc 8_664 . 13_554 54.69(11) ?
Sr1 Sr2b C2a 8_664 . 16_564 137.47(12) ?
Sr1 Sr2b C2a 8_664 . 17_654 107.1(2) ?
Sr1 Sr2b Fe1c 8_664 . 4_664 103.21(4) ?
Sr1 Sr2b Fe1b 8_664 . 10_564 145.41(4) ?
Sr1 Sr2b N3ab 8_664 . 1_665 51.21(11) ?
Sr1 Sr2b N1c 8_664 . 13_554 44.93(13) ?
Sr1 Sr2b N2b 8_664 . 10_564 116.3(2) ?
Sr1 Sr2b C2c 8_664 . 4_674 134.10(17) ?
Sr1 Sr2b C2c 8_664 . 6_554 105.8(2) ?
Sr1 Sr2b C2b 8_664 . 10_564 93.27(15) ?
Sr1 Sr2b C2b 8_664 . 12_454 149.73(13) ?
Sr1 Sr2b C1a 8_664 . 16_555 66.8(2) ?
Sr1 Sr2b C1c 8_664 . 4_664 63.2(2) ?
Sr1 Sr2b C1b 8_664 . 10_564 109.2(2) ?
Sr1 Sr2b Sr1 9_464 . 18_564 130.94(4) ?
Sr1 Sr2b Sr2a 9_464 . 7_444 98.23(2) ?
Sr1 Sr2b Sr2a 9_464 . 7_454 50.23(2) ?
Sr1 Sr2b Sr2a 9_464 . 7_554 119.77(2) ?
Sr1 Sr2b Sr2a 9_464 . 8_664 82.18(8) ?
Sr1 Sr2b Sr2a 9_464 . 9_564 129.81(3) ?
Sr1 Sr2b Fe1a 9_464 . 16_555 93.98(4) ?
Sr1 Sr2b Sr2c 9_464 . 13_444 60.23(2) ?
Sr1 Sr2b Sr2c 9_464 . 13_544 129.77(3) ?
Sr1 Sr2b Sr2c 9_464 . 13_554 81.77(2) ?
Sr1 Sr2b Sr2c 9_464 . 14_654 98.34(2) ?
Sr1 Sr2b Sr2c 9_464 . 15_564 50.40(7) ?
Sr1 Sr2b Sr2b 9_464 . 2_665 54.68(2) ?
Sr1 Sr2b Sr2b 9_464 . 2_765 131.91(3) ?
Sr1 Sr2b Sr2b 9_464 . 3_565 90.38(2) ?
Sr1 Sr2b Sr2b 9_464 . 3_675 113.16(3) ?
Sr1 Sr2b N1a 9_464 . 7_454 42.19(9) ?
Sr1 Sr2b N3bc 9_464 . 13_554 46.92(9) ?
Sr1 Sr2b C2a 9_464 . 16_564 87.20(16) ?
Sr1 Sr2b C2a 9_464 . 17_654 136.7(2) ?
Sr1 Sr2b Fe1c 9_464 . 4_664 153.36(4) ?
Sr1 Sr2b Fe1b 9_464 . 10_564 82.31(3) ?
Sr1 Sr2b N3ab 9_464 . 1_665 96.12(14) ?
Sr1 Sr2b N1c 9_464 . 13_554 87.84(18) ?
Sr1 Sr2b N2b 9_464 . 10_564 150.23(15) ?
Sr1 Sr2b C2c 9_464 . 4_674 130.09(17) ?
Sr1 Sr2b C2c 9_464 . 6_554 161.50(16) ?
Sr1 Sr2b C2b 9_464 . 10_564 143.25(12) ?
Sr1 Sr2b C2b 9_464 . 12_454 84.71(16) ?
Sr1 Sr2b C1a 9_464 . 16_555 57.0(2) ?
Sr1 Sr2b C1c 9_464 . 4_664 110.6(3) ?
Sr1 Sr2b C1b 9_464 . 10_564 52.06(17) ?
Sr1 Sr2b Sr2a 18_564 . 7_444 95.90(2) ?
Sr1 Sr2b Sr2a 18_564 . 7_454 82.21(3) ?
Sr1 Sr2b Sr2a 18_564 . 7_554 91.87(2) ?
Sr1 Sr2b Sr2a 18_564 . 8_664 84.16(7) ?
Sr1 Sr2b Sr2a 18_564 . 9_564 97.78(3) ?
Sr1 Sr2b Fe1a 18_564 . 16_555 62.09(4) ?
Sr1 Sr2b Sr2c 18_564 . 13_444 88.13(2) ?
Sr1 Sr2b Sr2c 18_564 . 13_544 97.79(3) ?
Sr1 Sr2b Sr2c 18_564 . 13_554 84.10(2) ?
Sr1 Sr2b Sr2c 18_564 . 14_654 95.91(3) ?
Sr1 Sr2b Sr2c 18_564 . 15_564 82.19(7) ?
Sr1 Sr2b Sr2b 18_564 . 2_665 86.56(2) ?
Sr1 Sr2b Sr2b 18_564 . 2_765 97.14(3) ?
Sr1 Sr2b Sr2b 18_564 . 3_565 94.64(2) ?
Sr1 Sr2b Sr2b 18_564 . 3_675 90.22(2) ?
Sr1 Sr2b N1a 18_564 . 7_454 132.14(19) ?
Sr1 Sr2b N3bc 18_564 . 13_554 123.65(14) ?
Sr1 Sr2b C2a 18_564 . 16_564 46.69(15) ?
Sr1 Sr2b C2a 18_564 . 17_654 48.5(2) ?
Sr1 Sr2b Fe1c 18_564 . 4_664 65.67(4) ?
Sr1 Sr2b Fe1b 18_564 . 10_564 59.65(4) ?
Sr1 Sr2b N3ab 18_564 . 1_665 127.17(15) ?
Sr1 Sr2b N1c 18_564 . 13_554 135.67(19) ?
Sr1 Sr2b N2b 18_564 . 10_564 38.6(2) ?
Sr1 Sr2b C2c 18_564 . 4_674 49.95(13) ?
Sr1 Sr2b C2c 18_564 . 6_554 50.2(2) ?
Sr1 Sr2b C2b 18_564 . 10_564 61.66(15) ?
Sr1 Sr2b C2b 18_564 . 12_454 46.30(16) ?
Sr1 Sr2b C1a 18_564 . 16_555 108.7(3) ?
Sr1 Sr2b C1c 18_564 . 4_664 112.2(3) ?
Sr1 Sr2b C1b 18_564 . 10_564 95.9(2) ?
Sr2a Sr2b Sr2a 7_444 . 7_454 120.00(2) ?
Sr2a Sr2b Sr2a 7_444 . 7_554 120.00(3) ?
Sr2a Sr2b Sr2a 7_444 . 8_664 179.39(9) ?
Sr2a Sr2b Sr2a 7_444 . 9_564 60.17(2) ?
Sr2a Sr2b Fe1a 7_444 . 16_555 49.22(2) ?
Sr2a Sr2b Sr2c 7_444 . 13_444 60.000(19) ?
Sr2a Sr2b Sr2c 7_444 . 13_544 60.000(19) ?
Sr2a Sr2b Sr2c 7_444 . 13_554 180 ?
Sr2a Sr2b Sr2c 7_444 . 14_654 0.17(2) ?
Sr2a Sr2b Sr2c 7_444 . 15_564 120.61(6) ?
Sr2a Sr2b Sr2b 7_444 . 2_665 71.75(2) ?
Sr2a Sr2b Sr2b 7_444 . 2_765 71.84(2) ?
Sr2a Sr2b Sr2b 7_444 . 3_565 11.75(2) ?
Sr2a Sr2b Sr2b 7_444 . 3_675 131.84(3) ?
Sr2a Sr2b N1a 7_444 . 7_454 56.30(11) ?
Sr2a Sr2b N3bc 7_444 . 13_554 51.44(8) ?
Sr2a Sr2b C2a 7_444 . 16_564 87.77(14) ?
Sr2a Sr2b C2a 7_444 . 17_654 49.36(16) ?
Sr2a Sr2b Fe1c 7_444 . 4_664 100.35(3) ?
Sr2a Sr2b Fe1b 7_444 . 10_564 143.25(3) ?
Sr2a Sr2b N3ab 7_444 . 1_665 99.88(3) ?
Sr2a Sr2b N1c 7_444 . 13_554 98.79(4) ?
Sr2a Sr2b N2b 7_444 . 10_564 63.77(16) ?
Sr2a Sr2b C2c 7_444 . 4_674 131.21(16) ?
Sr2a Sr2b C2c 7_444 . 6_554 64.46(19) ?
Sr2a Sr2b C2b 7_444 . 10_564 45.59(12) ?
Sr2a Sr2b C2b 7_444 . 12_454 108.63(16) ?
Sr2a Sr2b C1a 7_444 . 16_555 44.85(9) ?
Sr2a Sr2b C1c 7_444 . 4_664 101.24(4) ?
Sr2a Sr2b C1b 7_444 . 10_564 147.35(9) ?
Sr2a Sr2b Sr2a 7_454 . 7_554 120.00(2) ?
Sr2a Sr2b Sr2a 7_454 . 8_664 60.61(8) ?
Sr2a Sr2b Sr2a 7_454 . 9_564 179.83(2) ?
Sr2a Sr2b Fe1a 7_454 . 16_555 79.74(2) ?
Sr2a Sr2b Sr2c 7_454 . 13_444 60.000(19) ?
Sr2a Sr2b Sr2c 7_454 . 13_544 180 ?
Sr2a Sr2b Sr2c 7_454 . 13_554 60.000(19) ?
Sr2a Sr2b Sr2c 7_454 . 14_654 120.17(3) ?
Sr2a Sr2b Sr2c 7_454 . 15_564 0.61(5) ?
Sr2a Sr2b Sr2b 7_454 . 2_665 48.25(2) ?
Sr2a Sr2b Sr2b 7_454 . 2_765 168.16(2) ?
Sr2a Sr2b Sr2b 7_454 . 3_565 108.25(3) ?
Sr2a Sr2b Sr2b 7_454 . 3_675 108.16(2) ?
Sr2a Sr2b N1a 7_454 . 7_454 81.29(3) ?
Sr2a Sr2b N3bc 7_454 . 13_554 80.21(3) ?
Sr2a Sr2b C2a 7_454 . 16_564 48.77(17) ?
Sr2a Sr2b C2a 7_454 . 17_654 115.5(3) ?
Sr2a Sr2b Fe1c 7_454 . 4_664 130.76(3) ?
Sr2a Sr2b Fe1b 7_454 . 10_564 36.92(2) ?
Sr2a Sr2b N3ab 7_454 . 1_665 128.56(8) ?
Sr2a Sr2b N1c 7_454 . 13_554 123.72(11) ?
Sr2a Sr2b N2b 7_454 . 10_564 116.2(2) ?
Sr2a Sr2b C2c 7_454 . 4_674 92.1(2) ?
Sr2a Sr2b C2c 7_454 . 6_554 131.3(2) ?
Sr2a Sr2b C2b 7_454 . 10_564 134.16(16) ?
Sr2a Sr2b C2b 7_454 . 12_454 36.83(17) ?
Sr2a Sr2b C1a 7_454 . 16_555 78.85(3) ?
Sr2a Sr2b C1c 7_454 . 4_664 135.09(10) ?
Sr2a Sr2b C1b 7_454 . 10_564 32.85(9) ?
Sr2a Sr2b Sr2a 7_554 . 8_664 59.39(8) ?
Sr2a Sr2b Sr2a 7_554 . 9_564 59.83(2) ?
Sr2a Sr2b Fe1a 7_554 . 16_555 146.24(4) ?
Sr2a Sr2b Sr2c 7_554 . 13_444 180 ?
Sr2a Sr2b Sr2c 7_554 . 13_544 60.000(19) ?
Sr2a Sr2b Sr2c 7_554 . 13_554 60.000(19) ?
Sr2a Sr2b Sr2c 7_554 . 14_654 119.83(3) ?
Sr2a Sr2b Sr2c 7_554 . 15_564 119.39(6) ?
Sr2a Sr2b Sr2b 7_554 . 2_665 168.25(3) ?
Sr2a Sr2b Sr2b 7_554 . 2_765 48.16(2) ?
Sr2a Sr2b Sr2b 7_554 . 3_565 131.75(3) ?
Sr2a Sr2b Sr2b 7_554 . 3_675 11.84(2) ?
Sr2a Sr2b N1a 7_554 . 7_454 134.92(17) ?
Sr2a Sr2b N3bc 7_554 . 13_554 142.50(13) ?
Sr2a Sr2b C2a 7_554 . 16_564 134.27(12) ?
Sr2a Sr2b C2a 7_554 . 17_654 102.7(3) ?
Sr2a Sr2b Fe1c 7_554 . 4_664 33.62(3) ?
Sr2a Sr2b Fe1b 7_554 . 10_564 89.900(18) ?
Sr2a Sr2b N3ab 7_554 . 1_665 37.35(12) ?
Sr2a Sr2b N1c 7_554 . 13_554 44.93(17) ?
Sr2a Sr2b N2b 7_554 . 10_564 89.99(15) ?
Sr2a Sr2b C2c 7_554 . 4_674 46.00(17) ?
Sr2a Sr2b C2c 7_554 . 6_554 76.78(15) ?
Sr2a Sr2b C2b 7_554 . 10_564 90.18(14) ?
Sr2a Sr2b C2b 7_554 . 12_454 118.75(12) ?
Sr2a Sr2b C1a 7_554 . 16_555 154.5(2) ?
Sr2a Sr2b C1c 7_554 . 4_664 25.42(19) ?
Sr2a Sr2b C1b 7_554 . 10_564 89.895(18) ?
Sr2a Sr2b Sr2a 8_664 . 9_564 119.22(9) ?
Sr2a Sr2b Fe1a 8_664 . 16_555 131.25(9) ?
Sr2a Sr2b Sr2c 8_664 . 13_444 120.61(9) ?
Sr2a Sr2b Sr2c 8_664 . 13_544 119.39(9) ?
Sr2a Sr2b Sr2c 8_664 . 13_554 0.61(8) ?
Sr2a Sr2b Sr2c 8_664 . 14_654 179.22(10) ?
Sr2a Sr2b Sr2c 8_664 . 15_564 60.00(9) ?
Sr2a Sr2b Sr2b 8_664 . 2_665 108.87(9) ?
Sr2a Sr2b Sr2b 8_664 . 2_765 107.55(9) ?
Sr2a Sr2b Sr2b 8_664 . 3_565 168.87(10) ?
Sr2a Sr2b Sr2b 8_664 . 3_675 47.55(8) ?
Sr2a Sr2b N1a 8_664 . 7_454 124.06(14) ?
Sr2a Sr2b N3bc 8_664 . 13_554 128.99(12) ?
Sr2a Sr2b C2a 8_664 . 16_564 92.71(16) ?
Sr2a Sr2b C2a 8_664 . 17_654 130.54(18) ?
Sr2a Sr2b Fe1c 8_664 . 4_664 79.11(8) ?
Sr2a Sr2b Fe1b 8_664 . 10_564 37.23(7) ?
Sr2a Sr2b N3ab 8_664 . 1_665 79.61(8) ?
Sr2a Sr2b N1c 8_664 . 13_554 80.76(8) ?
Sr2a Sr2b N2b 8_664 . 10_564 116.05(17) ?
Sr2a Sr2b C2c 8_664 . 4_674 48.45(17) ?
Sr2a Sr2b C2c 8_664 . 6_554 115.2(2) ?
Sr2a Sr2b C2b 8_664 . 10_564 134.06(14) ?
Sr2a Sr2b C2b 8_664 . 12_454 71.85(18) ?
Sr2a Sr2b C1a 8_664 . 16_555 135.70(14) ?
Sr2a Sr2b C1c 8_664 . 4_664 78.18(8) ?
Sr2a Sr2b C1b 8_664 . 10_564 33.21(11) ?
Sr2a Sr2b Fe1a 9_564 . 16_555 100.41(3) ?
Sr2a Sr2b Sr2c 9_564 . 13_444 120.17(2) ?
Sr2a Sr2b Sr2c 9_564 . 13_544 0.168(14) ?
Sr2a Sr2b Sr2c 9_564 . 13_554 119.83(3) ?
Sr2a Sr2b Sr2c 9_564 . 14_654 60.00(3) ?
Sr2a Sr2b Sr2c 9_564 . 15_564 179.22(6) ?
Sr2a Sr2b Sr2b 9_564 . 2_665 131.91(3) ?
Sr2a Sr2b Sr2b 9_564 . 2_765 11.668(17) ?
Sr2a Sr2b Sr2b 9_564 . 3_565 71.91(3) ?
Sr2a Sr2b Sr2b 9_564 . 3_675 71.67(3) ?
Sr2a Sr2b N1a 9_564 . 7_454 98.83(4) ?
Sr2a Sr2b N3bc 9_564 . 13_554 99.93(3) ?
Sr2a Sr2b C2a 9_564 . 16_564 131.33(17) ?
Sr2a Sr2b C2a 9_564 . 17_654 64.6(3) ?
Sr2a Sr2b Fe1c 9_564 . 4_664 49.11(3) ?
Sr2a Sr2b Fe1b 9_564 . 10_564 142.95(3) ?
Sr2a Sr2b N3ab 9_564 . 1_665 51.32(8) ?
Sr2a Sr2b N1c 9_564 . 13_554 56.18(11) ?
Sr2a Sr2b N2b 9_564 . 10_564 63.8(2) ?
Sr2a Sr2b C2c 9_564 . 4_674 87.8(2) ?
Sr2a Sr2b C2c 9_564 . 6_554 48.7(2) ?
Sr2a Sr2b C2b 9_564 . 10_564 45.93(16) ?
Sr2a Sr2b C2b 9_564 . 12_454 143.19(18) ?
Sr2a Sr2b C1a 9_564 . 16_555 101.31(3) ?
Sr2a Sr2b C1c 9_564 . 4_664 44.76(10) ?
Sr2a Sr2b C1b 9_564 . 10_564 147.00(9) ?
Fe1a Sr2b Sr2c 16_555 . 13_444 33.76(3) ?
Fe1a Sr2b Sr2c 16_555 . 13_544 100.26(3) ?
Fe1a Sr2b Sr2c 16_555 . 13_554 130.78(4) ?
Fe1a Sr2b Sr2c 16_555 . 14_654 49.35(2) ?
Fe1a Sr2b Sr2c 16_555 . 15_564 80.27(6) ?
Fe1a Sr2b Sr2b 16_555 . 2_665 40.70(3) ?
Fe1a Sr2b Sr2b 16_555 . 2_765 110.50(3) ?
Fe1a Sr2b Sr2b 16_555 . 3_565 40.70(3) ?
Fe1a Sr2b Sr2b 16_555 . 3_675 150.45(4) ?
Fe1a Sr2b N1a 16_555 . 7_454 70.87(19) ?
Fe1a Sr2b N3bc 16_555 . 13_554 62.25(15) ?
Fe1a Sr2b C2a 16_555 . 16_564 38.57(14) ?
Fe1a Sr2b C2a 16_555 . 17_654 44.2(3) ?
Fe1a Sr2b Fe1c 16_555 . 4_664 112.61(5) ?
Fe1a Sr2b Fe1b 16_555 . 10_564 94.03(3) ?
Fe1a Sr2b N3ab 16_555 . 1_665 148.67(4) ?
Fe1a Sr2b N1c 16_555 . 13_554 147.92(5) ?
Fe1a Sr2b N2b 16_555 . 10_564 56.25(15) ?
Fe1a Sr2b C2c 16_555 . 4_674 112.02(14) ?
Fe1a Sr2b C2c 16_555 . 6_554 70.04(16) ?
Fe1a Sr2b C2b 16_555 . 10_564 59.36(15) ?
Fe1a Sr2b C2b 16_555 . 12_454 59.42(16) ?
Fe1a Sr2b C1a 16_555 . 16_555 47.1(3) ?
Fe1a Sr2b C1c 16_555 . 4_664 145.05(13) ?
Fe1a Sr2b C1b 16_555 . 10_564 112.53(10) ?
Sr2c Sr2b Sr2c 13_444 . 13_544 120.00(2) ?
Sr2c Sr2b Sr2c 13_444 . 13_554 120.00(3) ?
Sr2c Sr2b Sr2c 13_444 . 14_654 60.17(2) ?
Sr2c Sr2b Sr2c 13_444 . 15_564 60.61(6) ?
Sr2c Sr2b Sr2b 13_444 . 2_665 11.75(2) ?
Sr2c Sr2b Sr2b 13_444 . 2_765 131.84(3) ?
Sr2c Sr2b Sr2b 13_444 . 3_565 48.25(2) ?
Sr2c Sr2b Sr2b 13_444 . 3_675 168.16(3) ?
Sr2c Sr2b N1a 13_444 . 7_454 45.08(17) ?
Sr2c Sr2b N3bc 13_444 . 13_554 37.50(12) ?
Sr2c Sr2b C2a 13_444 . 16_564 45.73(12) ?
Sr2c Sr2b C2a 13_444 . 17_654 77.3(3) ?
Sr2c Sr2b Fe1c 13_444 . 4_664 146.38(4) ?
Sr2c Sr2b Fe1b 13_444 . 10_564 90.10(2) ?
Sr2c Sr2b N3ab 13_444 . 1_665 142.65(13) ?
Sr2c Sr2b N1c 13_444 . 13_554 135.07(17) ?
Sr2c Sr2b N2b 13_444 . 10_564 90.01(15) ?
Sr2c Sr2b C2c 13_444 . 4_674 134.00(17) ?
Sr2c Sr2b C2c 13_444 . 6_554 103.22(15) ?
Sr2c Sr2b C2b 13_444 . 10_564 89.82(14) ?
Sr2c Sr2b C2b 13_444 . 12_454 61.25(12) ?
Sr2c Sr2b C1a 13_444 . 16_555 25.54(19) ?
Sr2c Sr2b C1c 13_444 . 4_664 154.6(2) ?
Sr2c Sr2b C1b 13_444 . 10_564 90.11(2) ?
Sr2c Sr2b Sr2c 13_544 . 13_554 120.00(2) ?
Sr2c Sr2b Sr2c 13_544 . 14_654 59.83(2) ?
Sr2c Sr2b Sr2c 13_544 . 15_564 179.39(6) ?
Sr2c Sr2b Sr2b 13_544 . 2_665 131.75(3) ?
Sr2c Sr2b Sr2b 13_544 . 2_765 11.836(14) ?
Sr2c Sr2b Sr2b 13_544 . 3_565 71.75(2) ?
Sr2c Sr2b Sr2b 13_544 . 3_675 71.84(2) ?
Sr2c Sr2b N1a 13_544 . 7_454 98.71(3) ?
Sr2c Sr2b N3bc 13_544 . 13_554 99.79(3) ?
Sr2c Sr2b C2a 13_544 . 16_564 131.23(17) ?
Sr2c Sr2b C2a 13_544 . 17_654 64.5(3) ?
Sr2c Sr2b Fe1c 13_544 . 4_664 49.24(2) ?
Sr2c Sr2b Fe1b 13_544 . 10_564 143.08(3) ?
Sr2c Sr2b N3ab 13_544 . 1_665 51.44(8) ?
Sr2c Sr2b N1c 13_544 . 13_554 56.28(11) ?
Sr2c Sr2b N2b 13_544 . 10_564 63.8(2) ?
Sr2c Sr2b C2c 13_544 . 4_674 87.9(2) ?
Sr2c Sr2b C2c 13_544 . 6_554 48.7(2) ?
Sr2c Sr2b C2b 13_544 . 10_564 45.84(16) ?
Sr2c Sr2b C2b 13_544 . 12_454 143.17(18) ?
Sr2c Sr2b C1a 13_544 . 16_555 101.15(3) ?
Sr2c Sr2b C1c 13_544 . 4_664 44.91(9) ?
Sr2c Sr2b C1b 13_544 . 10_564 147.15(9) ?
Sr2c Sr2b Sr2c 13_554 . 14_654 179.83(3) ?
Sr2c Sr2b Sr2c 13_554 . 15_564 59.39(6) ?
Sr2c Sr2b Sr2b 13_554 . 2_665 108.25(3) ?
Sr2c Sr2b Sr2b 13_554 . 2_765 108.16(2) ?
Sr2c Sr2b Sr2b 13_554 . 3_565 168.25(3) ?
Sr2c Sr2b Sr2b 13_554 . 3_675 48.16(2) ?
Sr2c Sr2b N1a 13_554 . 7_454 123.70(12) ?
Sr2c Sr2b N3bc 13_554 . 13_554 128.56(8) ?
Sr2c Sr2b C2a 13_554 . 16_564 92.23(14) ?
Sr2c Sr2b C2a 13_554 . 17_654 130.64(17) ?
Sr2c Sr2b Fe1c 13_554 . 4_664 79.645(19) ?
Sr2c Sr2b Fe1b 13_554 . 10_564 36.75(2) ?
Sr2c Sr2b N3ab 13_554 . 1_665 80.12(2) ?
Sr2c Sr2b N1c 13_554 . 13_554 81.21(3) ?
Sr2c Sr2b N2b 13_554 . 10_564 116.23(16) ?
Sr2c Sr2b C2c 13_554 . 4_674 48.79(16) ?
Sr2c Sr2b C2c 13_554 . 6_554 115.54(19) ?
Sr2c Sr2b C2b 13_554 . 10_564 134.41(12) ?
Sr2c Sr2b C2b 13_554 . 12_454 71.37(16) ?
Sr2c Sr2b C1a 13_554 . 16_555 135.15(10) ?
Sr2c Sr2b C1c 13_554 . 4_664 78.76(3) ?
Sr2c Sr2b C1b 13_554 . 10_564 32.65(9) ?
Sr2c Sr2b Sr2c 14_654 . 15_564 120.78(6) ?
Sr2c Sr2b Sr2b 14_654 . 2_665 71.91(3) ?
Sr2c Sr2b Sr2b 14_654 . 2_765 71.67(3) ?
Sr2c Sr2b Sr2b 14_654 . 3_565 11.91(3) ?
Sr2c Sr2b Sr2b 14_654 . 3_675 131.67(4) ?
Sr2c Sr2b N1a 14_654 . 7_454 56.40(11) ?
Sr2c Sr2b N3bc 14_654 . 13_554 51.56(8) ?
Sr2c Sr2b C2a 14_654 . 16_564 87.90(14) ?
Sr2c Sr2b C2a 14_654 . 17_654 49.33(16) ?
Sr2c Sr2b Fe1c 14_654 . 4_664 100.21(3) ?
Sr2c Sr2b Fe1b 14_654 . 10_564 143.38(3) ?
Sr2c Sr2b N3ab 14_654 . 1_665 99.74(4) ?
Sr2c Sr2b N1c 14_654 . 13_554 98.67(4) ?
Sr2c Sr2b N2b 14_654 . 10_564 63.72(16) ?
Sr2c Sr2b C2c 14_654 . 4_674 131.12(16) ?
Sr2c Sr2b C2c 14_654 . 6_554 64.37(19) ?
Sr2c Sr2b C2b 14_654 . 10_564 45.49(12) ?
Sr2c Sr2b C2b 14_654 . 12_454 108.76(16) ?
Sr2c Sr2b C1a 14_654 . 16_555 45.00(9) ?
Sr2c Sr2b C1c 14_654 . 4_664 101.08(4) ?
Sr2c Sr2b C1b 14_654 . 10_564 147.50(9) ?
Sr2c Sr2b Sr2b 15_564 . 2_665 48.87(6) ?
Sr2c Sr2b Sr2b 15_564 . 2_765 167.55(6) ?
Sr2c Sr2b Sr2b 15_564 . 3_565 108.87(6) ?
Sr2c Sr2b Sr2b 15_564 . 3_675 107.55(6) ?
Sr2c Sr2b N1a 15_564 . 7_454 81.75(7) ?
Sr2c Sr2b N3bc 15_564 . 13_554 80.72(7) ?
Sr2c Sr2b C2a 15_564 . 16_564 49.12(18) ?
Sr2c Sr2b C2a 15_564 . 17_654 115.9(3) ?
Sr2c Sr2b Fe1c 15_564 . 4_664 130.29(7) ?
Sr2c Sr2b Fe1b 15_564 . 10_564 36.45(6) ?
Sr2c Sr2b N3ab 15_564 . 1_665 128.12(10) ?
Sr2c Sr2b N1c 15_564 . 13_554 123.36(13) ?
Sr2c Sr2b N2b 15_564 . 10_564 116.4(2) ?
Sr2c Sr2b C2c 15_564 . 4_674 91.6(2) ?
Sr2c Sr2b C2c 15_564 . 6_554 131.4(2) ?
Sr2c Sr2b C2b 15_564 . 10_564 134.51(18) ?
Sr2c Sr2b C2b 15_564 . 12_454 36.93(19) ?
Sr2c Sr2b C1a 15_564 . 16_555 79.43(6) ?
Sr2c Sr2b C1c 15_564 . 4_664 134.54(11) ?
Sr2c Sr2b C1b 15_564 . 10_564 32.30(10) ?
Sr2b Sr2b Sr2b 2_665 . 2_765 143.58(3) ?
Sr2b Sr2b Sr2b 2_665 . 3_565 60.00(3) ?
Sr2b Sr2b Sr2b 2_665 . 3_675 156.42(3) ?
Sr2b Sr2b N1a 2_665 . 7_454 49.91(14) ?
Sr2b Sr2b N3bc 2_665 . 13_554 43.66(10) ?
Sr2b Sr2b C2a 2_665 . 16_564 40.86(13) ?
Sr2b Sr2b C2a 2_665 . 17_654 84.9(3) ?
Sr2b Sr2b Fe1c 2_665 . 4_664 150.56(4) ?
Sr2b Sr2b Fe1b 2_665 . 10_564 79.26(3) ?
Sr2b Sr2b N3ab 2_665 . 1_665 146.24(14) ?
Sr2b Sr2b N1c 2_665 . 13_554 137.77(19) ?
Sr2b Sr2b N2b 2_665 . 10_564 95.98(16) ?
Sr2b Sr2b C2c 2_665 . 4_674 127.37(18) ?
Sr2b Sr2b C2c 2_665 . 6_554 110.62(16) ?
Sr2b Sr2b C2b 2_665 . 10_564 99.27(15) ?
Sr2b Sr2b C2b 2_665 . 12_454 52.95(12) ?
Sr2b Sr2b C1a 2_665 . 16_555 34.63(14) ?
Sr2b Sr2b C1c 2_665 . 4_664 160.8(3) ?
Sr2b Sr2b C1b 2_665 . 10_564 78.70(3) ?
Sr2b Sr2b Sr2b 2_765 . 3_565 83.58(3) ?
Sr2b Sr2b Sr2b 2_765 . 3_675 60.00(2) ?
Sr2b Sr2b N1a 2_765 . 7_454 107.30(6) ?
Sr2b Sr2b N3bc 2_765 . 13_554 109.52(4) ?
Sr2b Sr2b C2a 2_765 . 16_564 137.08(17) ?
Sr2b Sr2b C2a 2_765 . 17_654 71.4(3) ?
Sr2b Sr2b Fe1c 2_765 . 4_664 40.63(3) ?
Sr2b Sr2b Fe1b 2_765 . 10_564 133.42(3) ?
Sr2b Sr2b N3ab 2_765 . 1_665 43.57(10) ?
Sr2b Sr2b N1c 2_765 . 13_554 49.81(14) ?
Sr2b Sr2b N2b 2_765 . 10_564 67.6(2) ?
Sr2b Sr2b C2c 2_765 . 4_674 78.7(2) ?
Sr2b Sr2b C2c 2_765 . 6_554 51.5(2) ?
Sr2b Sr2b C2b 2_765 . 10_564 53.23(16) ?
Sr2b Sr2b C2b 2_765 . 12_454 143.37(16) ?
Sr2b Sr2b C1a 2_765 . 16_555 112.34(5) ?
Sr2b Sr2b C1c 2_765 . 4_664 34.59(13) ?
Sr2b Sr2b C1b 2_765 . 10_564 136.25(6) ?
Sr2b Sr2b Sr2b 3_565 . 3_675 143.58(4) ?
Sr2b Sr2b N1a 3_565 . 7_454 49.91(14) ?
Sr2b Sr2b N3bc 3_565 . 13_554 43.66(10) ?
Sr2b Sr2b C2a 3_565 . 16_564 78.60(13) ?
Sr2b Sr2b C2a 3_565 . 17_654 52.20(16) ?
Sr2b Sr2b Fe1c 3_565 . 4_664 110.52(3) ?
Sr2b Sr2b Fe1b 3_565 . 10_564 133.69(3) ?
Sr2b Sr2b N3ab 3_565 . 1_665 109.55(5) ?
Sr2b Sr2b N1c 3_565 . 13_554 107.34(6) ?
Sr2b Sr2b N2b 3_565 . 10_564 67.62(14) ?
Sr2b Sr2b C2c 3_565 . 4_674 136.96(15) ?
Sr2b Sr2b C2c 3_565 . 6_554 71.48(18) ?
Sr2b Sr2b C2b 3_565 . 10_564 52.87(12) ?
Sr2b Sr2b C2b 3_565 . 12_454 99.33(15) ?
Sr2b Sr2b C1a 3_565 . 16_555 34.63(14) ?
Sr2b Sr2b C1c 3_565 . 4_664 112.35(5) ?
Sr2b Sr2b C1b 3_565 . 10_564 136.53(7) ?
Sr2b Sr2b N1a 3_675 . 7_454 137.64(19) ?
Sr2b Sr2b N3bc 3_675 . 13_554 146.12(14) ?
Sr2b Sr2b C2a 3_675 . 16_564 127.57(12) ?
Sr2b Sr2b C2a 3_675 . 17_654 110.1(2) ?
Sr2b Sr2b Fe1c 3_675 . 4_664 40.63(3) ?
Sr2b Sr2b Fe1b 3_675 . 10_564 78.97(2) ?
Sr2b Sr2b N3ab 3_675 . 1_665 43.57(10) ?
Sr2b Sr2b N1c 3_675 . 13_554 49.81(14) ?
Sr2b Sr2b N2b 3_675 . 10_564 96.00(14) ?
Sr2b Sr2b C2c 3_675 . 4_674 41.09(15) ?
Sr2b Sr2b C2c 3_675 . 6_554 84.57(15) ?
Sr2b Sr2b C2b 3_675 . 10_564 99.69(14) ?
Sr2b Sr2b C2b 3_675 . 12_454 109.76(13) ?
Sr2b Sr2b C1a 3_675 . 16_555 160.8(3) ?
Sr2b Sr2b C1c 3_675 . 4_664 34.59(13) ?
Sr2b Sr2b C1b 3_675 . 10_564 78.41(2) ?
N1a Sr2b N3bc 7_454 . 13_554 8.6(2) ?
N1a Sr2b C2a 7_454 . 16_564 90.3(2) ?
N1a Sr2b C2a 7_454 . 17_654 101.5(2) ?
N1a Sr2b Fe1c 7_454 . 4_664 147.82(6) ?
N1a Sr2b Fe1b 7_454 . 10_564 118.16(4) ?
N1a Sr2b N3ab 7_454 . 1_665 97.7(2) ?
N1a Sr2b N1c 7_454 . 13_554 90.0(2) ?
N1a Sr2b N2b 7_454 . 10_564 117.1(2) ?
N1a Sr2b C2c 7_454 . 4_674 172.2(2) ?
N1a Sr2b C2c 7_454 . 6_554 120.7(2) ?
N1a Sr2b C2b 7_454 . 10_564 101.86(16) ?
N1a Sr2b C2b 7_454 . 12_454 101.94(17) ?
N1a Sr2b C1a 7_454 . 16_555 23.8(3) ?
N1a Sr2b C1c 7_454 . 4_664 111.2(3) ?
N1a Sr2b C1b 7_454 . 10_564 93.90(17) ?
N3bc Sr2b C2a 13_554 . 16_564 83.15(17) ?
N3bc Sr2b C2a 13_554 . 17_654 94.2(2) ?
N3bc Sr2b Fe1c 13_554 . 4_664 148.63(4) ?
N3bc Sr2b Fe1b 13_554 . 10_564 116.95(4) ?
N3bc Sr2b N3ab 13_554 . 1_665 105.15(18) ?
N3bc Sr2b N1c 13_554 . 13_554 97.7(2) ?
N3bc Sr2b N2b 13_554 . 10_564 109.83(18) ?
N3bc Sr2b C2c 13_554 . 4_674 171.0(2) ?
N3bc Sr2b C2c 13_554 . 6_554 115.1(2) ?
N3bc Sr2b C2b 13_554 . 10_564 96.41(15) ?
N3bc Sr2b C2b 13_554 . 12_454 96.50(15) ?
N3bc Sr2b C1a 13_554 . 16_555 15.2(3) ?
N3bc Sr2b C1c 13_554 . 4_664 117.9(3) ?
N3bc Sr2b C1b 13_554 . 10_564 97.15(15) ?
C2a Sr2b C2a 16_564 . 17_654 66.8(3) ?
C2a Sr2b Fe1c 16_564 . 4_664 112.36(15) ?
C2a Sr2b Fe1b 16_564 . 10_564 55.49(13) ?
C2a Sr2b N3ab 16_564 . 1_665 171.10(15) ?
C2a Sr2b N1c 16_564 . 13_554 172.28(18) ?
C2a Sr2b N2b 16_564 . 10_564 69.5(3) ?
C2a Sr2b C2c 16_564 . 4_674 88.3(2) ?
C2a Sr2b C2c 16_564 . 6_554 85.7(3) ?
C2a Sr2b C2b 16_564 . 10_564 85.4(2) ?
C2a Sr2b C2b 16_564 . 12_454 20.9(2) ?
C2a Sr2b C1a 16_564 . 16_555 70.7(3) ?
C2a Sr2b C1c 16_564 . 4_664 158.3(3) ?
C2a Sr2b C1b 16_564 . 10_564 78.6(2) ?
C2a Sr2b Fe1c 17_654 . 4_664 69.6(2) ?
C2a Sr2b Fe1b 17_654 . 10_564 107.0(2) ?
C2a Sr2b N3ab 17_654 . 1_665 115.0(3) ?
C2a Sr2b N1c 17_654 . 13_554 120.7(3) ?
C2a Sr2b N2b 17_654 . 10_564 15.6(2) ?
C2a Sr2b C2c 17_654 . 4_674 84.9(2) ?
C2a Sr2b C2c 17_654 . 6_554 26.0(3) ?
C2a Sr2b C2b 17_654 . 10_564 18.6(3) ?
C2a Sr2b C2b 17_654 . 12_454 81.6(3) ?
C2a Sr2b C1a 17_654 . 16_555 81.3(3) ?
C2a Sr2b C1c 17_654 . 4_664 104.3(4) ?
C2a Sr2b C1b 17_654 . 10_564 141.8(3) ?
Fe1c Sr2b Fe1b 4_664 . 10_564 93.84(3) ?
Fe1c Sr2b N3ab 4_664 . 1_665 62.01(15) ?
Fe1c Sr2b N1c 4_664 . 13_554 70.62(19) ?
Fe1c Sr2b N2b 4_664 . 10_564 56.37(15) ?
Fe1c Sr2b C2c 4_664 . 4_674 38.7(2) ?
Fe1c Sr2b C2c 4_664 . 6_554 43.94(15) ?
Fe1c Sr2b C2b 4_664 . 10_564 59.83(13) ?
Fe1c Sr2b C2b 4_664 . 12_454 106.97(14) ?
Fe1c Sr2b C1a 4_664 . 16_555 145.11(12) ?
Fe1c Sr2b C1c 4_664 . 4_664 46.9(3) ?
Fe1c Sr2b C1b 4_664 . 10_564 112.25(10) ?
Fe1b Sr2b N3ab 10_564 . 1_665 116.67(3) ?
Fe1b Sr2b N1c 10_564 . 13_554 117.92(3) ?
Fe1b Sr2b N2b 10_564 . 10_564 98.2(2) ?
Fe1b Sr2b C2c 10_564 . 4_674 55.1(2) ?
Fe1b Sr2b C2c 10_564 . 6_554 107.3(2) ?
Fe1b Sr2b C2b 10_564 . 10_564 121.28(15) ?
Fe1b Sr2b C2b 10_564 . 12_454 34.62(16) ?
Fe1b Sr2b C1a 10_564 . 16_555 113.31(9) ?
Fe1b Sr2b C1c 10_564 . 4_664 113.01(9) ?
Fe1b Sr2b C1b 10_564 . 10_564 36.3(2) ?
N3ab Sr2b N1c 1_665 . 13_554 8.6(2) ?
N3ab Sr2b N2b 1_665 . 10_564 109.7(2) ?
N3ab Sr2b C2c 1_665 . 4_674 83.3(2) ?
N3ab Sr2b C2c 1_665 . 6_554 93.5(2) ?
N3ab Sr2b C2b 1_665 . 10_564 96.67(19) ?
N3ab Sr2b C2b 1_665 . 12_454 151.08(15) ?
N3ab Sr2b C1a 1_665 . 16_555 118.0(3) ?
N3ab Sr2b C1c 1_665 . 4_664 15.1(3) ?
N3ab Sr2b C1b 1_665 . 10_564 96.96(14) ?
N1c Sr2b N2b 13_554 . 10_564 117.0(3) ?
N1c Sr2b C2c 13_554 . 4_674 90.4(2) ?
N1c Sr2b C2c 13_554 . 6_554 100.8(3) ?
N1c Sr2b C2b 13_554 . 10_564 102.1(2) ?
N1c Sr2b C2b 13_554 . 12_454 152.33(17) ?
N1c Sr2b C1a 13_554 . 16_555 111.2(3) ?
N1c Sr2b C1c 13_554 . 4_664 23.7(3) ?
N1c Sr2b C1b 13_554 . 10_564 93.74(17) ?
N2b Sr2b C2c 10_564 . 4_674 69.4(2) ?
N2b Sr2b C2c 10_564 . 6_554 16.3(3) ?
N2b Sr2b C2b 10_564 . 10_564 23.0(2) ?
N2b Sr2b C2b 10_564 . 12_454 79.7(3) ?
N2b Sr2b C1a 10_564 . 16_555 96.7(3) ?
N2b Sr2b C1c 10_564 . 4_664 96.6(3) ?
N2b Sr2b C1b 10_564 . 10_564 134.5(3) ?
C2c Sr2b C2c 4_674 . 6_554 66.8(3) ?
C2c Sr2b C2b 4_674 . 10_564 85.6(2) ?
C2c Sr2b C2b 4_674 . 12_454 74.5(2) ?
C2c Sr2b C1a 4_674 . 16_555 158.1(3) ?
C2c Sr2b C1c 4_674 . 4_664 70.9(3) ?
C2c Sr2b C1b 4_674 . 10_564 78.3(2) ?
C2c Sr2b C2b 6_554 . 10_564 18.9(2) ?
C2c Sr2b C2b 6_554 . 12_454 94.5(3) ?
C2c Sr2b C1a 6_554 . 16_555 104.5(3) ?
C2c Sr2b C1c 6_554 . 4_664 80.6(3) ?
C2c Sr2b C1b 6_554 . 10_564 142.0(3) ?
C2b Sr2b C2b 10_564 . 12_454 99.8(2) ?
C2b Sr2b C1a 10_564 . 16_555 86.7(2) ?
C2b Sr2b C1c 10_564 . 4_664 87.0(2) ?
C2b Sr2b C1b 10_564 . 10_564 157.5(3) ?
C2b Sr2b C1a 12_454 . 16_555 86.7(2) ?
C2b Sr2b C1c 12_454 . 4_664 144.1(2) ?
C2b Sr2b C1b 12_454 . 10_564 60.9(3) ?
C1a Sr2b C1c 16_555 . 4_664 129.0(3) ?
C1a Sr2b C1b 16_555 . 10_564 102.49(13) ?
C1c Sr2b C1b 4_664 . 10_564 102.24(13) ?
Sr1 N3ac Sr1 1_545 . 2_665 90.37(19) ?
Sr1 N3ac Sr1 1_545 . 3_455 90.37(19) ?
Sr1 N3ac Sr2a 1_545 . 1_445 167.81(5) ?
Sr1 N3ac Sr2a 1_545 . 2_655 80.40(3) ?
Sr1 N3ac Sr2a 1_545 . 3_565 97.58(3) ?
Sr1 N3ac Sr2c 1_545 . 7_445 83.37(3) ?
Sr1 N3ac Sr2c 1_545 . 8_555 172.37(7) ?
Sr1 N3ac Sr2c 1_545 . 9_455 94.02(4) ?
Sr1 N3ac N1b 1_545 . 13_445 55.00(13) ?
Sr1 N3ac C1b 1_545 . 4_555 125.00(13) ?
Sr1 N3ac Sr1 2_665 . 3_455 90.37(19) ?
Sr1 N3ac Sr2a 2_665 . 1_445 97.58(3) ?
Sr1 N3ac Sr2a 2_665 . 2_655 167.81(5) ?
Sr1 N3ac Sr2a 2_665 . 3_565 80.40(3) ?
Sr1 N3ac Sr2c 2_665 . 7_445 94.02(3) ?
Sr1 N3ac Sr2c 2_665 . 8_555 83.37(4) ?
Sr1 N3ac Sr2c 2_665 . 9_455 172.37(7) ?
Sr1 N3ac N1b 2_665 . 13_445 55.00(13) ?
Sr1 N3ac C1b 2_665 . 4_555 125.00(13) ?
Sr1 N3ac Sr2a 3_455 . 1_445 80.40(3) ?
Sr1 N3ac Sr2a 3_455 . 2_655 97.58(3) ?
Sr1 N3ac Sr2a 3_455 . 3_565 167.81(6) ?
Sr1 N3ac Sr2c 3_455 . 7_445 172.37(7) ?
Sr1 N3ac Sr2c 3_455 . 8_555 94.02(3) ?
Sr1 N3ac Sr2c 3_455 . 9_455 83.37(3) ?
Sr1 N3ac N1b 3_455 . 13_445 55.00(13) ?
Sr1 N3ac C1b 3_455 . 4_555 125.00(13) ?
Sr2a N3ac Sr2a 1_445 . 2_655 92.9(2) ?
Sr2a N3ac Sr2a 1_445 . 3_565 92.9(2) ?
Sr2a N3ac Sr2c 1_445 . 7_445 105.2(2) ?
Sr2a N3ac Sr2c 1_445 . 8_555 19.67(4) ?
Sr2a N3ac Sr2c 1_445 . 9_455 77.12(15) ?
Sr2a N3ac N1b 1_445 . 13_445 123.22(15) ?
Sr2a N3ac C1b 1_445 . 4_555 56.78(15) ?
Sr2a N3ac Sr2a 2_655 . 3_565 92.9(2) ?
Sr2a N3ac Sr2c 2_655 . 7_445 77.12(15) ?
Sr2a N3ac Sr2c 2_655 . 8_555 105.2(2) ?
Sr2a N3ac Sr2c 2_655 . 9_455 19.67(4) ?
Sr2a N3ac N1b 2_655 . 13_445 123.21(15) ?
Sr2a N3ac C1b 2_655 . 4_555 56.78(15) ?
Sr2a N3ac Sr2c 3_565 . 7_445 19.67(5) ?
Sr2a N3ac Sr2c 3_565 . 8_555 77.12(15) ?
Sr2a N3ac Sr2c 3_565 . 9_455 105.2(2) ?
Sr2a N3ac N1b 3_565 . 13_445 123.22(14) ?
Sr2a N3ac C1b 3_565 . 4_555 56.78(14) ?
Sr2c N3ac Sr2c 7_445 . 8_555 92.7(2) ?
Sr2c N3ac Sr2c 7_445 . 9_455 92.7(2) ?
Sr2c N3ac N1b 7_445 . 13_445 123.34(15) ?
Sr2c N3ac C1b 7_445 . 4_555 56.66(15) ?
Sr2c N3ac Sr2c 8_555 . 9_455 92.7(2) ?
Sr2c N3ac N1b 8_555 . 13_445 123.34(15) ?
Sr2c N3ac C1b 8_555 . 4_555 56.66(15) ?
Sr2c N3ac N1b 9_455 . 13_445 123.34(15) ?
Sr2c N3ac C1b 9_455 . 4_555 56.66(15) ?
N1b N3ac C1b 13_445 . 4_555 180 ?
Sr1 N1a Sr1 1_545 . 2_765 105.6(3) ?
Sr1 N1a Sr1 1_545 . 3_565 105.6(3) ?
Sr1 N1a Sr2c 1_545 . 7_445 78.42(7) ?
Sr1 N1a Sr2c 1_545 . 8_655 93.21(9) ?
Sr1 N1a Sr2c 1_545 . 9_565 158.6(4) ?
Sr1 N1a Sr2b 1_545 . 13_545 159.0(4) ?
Sr1 N1a Sr2b 1_545 . 14_655 92.36(9) ?
Sr1 N1a Sr2b 1_545 . 15_555 79.25(7) ?
Sr1 N1a N3bc 1_545 . 7_555 113.1(2) ?
Sr1 N1a C1a 1_545 . 10_555 113.1(2) ?
Sr1 N1a Sr1 2_765 . 3_565 105.6(3) ?
Sr1 N1a Sr2c 2_765 . 7_445 158.6(4) ?
Sr1 N1a Sr2c 2_765 . 8_655 78.42(8) ?
Sr1 N1a Sr2c 2_765 . 9_565 93.21(9) ?
Sr1 N1a Sr2b 2_765 . 13_545 79.25(7) ?
Sr1 N1a Sr2b 2_765 . 14_655 159.0(4) ?
Sr1 N1a Sr2b 2_765 . 15_555 92.36(9) ?
Sr1 N1a N3bc 2_765 . 7_555 113.1(2) ?
Sr1 N1a C1a 2_765 . 10_555 113.1(2) ?
Sr1 N1a Sr2c 3_565 . 7_445 93.21(9) ?
Sr1 N1a Sr2c 3_565 . 8_655 158.6(4) ?
Sr1 N1a Sr2c 3_565 . 9_565 78.42(7) ?
Sr1 N1a Sr2b 3_565 . 13_545 92.36(9) ?
Sr1 N1a Sr2b 3_565 . 14_655 79.25(8) ?
Sr1 N1a Sr2b 3_565 . 15_555 159.0(4) ?
Sr1 N1a N3bc 3_565 . 7_555 113.1(2) ?
Sr1 N1a C1a 3_565 . 10_555 113.1(2) ?
Sr2c N1a Sr2c 7_445 . 8_655 80.4(3) ?
Sr2c N1a Sr2c 7_445 . 9_565 80.4(3) ?
Sr2c N1a Sr2b 7_445 . 13_545 90.0(3) ?
Sr2c N1a Sr2b 7_445 . 14_655 17.50(6) ?
Sr2c N1a Sr2b 7_445 . 15_555 67.4(2) ?
Sr2c N1a N3bc 7_445 . 7_555 48.17(19) ?
Sr2c N1a C1a 7_445 . 10_555 48.17(19) ?
Sr2c N1a Sr2c 8_655 . 9_565 80.4(3) ?
Sr2c N1a Sr2b 8_655 . 13_545 67.4(2) ?
Sr2c N1a Sr2b 8_655 . 14_655 90.0(3) ?
Sr2c N1a Sr2b 8_655 . 15_555 17.50(6) ?
Sr2c N1a N3bc 8_655 . 7_555 48.17(19) ?
Sr2c N1a C1a 8_655 . 10_555 48.17(19) ?
Sr2c N1a Sr2b 9_565 . 13_545 17.50(6) ?
Sr2c N1a Sr2b 9_565 . 14_655 67.4(2) ?
Sr2c N1a Sr2b 9_565 . 15_555 90.0(3) ?
Sr2c N1a N3bc 9_565 . 7_555 48.17(19) ?
Sr2c N1a C1a 9_565 . 10_555 48.17(19) ?
Sr2b N1a Sr2b 13_545 . 14_655 80.2(3) ?
Sr2b N1a Sr2b 13_545 . 15_555 80.2(3) ?
Sr2b N1a N3bc 13_545 . 7_555 48.04(19) ?
Sr2b N1a C1a 13_545 . 10_555 48.04(19) ?
Sr2b N1a Sr2b 14_655 . 15_555 80.2(3) ?
Sr2b N1a N3bc 14_655 . 7_555 48.04(19) ?
Sr2b N1a C1a 14_655 . 10_555 48.04(19) ?
Sr2b N1a N3bc 15_555 . 7_555 48.04(19) ?
Sr2b N1a C1a 15_555 . 10_555 48.04(19) ?
N3bc N1a C1a 7_555 . 10_555 0 ?
Sr1 N3bc Sr1 13_434 . 14_654 93.98(17) ?
Sr1 N3bc Sr1 13_434 . 15_454 93.98(17) ?
Sr1 N3bc Sr2c 13_434 . 1_445 79.41(3) ?
Sr1 N3bc Sr2c 13_434 . 2_655 94.65(3) ?
Sr1 N3bc Sr2c 13_434 . 3_565 169.47(4) ?
Sr1 N3bc Sr2b 13_434 . 7_445 170.64(4) ?
Sr1 N3bc Sr2b 13_434 . 8_555 93.77(3) ?
Sr1 N3bc Sr2b 13_434 . 9_455 80.26(3) ?
Sr1 N3bc N1a 13_434 . 13_444 57.60(13) ?
Sr1 N3bc C1a 13_434 . 4_555 122.40(13) ?
Sr1 N3bc Sr1 14_654 . 15_454 93.98(18) ?
Sr1 N3bc Sr2c 14_654 . 1_445 169.47(4) ?
Sr1 N3bc Sr2c 14_654 . 2_655 79.41(3) ?
Sr1 N3bc Sr2c 14_654 . 3_565 94.65(3) ?
Sr1 N3bc Sr2b 14_654 . 7_445 80.26(3) ?
Sr1 N3bc Sr2b 14_654 . 8_555 170.64(4) ?
Sr1 N3bc Sr2b 14_654 . 9_455 93.77(4) ?
Sr1 N3bc N1a 14_654 . 13_444 57.60(13) ?
Sr1 N3bc C1a 14_654 . 4_555 122.40(13) ?
Sr1 N3bc Sr2c 15_454 . 1_445 94.65(3) ?
Sr1 N3bc Sr2c 15_454 . 2_655 169.47(3) ?
Sr1 N3bc Sr2c 15_454 . 3_565 79.41(3) ?
Sr1 N3bc Sr2b 15_454 . 7_445 93.77(3) ?
Sr1 N3bc Sr2b 15_454 . 8_555 80.26(4) ?
Sr1 N3bc Sr2b 15_454 . 9_455 170.64(4) ?
Sr1 N3bc N1a 15_454 . 13_444 57.60(13) ?
Sr1 N3bc C1a 15_454 . 4_555 122.40(13) ?
Sr2c N3bc Sr2c 1_445 . 2_655 92.9(2) ?
Sr2c N3bc Sr2c 1_445 . 3_565 92.9(2) ?
Sr2c N3bc Sr2b 1_445 . 7_445 105.2(2) ?
Sr2c N3bc Sr2b 1_445 . 8_555 19.67(4) ?
Sr2c N3bc Sr2b 1_445 . 9_455 77.12(15) ?
Sr2c N3bc N1a 1_445 . 13_444 123.22(15) ?
Sr2c N3bc C1a 1_445 . 4_555 56.78(15) ?
Sr2c N3bc Sr2c 2_655 . 3_565 92.9(2) ?
Sr2c N3bc Sr2b 2_655 . 7_445 77.12(15) ?
Sr2c N3bc Sr2b 2_655 . 8_555 105.2(2) ?
Sr2c N3bc Sr2b 2_655 . 9_455 19.67(4) ?
Sr2c N3bc N1a 2_655 . 13_444 123.21(15) ?
Sr2c N3bc C1a 2_655 . 4_555 56.78(15) ?
Sr2c N3bc Sr2b 3_565 . 7_445 19.67(5) ?
Sr2c N3bc Sr2b 3_565 . 8_555 77.12(15) ?
Sr2c N3bc Sr2b 3_565 . 9_455 105.2(2) ?
Sr2c N3bc N1a 3_565 . 13_444 123.22(15) ?
Sr2c N3bc C1a 3_565 . 4_555 56.78(15) ?
Sr2b N3bc Sr2b 7_445 . 8_555 92.7(2) ?
Sr2b N3bc Sr2b 7_445 . 9_455 92.7(2) ?
Sr2b N3bc N1a 7_445 . 13_444 123.34(15) ?
Sr2b N3bc C1a 7_445 . 4_555 56.66(15) ?
Sr2b N3bc Sr2b 8_555 . 9_455 92.7(2) ?
Sr2b N3bc N1a 8_555 . 13_444 123.34(15) ?
Sr2b N3bc C1a 8_555 . 4_555 56.66(15) ?
Sr2b N3bc N1a 9_455 . 13_444 123.34(15) ?
Sr2b N3bc C1a 9_455 . 4_555 56.66(15) ?
N1a N3bc C1a 13_444 . 4_555 180 ?
Sr1 N2a Sr1 1_545 . 3_555 91.9(2) ?
Sr1 N2a Sr2a 1_545 . 16_655 98.8(3) ?
Sr1 N2a C2a 1_545 . . 165.5(7) ?
Sr1 N2a N2c 1_545 . 8_545 129.9(9) ?
Sr1 N2a N2b 1_545 . 15_655 133.8(10) ?
Sr1 N2a C2c 1_545 . 8_545 126.9(13) ?
Sr1 N2a C2b 1_545 . 15_655 123.1(9) ?
Sr1 N2a Sr2a 3_555 . 16_655 138.3(3) ?
Sr1 N2a C2a 3_555 . . 75.8(6) ?
Sr1 N2a N2c 3_555 . 8_545 38.1(8) ?
Sr1 N2a N2b 3_555 . 15_655 81.3(10) ?
Sr1 N2a C2c 3_555 . 8_545 137.4(12) ?
Sr1 N2a C2b 3_555 . 15_655 78.1(10) ?
Sr2a N2a C2a 16_655 . . 95.6(6) ?
Sr2a N2a N2c 16_655 . 8_545 116.1(9) ?
Sr2a N2a N2b 16_655 . 15_655 116.4(9) ?
Sr2a N2a C2c 16_655 . 8_545 60.3(8) ?
Sr2a N2a C2b 16_655 . 15_655 62.3(10) ?
C2a N2a N2c . . 8_545 39.2(8) ?
C2a N2a N2b . . 15_655 37.6(9) ?
C2a N2a C2c . . 8_545 62.9(12) ?
C2a N2a C2b . . 15_655 62.6(11) ?
N2c N2a N2b 8_545 . 15_655 60.0(12) ?
N2c N2a C2c 8_545 . 8_545 102.1(15) ?
N2c N2a C2b 8_545 . 15_655 57.1(12) ?
N2b N2a C2c 15_655 . 8_545 59.9(11) ?
N2b N2a C2b 15_655 . 15_655 100.1(15) ?
C2c N2a C2b 8_545 . 15_655 91.4(13) ?
Sr1 C2a Sr1 2_765 . 3_555 82.45(18) ?
Sr1 C2a Sr2a 2_765 . 16_655 127.4(3) ?
Sr1 C2a Sr2a 2_765 . 18_555 82.67(17) ?
Sr1 C2a Fe1a 2_765 . 1_656 92.3(2) ?
Sr1 C2a Sr2c 2_765 . 4_765 84.47(16) ?
Sr1 C2a Sr2c 2_765 . 6_555 160.1(4) ?
Sr1 C2a Sr2b 2_765 . 10_655 145.4(3) ?
Sr1 C2a Sr2b 2_765 . 11_545 94.4(2) ?
Sr1 C2a N2a 2_765 . . 84.7(5) ?
Sr1 C2a N2c 2_765 . 8_545 90.1(8) ?
Sr1 C2a N2b 2_765 . 15_655 45.3(9) ?
Sr1 C2a C2c 2_765 . 8_545 83.2(5) ?
Sr1 C2a C2b 2_765 . 15_655 122.6(7) ?
Sr1 C2a Sr2a 3_555 . 16_655 124.8(2) ?
Sr1 C2a Sr2a 3_555 . 18_555 160.8(3) ?
Sr1 C2a Fe1a 3_555 . 1_656 95.2(4) ?
Sr1 C2a Sr2c 3_555 . 4_765 148.5(3) ?
Sr1 C2a Sr2c 3_555 . 6_555 95.4(3) ?
Sr1 C2a Sr2b 3_555 . 10_655 86.5(2) ?
Sr1 C2a Sr2b 3_555 . 11_545 163.2(4) ?
Sr1 C2a N2a 3_555 . . 80.6(5) ?
Sr1 C2a N2c 3_555 . 8_545 41.4(10) ?
Sr1 C2a N2b 3_555 . 15_655 85.4(9) ?
Sr1 C2a C2c 3_555 . 8_545 117.6(6) ?
Sr1 C2a C2b 3_555 . 15_655 78.7(6) ?
Sr2a C2a Sr2a 16_655 . 18_555 74.18(19) ?
Sr2a C2a Fe1a 16_655 . 1_656 123.4(3) ?
Sr2a C2a Sr2c 16_655 . 4_765 85.6(2) ?
Sr2a C2a Sr2c 16_655 . 6_555 69.70(17) ?
Sr2a C2a Sr2b 16_655 . 10_655 85.40(17) ?
Sr2a C2a Sr2b 16_655 . 11_545 70.0(2) ?
Sr2a C2a N2a 16_655 . . 61.4(5) ?
Sr2a C2a N2c 16_655 . 8_545 88.2(9) ?
Sr2a C2a N2b 16_655 . 15_655 88.8(11) ?
Sr2a C2a C2c 16_655 . 8_545 45.1(5) ?
Sr2a C2a C2b 16_655 . 15_655 46.4(5) ?
Sr2a C2a Fe1a 18_555 . 1_656 73.4(2) ?
Sr2a C2a Sr2c 18_555 . 4_765 16.58(5) ?
Sr2a C2a Sr2c 18_555 . 6_555 94.5(2) ?
Sr2a C2a Sr2b 18_555 . 10_655 99.1(2) ?
Sr2a C2a Sr2b 18_555 . 11_545 12.53(6) ?
Sr2a C2a N2a 18_555 . . 110.0(7) ?
Sr2a C2a N2c 18_555 . 8_545 150.6(13) ?
Sr2a C2a N2b 18_555 . 15_655 92.7(8) ?
Sr2a C2a C2c 18_555 . 8_545 72.4(5) ?
Sr2a C2a C2b 18_555 . 15_655 119.7(7) ?
Fe1a C2a Sr2c 1_656 . 4_765 56.77(16) ?
Fe1a C2a Sr2c 1_656 . 6_555 68.1(3) ?
Fe1a C2a Sr2b 1_656 . 10_655 56.2(2) ?
Fe1a C2a Sr2b 1_656 . 11_545 68.4(2) ?
Fe1a C2a N2a 1_656 . . 175.1(7) ?
Fe1a C2a N2c 1_656 . 8_545 135.7(13) ?
Fe1a C2a N2b 1_656 . 15_655 137.3(10) ?
Fe1a C2a C2c 1_656 . 8_545 145.8(6) ?
Fe1a C2a C2b 1_656 . 15_655 142.8(8) ?
Sr2c C2a Sr2c 4_765 . 6_555 87.4(2) ?
Sr2c C2a Sr2b 4_765 . 10_655 88.3(2) ?
Sr2c C2a Sr2b 4_765 . 11_545 15.67(5) ?
Sr2c C2a N2a 4_765 . . 126.6(7) ?
Sr2c C2a N2c 4_765 . 8_545 166.8(13) ?
Sr2c C2a N2b 4_765 . 15_655 105.2(8) ?
Sr2c C2a C2c 4_765 . 8_545 89.0(5) ?
Sr2c C2a C2b 4_765 . 15_655 132.0(7) ?
Sr2c C2a Sr2b 6_555 . 10_655 15.69(7) ?
Sr2c C2a Sr2b 6_555 . 11_545 81.9(2) ?
Sr2c C2a N2a 6_555 . . 114.6(5) ?
Sr2c C2a N2c 6_555 . 8_545 101.4(9) ?
Sr2c C2a N2b 6_555 . 15_655 154.5(10) ?
Sr2c C2a C2c 6_555 . 8_545 114.8(6) ?
Sr2c C2a C2b 6_555 . 15_655 75.9(6) ?
Sr2b C2a Sr2b 10_655 . 11_545 86.9(2) ?
Sr2b C2a N2a 10_655 . . 125.6(5) ?
Sr2b C2a N2c 10_655 . 8_545 102.8(10) ?
Sr2b C2a N2b 10_655 . 15_655 165.0(8) ?
Sr2b C2a C2c 10_655 . 8_545 130.5(6) ?
Sr2b C2a C2b 10_655 . 15_655 86.7(6) ?
Sr2b C2a N2a 11_545 . . 115.7(7) ?
Sr2b C2a N2c 11_545 . 8_545 155.4(13) ?
Sr2b C2a N2b 11_545 . 15_655 104.1(9) ?
Sr2b C2a C2c 11_545 . 8_545 78.1(5) ?
Sr2b C2a C2b 11_545 . 15_655 116.3(7) ?
N2a C2a N2c . . 8_545 40.7(11) ?
N2a C2a N2b . . 15_655 40.3(9) ?
N2a C2a C2c . . 8_545 37.8(6) ?
N2a C2a C2b . . 15_655 39.0(6) ?
N2c C2a N2b 8_545 . 15_655 63.0(12) ?
N2c C2a C2c 8_545 . 8_545 78.4(13) ?
N2c C2a C2b 8_545 . 15_655 43.4(8) ?
N2b C2a C2c 15_655 . 8_545 45.1(11) ?
N2b C2a C2b 15_655 . 15_655 79.3(11) ?
C2c C2a C2b 8_545 . 15_655 60.0(8) ?
Sr2a Fe1c Sr2a 10_554 . 11_444 98.60(5) ?
Sr2a Fe1c Sr2a 10_554 . 12_454 98.60(5) ?
Sr2a Fe1c Sr2c 10_554 . 16_655 94.03(4) ?
Sr2a Fe1c Sr2c 10_554 . 17_435 12.30(3) ?
Sr2a Fe1c Sr2c 10_554 . 18_455 110.66(5) ?
Sr2a Fe1c Sr2b 10_554 . 4_665 112.61(6) ?
Sr2a Fe1c Sr2b 10_554 . 5_545 81.54(4) ?
Sr2a Fe1c Sr2b 10_554 . 6_455 20.62(4) ?
Sr2a Fe1c C2c 10_554 . 1_455 85.3(2) ?
Sr2a Fe1c C2c 10_554 . 2_545 67.4(2) ?
Sr2a Fe1c C2c 10_554 . 3_665 166.0(3) ?
Sr2a Fe1c C1c 10_554 . . 61.09(3) ?
Sr2a Fe1c Sr2a 11_444 . 12_454 98.60(5) ?
Sr2a Fe1c Sr2c 11_444 . 16_655 110.66(5) ?
Sr2a Fe1c Sr2c 11_444 . 17_435 94.03(4) ?
Sr2a Fe1c Sr2c 11_444 . 18_455 12.30(2) ?
Sr2a Fe1c Sr2b 11_444 . 4_665 20.62(3) ?
Sr2a Fe1c Sr2b 11_444 . 5_545 112.61(6) ?
Sr2a Fe1c Sr2b 11_444 . 6_455 81.54(4) ?
Sr2a Fe1c C2c 11_444 . 1_455 67.4(3) ?
Sr2a Fe1c C2c 11_444 . 2_545 166.0(2) ?
Sr2a Fe1c C2c 11_444 . 3_665 85.3(3) ?
Sr2a Fe1c C1c 11_444 . . 61.09(4) ?
Sr2a Fe1c Sr2c 12_454 . 16_655 12.30(3) ?
Sr2a Fe1c Sr2c 12_454 . 17_435 110.66(5) ?
Sr2a Fe1c Sr2c 12_454 . 18_455 94.03(4) ?
Sr2a Fe1c Sr2b 12_454 . 4_665 81.54(4) ?
Sr2a Fe1c Sr2b 12_454 . 5_545 20.62(3) ?
Sr2a Fe1c Sr2b 12_454 . 6_455 112.61(6) ?
Sr2a Fe1c C2c 12_454 . 1_455 166.0(3) ?
Sr2a Fe1c C2c 12_454 . 2_545 85.3(3) ?
Sr2a Fe1c C2c 12_454 . 3_665 67.4(3) ?
Sr2a Fe1c C1c 12_454 . . 61.09(4) ?
Sr2c Fe1c Sr2c 16_655 . 17_435 106.33(4) ?
Sr2c Fe1c Sr2c 16_655 . 18_455 106.33(4) ?
Sr2c Fe1c Sr2b 16_655 . 4_665 93.84(4) ?
Sr2c Fe1c Sr2b 16_655 . 5_545 12.484(19) ?
Sr2c Fe1c Sr2b 16_655 . 6_455 110.94(5) ?
Sr2c Fe1c C2c 16_655 . 1_455 177.8(2) ?
Sr2c Fe1c C2c 16_655 . 2_545 73.0(3) ?
Sr2c Fe1c C2c 16_655 . 3_665 72.0(4) ?
Sr2c Fe1c C1c 16_655 . . 67.54(3) ?
Sr2c Fe1c Sr2c 17_435 . 18_455 106.33(4) ?
Sr2c Fe1c Sr2b 17_435 . 4_665 110.94(5) ?
Sr2c Fe1c Sr2b 17_435 . 5_545 93.84(4) ?
Sr2c Fe1c Sr2b 17_435 . 6_455 12.48(3) ?
Sr2c Fe1c C2c 17_435 . 1_455 73.0(2) ?
Sr2c Fe1c C2c 17_435 . 2_545 72.0(2) ?
Sr2c Fe1c C2c 17_435 . 3_665 177.8(2) ?
Sr2c Fe1c C1c 17_435 . . 67.54(3) ?
Sr2c Fe1c Sr2b 18_455 . 4_665 12.48(2) ?
Sr2c Fe1c Sr2b 18_455 . 5_545 110.94(5) ?
Sr2c Fe1c Sr2b 18_455 . 6_455 93.84(4) ?
Sr2c Fe1c C2c 18_455 . 1_455 72.0(3) ?
Sr2c Fe1c C2c 18_455 . 2_545 177.8(2) ?
Sr2c Fe1c C2c 18_455 . 3_665 73.0(3) ?
Sr2c Fe1c C1c 18_455 . . 67.54(3) ?
Sr2b Fe1c Sr2b 4_665 . 5_545 98.74(5) ?
Sr2b Fe1c Sr2b 4_665 . 6_455 98.74(5) ?
Sr2b Fe1c C2c 4_665 . 1_455 84.5(3) ?
Sr2b Fe1c C2c 4_665 . 2_545 166.7(3) ?
Sr2b Fe1c C2c 4_665 . 3_665 67.9(3) ?
Sr2b Fe1c C1c 4_665 . . 61.21(4) ?
Sr2b Fe1c Sr2b 5_545 . 6_455 98.74(5) ?
Sr2b Fe1c C2c 5_545 . 1_455 166.7(2) ?
Sr2b Fe1c C2c 5_545 . 2_545 67.9(3) ?
Sr2b Fe1c C2c 5_545 . 3_665 84.5(4) ?
Sr2b Fe1c C1c 5_545 . . 61.21(4) ?
Sr2b Fe1c C2c 6_455 . 1_455 67.9(2) ?
Sr2b Fe1c C2c 6_455 . 2_545 84.5(2) ?
Sr2b Fe1c C2c 6_455 . 3_665 166.7(3) ?
Sr2b Fe1c C1c 6_455 . . 61.21(4) ?
C2c Fe1c C2c 1_455 . 2_545 108.6(4) ?
C2c Fe1c C2c 1_455 . 3_665 108.6(4) ?
C2c Fe1c C1c 1_455 . . 110.3(2) ?
C2c Fe1c C2c 2_545 . 3_665 108.6(4) ?
C2c Fe1c C1c 2_545 . . 110.3(2) ?
C2c Fe1c C1c 3_665 . . 110.3(2) ?
Sr2a Fe1b Sr2a 4_664 . 5_544 98.75(5) ?
Sr2a Fe1b Sr2a 4_664 . 6_454 98.75(5) ?
Sr2a Fe1b Sr2c 4_664 . 10_554 112.61(6) ?
Sr2a Fe1b Sr2c 4_664 . 11_444 20.62(3) ?
Sr2a Fe1b Sr2c 4_664 . 12_454 81.54(4) ?
Sr2a Fe1b Sr2b 4_664 . 16_655 93.84(4) ?
Sr2a Fe1b Sr2b 4_664 . 17_435 110.94(5) ?
Sr2a Fe1b Sr2b 4_664 . 18_455 12.48(2) ?
Sr2a Fe1b C2b 4_664 . 1_455 84.5(3) ?
Sr2a Fe1b C2b 4_664 . 2_545 166.7(3) ?
Sr2a Fe1b C2b 4_664 . 3_665 67.9(3) ?
Sr2a Fe1b C1b 4_664 . . 61.21(4) ?
Sr2a Fe1b Sr2a 5_544 . 6_454 98.75(5) ?
Sr2a Fe1b Sr2c 5_544 . 10_554 81.54(4) ?
Sr2a Fe1b Sr2c 5_544 . 11_444 112.61(6) ?
Sr2a Fe1b Sr2c 5_544 . 12_454 20.62(3) ?
Sr2a Fe1b Sr2b 5_544 . 16_655 12.483(19) ?
Sr2a Fe1b Sr2b 5_544 . 17_435 93.84(4) ?
Sr2a Fe1b Sr2b 5_544 . 18_455 110.94(5) ?
Sr2a Fe1b C2b 5_544 . 1_455 166.7(2) ?
Sr2a Fe1b C2b 5_544 . 2_545 67.9(3) ?
Sr2a Fe1b C2b 5_544 . 3_665 84.5(4) ?
Sr2a Fe1b C1b 5_544 . . 61.21(4) ?
Sr2a Fe1b Sr2c 6_454 . 10_554 20.62(4) ?
Sr2a Fe1b Sr2c 6_454 . 11_444 81.54(4) ?
Sr2a Fe1b Sr2c 6_454 . 12_454 112.61(6) ?
Sr2a Fe1b Sr2b 6_454 . 16_655 110.94(5) ?
Sr2a Fe1b Sr2b 6_454 . 17_435 12.48(3) ?
Sr2a Fe1b Sr2b 6_454 . 18_455 93.84(4) ?
Sr2a Fe1b C2b 6_454 . 1_455 67.9(2) ?
Sr2a Fe1b C2b 6_454 . 2_545 84.5(2) ?
Sr2a Fe1b C2b 6_454 . 3_665 166.7(3) ?
Sr2a Fe1b C1b 6_454 . . 61.21(3) ?
Sr2c Fe1b Sr2c 10_554 . 11_444 98.60(5) ?
Sr2c Fe1b Sr2c 10_554 . 12_454 98.60(5) ?
Sr2c Fe1b Sr2b 10_554 . 16_655 94.03(4) ?
Sr2c Fe1b Sr2b 10_554 . 17_435 12.30(3) ?
Sr2c Fe1b Sr2b 10_554 . 18_455 110.66(5) ?
Sr2c Fe1b C2b 10_554 . 1_455 85.3(2) ?
Sr2c Fe1b C2b 10_554 . 2_545 67.4(2) ?
Sr2c Fe1b C2b 10_554 . 3_665 166.0(3) ?
Sr2c Fe1b C1b 10_554 . . 61.09(4) ?
Sr2c Fe1b Sr2c 11_444 . 12_454 98.60(5) ?
Sr2c Fe1b Sr2b 11_444 . 16_655 110.66(5) ?
Sr2c Fe1b Sr2b 11_444 . 17_435 94.03(4) ?
Sr2c Fe1b Sr2b 11_444 . 18_455 12.30(2) ?
Sr2c Fe1b C2b 11_444 . 1_455 67.4(3) ?
Sr2c Fe1b C2b 11_444 . 2_545 166.0(2) ?
Sr2c Fe1b C2b 11_444 . 3_665 85.3(3) ?
Sr2c Fe1b C1b 11_444 . . 61.09(4) ?
Sr2c Fe1b Sr2b 12_454 . 16_655 12.30(3) ?
Sr2c Fe1b Sr2b 12_454 . 17_435 110.66(5) ?
Sr2c Fe1b Sr2b 12_454 . 18_455 94.03(4) ?
Sr2c Fe1b C2b 12_454 . 1_455 166.0(3) ?
Sr2c Fe1b C2b 12_454 . 2_545 85.3(3) ?
Sr2c Fe1b C2b 12_454 . 3_665 67.4(3) ?
Sr2c Fe1b C1b 12_454 . . 61.09(4) ?
Sr2b Fe1b Sr2b 16_655 . 17_435 106.33(4) ?
Sr2b Fe1b Sr2b 16_655 . 18_455 106.33(4) ?
Sr2b Fe1b C2b 16_655 . 1_455 177.8(2) ?
Sr2b Fe1b C2b 16_655 . 2_545 73.0(3) ?
Sr2b Fe1b C2b 16_655 . 3_665 72.0(4) ?
Sr2b Fe1b C1b 16_655 . . 67.54(3) ?
Sr2b Fe1b Sr2b 17_435 . 18_455 106.33(4) ?
Sr2b Fe1b C2b 17_435 . 1_455 73.0(2) ?
Sr2b Fe1b C2b 17_435 . 2_545 72.0(2) ?
Sr2b Fe1b C2b 17_435 . 3_665 177.8(2) ?
Sr2b Fe1b C1b 17_435 . . 67.54(3) ?
Sr2b Fe1b C2b 18_455 . 1_455 72.0(3) ?
Sr2b Fe1b C2b 18_455 . 2_545 177.8(2) ?
Sr2b Fe1b C2b 18_455 . 3_665 73.0(3) ?
Sr2b Fe1b C1b 18_455 . . 67.54(3) ?
C2b Fe1b C2b 1_455 . 2_545 108.6(4) ?
C2b Fe1b C2b 1_455 . 3_665 108.6(4) ?
C2b Fe1b C1b 1_455 . . 110.3(2) ?
C2b Fe1b C2b 2_545 . 3_665 108.6(4) ?
C2b Fe1b C1b 2_545 . . 110.3(2) ?
C2b Fe1b C1b 3_665 . . 110.3(2) ?
Sr1 N3ab Sr1 7_444 . 8_554 91.21(19) ?
Sr1 N3ab Sr1 7_444 . 9_454 91.21(18) ?
Sr1 N3ab Sr2a 7_444 . 7_444 97.68(3) ?
Sr1 N3ab Sr2a 7_444 . 8_554 79.75(3) ?
Sr1 N3ab Sr2a 7_444 . 9_454 167.40(4) ?
Sr1 N3ab Sr2b 7_444 . 1_445 93.21(3) ?
Sr1 N3ab Sr2b 7_444 . 2_655 172.88(5) ?
Sr1 N3ab Sr2b 7_444 . 3_565 83.13(3) ?
Sr1 N3ab N1c 7_444 . 13_444 55.60(13) ?
Sr1 N3ab C1c 7_444 . 4_554 124.40(13) ?
Sr1 N3ab Sr1 8_554 . 9_454 91.21(19) ?
Sr1 N3ab Sr2a 8_554 . 7_444 167.40(5) ?
Sr1 N3ab Sr2a 8_554 . 8_554 97.68(3) ?
Sr1 N3ab Sr2a 8_554 . 9_454 79.75(3) ?
Sr1 N3ab Sr2b 8_554 . 1_445 83.13(3) ?
Sr1 N3ab Sr2b 8_554 . 2_655 93.21(4) ?
Sr1 N3ab Sr2b 8_554 . 3_565 172.88(6) ?
Sr1 N3ab N1c 8_554 . 13_444 55.60(13) ?
Sr1 N3ab C1c 8_554 . 4_554 124.40(13) ?
Sr1 N3ab Sr2a 9_454 . 7_444 79.75(3) ?
Sr1 N3ab Sr2a 9_454 . 8_554 167.40(3) ?
Sr1 N3ab Sr2a 9_454 . 9_454 97.68(3) ?
Sr1 N3ab Sr2b 9_454 . 1_445 172.88(5) ?
Sr1 N3ab Sr2b 9_454 . 2_655 83.13(3) ?
Sr1 N3ab Sr2b 9_454 . 3_565 93.21(3) ?
Sr1 N3ab N1c 9_454 . 13_444 55.60(13) ?
Sr1 N3ab C1c 9_454 . 4_554 124.40(13) ?
Sr2a N3ab Sr2a 7_444 . 8_554 92.7(2) ?
Sr2a N3ab Sr2a 7_444 . 9_454 92.7(2) ?
Sr2a N3ab Sr2b 7_444 . 1_445 105.1(2) ?
Sr2a N3ab Sr2b 7_444 . 2_655 77.12(15) ?
Sr2a N3ab Sr2b 7_444 . 3_565 19.67(5) ?
Sr2a N3ab N1c 7_444 . 13_444 123.34(15) ?
Sr2a N3ab C1c 7_444 . 4_554 56.66(15) ?
Sr2a N3ab Sr2a 8_554 . 9_454 92.7(2) ?
Sr2a N3ab Sr2b 8_554 . 1_445 19.67(4) ?
Sr2a N3ab Sr2b 8_554 . 2_655 105.1(2) ?
Sr2a N3ab Sr2b 8_554 . 3_565 77.12(15) ?
Sr2a N3ab N1c 8_554 . 13_444 123.34(15) ?
Sr2a N3ab C1c 8_554 . 4_554 56.66(15) ?
Sr2a N3ab Sr2b 9_454 . 1_445 77.12(15) ?
Sr2a N3ab Sr2b 9_454 . 2_655 19.67(4) ?
Sr2a N3ab Sr2b 9_454 . 3_565 105.1(2) ?
Sr2a N3ab N1c 9_454 . 13_444 123.34(15) ?
Sr2a N3ab C1c 9_454 . 4_554 56.66(15) ?
Sr2b N3ab Sr2b 1_445 . 2_655 92.9(2) ?
Sr2b N3ab Sr2b 1_445 . 3_565 92.9(2) ?
Sr2b N3ab N1c 1_445 . 13_444 123.22(15) ?
Sr2b N3ab C1c 1_445 . 4_554 56.78(15) ?
Sr2b N3ab Sr2b 2_655 . 3_565 92.9(2) ?
Sr2b N3ab N1c 2_655 . 13_444 123.21(15) ?
Sr2b N3ab C1c 2_655 . 4_554 56.78(15) ?
Sr2b N3ab N1c 3_565 . 13_444 123.22(15) ?
Sr2b N3ab C1c 3_565 . 4_554 56.78(15) ?
N1c N3ab C1c 13_444 . 4_554 180 ?
Sr1 N1c Sr1 13_544 . 14_654 103.7(3) ?
Sr1 N1c Sr1 13_544 . 15_554 103.7(3) ?
Sr1 N1c Sr2a 13_544 . 13_544 96.14(9) ?
Sr1 N1c Sr2a 13_544 . 14_654 78.55(8) ?
Sr1 N1c Sr2a 13_544 . 15_554 158.7(4) ?
Sr1 N1c Sr2b 13_544 . 7_445 91.76(9) ?
Sr1 N1c Sr2b 13_544 . 8_655 161.6(4) ?
Sr1 N1c Sr2b 13_544 . 9_565 81.87(8) ?
Sr1 N1c N3ab 13_544 . 7_555 114.8(3) ?
Sr1 N1c C1c 13_544 . 10_554 114.8(3) ?
Sr1 N1c Sr1 14_654 . 15_554 103.7(3) ?
Sr1 N1c Sr2a 14_654 . 13_544 158.7(4) ?
Sr1 N1c Sr2a 14_654 . 14_654 96.14(10) ?
Sr1 N1c Sr2a 14_654 . 15_554 78.55(8) ?
Sr1 N1c Sr2b 14_654 . 7_445 81.87(8) ?
Sr1 N1c Sr2b 14_654 . 8_655 91.76(9) ?
Sr1 N1c Sr2b 14_654 . 9_565 161.6(4) ?
Sr1 N1c N3ab 14_654 . 7_555 114.8(3) ?
Sr1 N1c C1c 14_654 . 10_554 114.8(3) ?
Sr1 N1c Sr2a 15_554 . 13_544 78.55(8) ?
Sr1 N1c Sr2a 15_554 . 14_654 158.7(4) ?
Sr1 N1c Sr2a 15_554 . 15_554 96.14(10) ?
Sr1 N1c Sr2b 15_554 . 7_445 161.6(4) ?
Sr1 N1c Sr2b 15_554 . 8_655 81.87(8) ?
Sr1 N1c Sr2b 15_554 . 9_565 91.76(9) ?
Sr1 N1c N3ab 15_554 . 7_555 114.8(3) ?
Sr1 N1c C1c 15_554 . 10_554 114.8(3) ?
Sr2a N1c Sr2a 13_544 . 14_654 80.2(3) ?
Sr2a N1c Sr2a 13_544 . 15_554 80.2(3) ?
Sr2a N1c Sr2b 13_544 . 7_445 90.0(3) ?
Sr2a N1c Sr2b 13_544 . 8_655 67.4(2) ?
Sr2a N1c Sr2b 13_544 . 9_565 17.50(6) ?
Sr2a N1c N3ab 13_544 . 7_555 48.03(19) ?
Sr2a N1c C1c 13_544 . 10_554 48.03(19) ?
Sr2a N1c Sr2a 14_654 . 15_554 80.2(3) ?
Sr2a N1c Sr2b 14_654 . 7_445 17.50(6) ?
Sr2a N1c Sr2b 14_654 . 8_655 90.0(3) ?
Sr2a N1c Sr2b 14_654 . 9_565 67.4(2) ?
Sr2a N1c N3ab 14_654 . 7_555 48.03(19) ?
Sr2a N1c C1c 14_654 . 10_554 48.03(19) ?
Sr2a N1c Sr2b 15_554 . 7_445 67.4(2) ?
Sr2a N1c Sr2b 15_554 . 8_655 17.50(6) ?
Sr2a N1c Sr2b 15_554 . 9_565 90.0(3) ?
Sr2a N1c N3ab 15_554 . 7_555 48.04(19) ?
Sr2a N1c C1c 15_554 . 10_554 48.03(19) ?
Sr2b N1c Sr2b 7_445 . 8_655 80.4(3) ?
Sr2b N1c Sr2b 7_445 . 9_565 80.4(3) ?
Sr2b N1c N3ab 7_445 . 7_555 48.17(19) ?
Sr2b N1c C1c 7_445 . 10_554 48.17(19) ?
Sr2b N1c Sr2b 8_655 . 9_565 80.4(3) ?
Sr2b N1c N3ab 8_655 . 7_555 48.17(19) ?
Sr2b N1c C1c 8_655 . 10_554 48.17(19) ?
Sr2b N1c N3ab 9_565 . 7_555 48.17(19) ?
Sr2b N1c C1c 9_565 . 10_554 48.17(19) ?
N3ab N1c C1c 7_555 . 10_554 0 ?
Sr1 N2c Sr2c 14_654 . 16_655 102.4(3) ?
Sr1 N2c N2a 14_654 . 15_654 130.0(10) ?
Sr1 N2c C2a 14_654 . 15_654 126.3(9) ?
Sr1 N2c N2b 14_654 . 8_545 128.4(9) ?
Sr1 N2c C2c 14_654 . . 162.0(7) ?
Sr1 N2c C2b 14_654 . 8_545 127.2(13) ?
Sr2c N2c N2a 16_655 . 15_654 116.4(9) ?
Sr2c N2c C2a 16_655 . 15_654 62.3(10) ?
Sr2c N2c N2b 16_655 . 8_545 116.1(9) ?
Sr2c N2c C2c 16_655 . . 95.6(6) ?
Sr2c N2c C2b 16_655 . 8_545 60.3(8) ?
N2a N2c C2a 15_654 . 15_654 100.1(15) ?
N2a N2c N2b 15_654 . 8_545 60.0(12) ?
N2a N2c C2c 15_654 . . 37.6(9) ?
N2a N2c C2b 15_654 . 8_545 59.9(11) ?
C2a N2c N2b 15_654 . 8_545 57.1(12) ?
C2a N2c C2c 15_654 . . 62.6(11) ?
C2a N2c C2b 15_654 . 8_545 91.4(13) ?
N2b N2c C2c 8_545 . . 39.2(8) ?
N2b N2c C2b 8_545 . 8_545 102.1(15) ?
C2c N2c C2b . . 8_545 62.9(12) ?
Sr1 N2b Sr1 7_544 . 9_454 90.4(3) ?
Sr1 N2b Sr2b 7_544 . 16_655 137.9(3) ?
Sr1 N2b N2a 7_544 . 8_544 83.3(8) ?
Sr1 N2b C2a 7_544 . 8_544 79.9(7) ?
Sr1 N2b N2c 7_544 . 15_654 39.4(8) ?
Sr1 N2b C2c 7_544 . 15_654 136.8(12) ?
Sr1 N2b C2b 7_544 . . 76.0(4) ?
Sr1 N2b Sr2b 9_454 . 16_655 99.5(3) ?
Sr1 N2b N2a 9_454 . 8_544 133.0(9) ?
Sr1 N2b C2a 9_454 . 8_544 122.5(13) ?
Sr1 N2b N2c 9_454 . 15_654 129.7(10) ?
Sr1 N2b C2c 9_454 . 15_654 128.3(9) ?
Sr1 N2b C2b 9_454 . . 164.5(7) ?
Sr2b N2b N2a 16_655 . 8_544 116.1(9) ?
Sr2b N2b C2a 16_655 . 8_544 60.3(8) ?
Sr2b N2b N2c 16_655 . 15_654 116.4(9) ?
Sr2b N2b C2c 16_655 . 15_654 62.3(10) ?
Sr2b N2b C2b 16_655 . . 95.6(6) ?
N2a N2b C2a 8_544 . 8_544 102.1(15) ?
N2a N2b N2c 8_544 . 15_654 60.0(12) ?
N2a N2b C2c 8_544 . 15_654 57.1(12) ?
N2a N2b C2b 8_544 . . 39.2(8) ?
C2a N2b N2c 8_544 . 15_654 59.9(11) ?
C2a N2b C2c 8_544 . 15_654 91.4(13) ?
C2a N2b C2b 8_544 . . 62.9(12) ?
N2c N2b C2c 15_654 . 15_654 100.1(15) ?
N2c N2b C2b 15_654 . . 37.6(9) ?
C2c N2b C2b 15_654 . . 62.6(11) ?
Sr1 N1b Sr1 7_544 . 8_664 103.1(3) ?
Sr1 N1b Sr1 7_544 . 9_454 103.1(3) ?
Sr1 N1b Sr2a 7_544 . 7_444 159.5(4) ?
Sr1 N1b Sr2a 7_544 . 8_654 79.14(9) ?
Sr1 N1b Sr2a 7_544 . 9_564 96.04(10) ?
Sr1 N1b Sr2c 7_544 . 13_544 82.07(9) ?
Sr1 N1b Sr2c 7_544 . 14_654 161.7(4) ?
Sr1 N1b Sr2c 7_544 . 15_554 92.54(10) ?
Sr1 N1b N3ac 7_544 . 7_554 115.3(3) ?
Sr1 N1b C1b 7_544 . 10_554 115.3(3) ?
Sr1 N1b Sr1 8_664 . 9_454 103.1(3) ?
Sr1 N1b Sr2a 8_664 . 7_444 96.04(10) ?
Sr1 N1b Sr2a 8_664 . 8_654 159.5(4) ?
Sr1 N1b Sr2a 8_664 . 9_564 79.14(8) ?
Sr1 N1b Sr2c 8_664 . 13_544 92.54(9) ?
Sr1 N1b Sr2c 8_664 . 14_654 82.07(9) ?
Sr1 N1b Sr2c 8_664 . 15_554 161.7(4) ?
Sr1 N1b N3ac 8_664 . 7_554 115.3(3) ?
Sr1 N1b C1b 8_664 . 10_554 115.3(3) ?
Sr1 N1b Sr2a 9_454 . 7_444 79.14(9) ?
Sr1 N1b Sr2a 9_454 . 8_654 96.04(10) ?
Sr1 N1b Sr2a 9_454 . 9_564 159.5(4) ?
Sr1 N1b Sr2c 9_454 . 13_544 161.7(4) ?
Sr1 N1b Sr2c 9_454 . 14_654 92.54(9) ?
Sr1 N1b Sr2c 9_454 . 15_554 82.07(9) ?
Sr1 N1b N3ac 9_454 . 7_554 115.3(3) ?
Sr1 N1b C1b 9_454 . 10_554 115.3(3) ?
Sr2a N1b Sr2a 7_444 . 8_654 80.4(3) ?
Sr2a N1b Sr2a 7_444 . 9_564 80.4(3) ?
Sr2a N1b Sr2c 7_444 . 13_544 90.0(3) ?
Sr2a N1b Sr2c 7_444 . 14_654 17.50(6) ?
Sr2a N1b Sr2c 7_444 . 15_554 67.4(2) ?
Sr2a N1b N3ac 7_444 . 7_554 48.17(19) ?
Sr2a N1b C1b 7_444 . 10_554 48.17(19) ?
Sr2a N1b Sr2a 8_654 . 9_564 80.4(3) ?
Sr2a N1b Sr2c 8_654 . 13_544 67.4(2) ?
Sr2a N1b Sr2c 8_654 . 14_654 90.0(3) ?
Sr2a N1b Sr2c 8_654 . 15_554 17.50(6) ?
Sr2a N1b N3ac 8_654 . 7_554 48.17(19) ?
Sr2a N1b C1b 8_654 . 10_554 48.17(19) ?
Sr2a N1b Sr2c 9_564 . 13_544 17.50(6) ?
Sr2a N1b Sr2c 9_564 . 14_654 67.4(2) ?
Sr2a N1b Sr2c 9_564 . 15_554 90.0(3) ?
Sr2a N1b N3ac 9_564 . 7_554 48.17(19) ?
Sr2a N1b C1b 9_564 . 10_554 48.17(19) ?
Sr2c N1b Sr2c 13_544 . 14_654 80.2(3) ?
Sr2c N1b Sr2c 13_544 . 15_554 80.2(3) ?
Sr2c N1b N3ac 13_544 . 7_554 48.03(19) ?
Sr2c N1b C1b 13_544 . 10_554 48.03(19) ?
Sr2c N1b Sr2c 14_654 . 15_554 80.2(3) ?
Sr2c N1b N3ac 14_654 . 7_554 48.03(19) ?
Sr2c N1b C1b 14_654 . 10_554 48.03(19) ?
Sr2c N1b N3ac 15_554 . 7_554 48.04(19) ?
Sr2c N1b C1b 15_554 . 10_554 48.03(19) ?
N3ac N1b C1b 7_554 . 10_554 0 ?
Sr2a C2c Sr2a 10_654 . 11_544 86.9(2) ?
Sr2a C2c Sr2c 10_654 . 16_655 85.40(17) ?
Sr2a C2c Sr2c 10_654 . 18_555 99.1(2) ?
Sr2a C2c Sr2b 10_654 . 4_765 88.3(2) ?
Sr2a C2c Sr2b 10_654 . 6_555 15.69(7) ?
Sr2a C2c N2a 10_654 . 15_654 165.0(8) ?
Sr2a C2c C2a 10_654 . 15_654 86.7(6) ?
Sr2a C2c Fe1c 10_654 . 1_655 56.2(2) ?
Sr2a C2c N2c 10_654 . . 125.6(5) ?
Sr2a C2c N2b 10_654 . 8_545 102.8(10) ?
Sr2a C2c C2b 10_654 . 8_545 130.5(6) ?
Sr2a C2c Sr2c 11_544 . 16_655 69.9(2) ?
Sr2a C2c Sr2c 11_544 . 18_555 12.53(6) ?
Sr2a C2c Sr2b 11_544 . 4_765 15.67(5) ?
Sr2a C2c Sr2b 11_544 . 6_555 81.9(2) ?
Sr2a C2c N2a 11_544 . 15_654 104.1(9) ?
Sr2a C2c C2a 11_544 . 15_654 116.3(7) ?
Sr2a C2c Fe1c 11_544 . 1_655 68.3(2) ?
Sr2a C2c N2c 11_544 . . 115.7(7) ?
Sr2a C2c N2b 11_544 . 8_545 155.4(13) ?
Sr2a C2c C2b 11_544 . 8_545 78.1(5) ?
Sr2c C2c Sr2c 16_655 . 18_555 74.18(19) ?
Sr2c C2c Sr2b 16_655 . 4_765 85.6(2) ?
Sr2c C2c Sr2b 16_655 . 6_555 69.70(17) ?
Sr2c C2c N2a 16_655 . 15_654 88.8(11) ?
Sr2c C2c C2a 16_655 . 15_654 46.4(5) ?
Sr2c C2c Fe1c 16_655 . 1_655 123.4(3) ?
Sr2c C2c N2c 16_655 . . 61.4(5) ?
Sr2c C2c N2b 16_655 . 8_545 88.2(9) ?
Sr2c C2c C2b 16_655 . 8_545 45.1(5) ?
Sr2c C2c Sr2b 18_555 . 4_765 16.58(5) ?
Sr2c C2c Sr2b 18_555 . 6_555 94.5(2) ?
Sr2c C2c N2a 18_555 . 15_654 92.7(8) ?
Sr2c C2c C2a 18_555 . 15_654 119.7(7) ?
Sr2c C2c Fe1c 18_555 . 1_655 73.3(2) ?
Sr2c C2c N2c 18_555 . . 110.0(7) ?
Sr2c C2c N2b 18_555 . 8_545 150.6(13) ?
Sr2c C2c C2b 18_555 . 8_545 72.4(5) ?
Sr2b C2c Sr2b 4_765 . 6_555 87.4(2) ?
Sr2b C2c N2a 4_765 . 15_654 105.1(8) ?
Sr2b C2c C2a 4_765 . 15_654 132.0(7) ?
Sr2b C2c Fe1c 4_765 . 1_655 56.77(16) ?
Sr2b C2c N2c 4_765 . . 126.6(7) ?
Sr2b C2c N2b 4_765 . 8_545 166.8(13) ?
Sr2b C2c C2b 4_765 . 8_545 89.0(5) ?
Sr2b C2c N2a 6_555 . 15_654 154.5(10) ?
Sr2b C2c C2a 6_555 . 15_654 75.9(6) ?
Sr2b C2c Fe1c 6_555 . 1_655 68.1(3) ?
Sr2b C2c N2c 6_555 . . 114.6(5) ?
Sr2b C2c N2b 6_555 . 8_545 101.4(9) ?
Sr2b C2c C2b 6_555 . 8_545 114.8(6) ?
N2a C2c C2a 15_654 . 15_654 79.3(11) ?
N2a C2c Fe1c 15_654 . 1_655 137.3(10) ?
N2a C2c N2c 15_654 . . 40.3(9) ?
N2a C2c N2b 15_654 . 8_545 63.1(12) ?
N2a C2c C2b 15_654 . 8_545 45.1(11) ?
C2a C2c Fe1c 15_654 . 1_655 142.8(8) ?
C2a C2c N2c 15_654 . . 39.0(6) ?
C2a C2c N2b 15_654 . 8_545 43.5(8) ?
C2a C2c C2b 15_654 . 8_545 60.0(8) ?
Fe1c C2c N2c 1_655 . . 175.1(7) ?
Fe1c C2c N2b 1_655 . 8_545 135.7(13) ?
Fe1c C2c C2b 1_655 . 8_545 145.8(6) ?
N2c C2c N2b . . 8_545 40.7(11) ?
N2c C2c C2b . . 8_545 37.8(6) ?
N2b C2c C2b 8_545 . 8_545 78.4(13) ?
Sr1 C2b Sr1 7_544 . 8_654 83.85(18) ?
Sr1 C2b Sr2a 7_544 . 4_764 87.05(17) ?
Sr1 C2b Sr2a 7_544 . 6_554 164.4(4) ?
Sr1 C2b Sr2c 7_544 . 10_654 149.4(3) ?
Sr1 C2b Sr2c 7_544 . 11_544 96.1(2) ?
Sr1 C2b Sr2b 7_544 . 16_655 124.3(3) ?
Sr1 C2b Sr2b 7_544 . 18_555 84.11(18) ?
Sr1 C2b N2a 7_544 . 8_544 86.8(8) ?
Sr1 C2b C2a 7_544 . 8_544 79.6(5) ?
Sr1 C2b Fe1b 7_544 . 1_655 96.7(2) ?
Sr1 C2b N2c 7_544 . 15_654 40.9(9) ?
Sr1 C2b N2b 7_544 . . 80.3(5) ?
Sr1 C2b C2c 7_544 . 15_654 118.2(7) ?
Sr1 C2b Sr2a 8_654 . 4_764 145.8(3) ?
Sr1 C2b Sr2a 8_654 . 6_554 92.7(3) ?
Sr1 C2b Sr2c 8_654 . 10_654 83.2(2) ?
Sr1 C2b Sr2c 8_654 . 11_544 159.9(4) ?
Sr1 C2b Sr2b 8_654 . 16_655 126.3(2) ?
Sr1 C2b Sr2b 8_654 . 18_555 159.5(3) ?
Sr1 C2b N2a 8_654 . 8_544 44.6(11) ?
Sr1 C2b C2a 8_654 . 8_544 121.4(6) ?
Sr1 C2b Fe1b 8_654 . 1_655 91.6(4) ?
Sr1 C2b N2c 8_654 . 15_654 89.1(9) ?
Sr1 C2b N2b 8_654 . . 84.2(5) ?
Sr1 C2b C2c 8_654 . 15_654 80.7(6) ?
Sr2a C2b Sr2a 4_764 . 6_554 87.4(2) ?
Sr2a C2b Sr2c 4_764 . 10_654 88.3(2) ?
Sr2a C2b Sr2c 4_764 . 11_544 15.67(5) ?
Sr2a C2b Sr2b 4_764 . 16_655 85.6(2) ?
Sr2a C2b Sr2b 4_764 . 18_555 16.58(5) ?
Sr2a C2b N2a 4_764 . 8_544 166.8(13) ?
Sr2a C2b C2a 4_764 . 8_544 89.0(5) ?
Sr2a C2b Fe1b 4_764 . 1_655 56.77(16) ?
Sr2a C2b N2c 4_764 . 15_654 105.1(8) ?
Sr2a C2b N2b 4_764 . . 126.6(7) ?
Sr2a C2b C2c 4_764 . 15_654 132.0(7) ?
Sr2a C2b Sr2c 6_554 . 10_654 15.69(7) ?
Sr2a C2b Sr2c 6_554 . 11_544 81.9(2) ?
Sr2a C2b Sr2b 6_554 . 16_655 69.70(17) ?
Sr2a C2b Sr2b 6_554 . 18_555 94.5(2) ?
Sr2a C2b N2a 6_554 . 8_544 101.4(9) ?
Sr2a C2b C2a 6_554 . 8_544 114.8(6) ?
Sr2a C2b Fe1b 6_554 . 1_655 68.1(3) ?
Sr2a C2b N2c 6_554 . 15_654 154.5(10) ?
Sr2a C2b N2b 6_554 . . 114.6(5) ?
Sr2a C2b C2c 6_554 . 15_654 75.9(6) ?
Sr2c C2b Sr2c 10_654 . 11_544 86.9(2) ?
Sr2c C2b Sr2b 10_654 . 16_655 85.40(17) ?
Sr2c C2b Sr2b 10_654 . 18_555 99.1(2) ?
Sr2c C2b N2a 10_654 . 8_544 102.8(10) ?
Sr2c C2b C2a 10_654 . 8_544 130.5(6) ?
Sr2c C2b Fe1b 10_654 . 1_655 56.2(2) ?
Sr2c C2b N2c 10_654 . 15_654 165.0(8) ?
Sr2c C2b N2b 10_654 . . 125.6(5) ?
Sr2c C2b C2c 10_654 . 15_654 86.7(6) ?
Sr2c C2b Sr2b 11_544 . 16_655 69.9(2) ?
Sr2c C2b Sr2b 11_544 . 18_555 12.53(6) ?
Sr2c C2b N2a 11_544 . 8_544 155.4(13) ?
Sr2c C2b C2a 11_544 . 8_544 78.1(5) ?
Sr2c C2b Fe1b 11_544 . 1_655 68.3(2) ?
Sr2c C2b N2c 11_544 . 15_654 104.1(9) ?
Sr2c C2b N2b 11_544 . . 115.7(7) ?
Sr2c C2b C2c 11_544 . 15_654 116.3(7) ?
Sr2b C2b Sr2b 16_655 . 18_555 74.18(19) ?
Sr2b C2b N2a 16_655 . 8_544 88.2(9) ?
Sr2b C2b C2a 16_655 . 8_544 45.1(5) ?
Sr2b C2b Fe1b 16_655 . 1_655 123.4(3) ?
Sr2b C2b N2c 16_655 . 15_654 88.8(11) ?
Sr2b C2b N2b 16_655 . . 61.4(5) ?
Sr2b C2b C2c 16_655 . 15_654 46.4(5) ?
Sr2b C2b N2a 18_555 . 8_544 150.6(13) ?
Sr2b C2b C2a 18_555 . 8_544 72.4(5) ?
Sr2b C2b Fe1b 18_555 . 1_655 73.3(2) ?
Sr2b C2b N2c 18_555 . 15_654 92.7(8) ?
Sr2b C2b N2b 18_555 . . 110.0(7) ?
Sr2b C2b C2c 18_555 . 15_654 119.7(7) ?
N2a C2b C2a 8_544 . 8_544 78.4(13) ?
N2a C2b Fe1b 8_544 . 1_655 135.7(13) ?
N2a C2b N2c 8_544 . 15_654 63.1(12) ?
N2a C2b N2b 8_544 . . 40.7(11) ?
N2a C2b C2c 8_544 . 15_654 43.4(8) ?
C2a C2b Fe1b 8_544 . 1_655 145.8(6) ?
C2a C2b N2c 8_544 . 15_654 45.1(11) ?
C2a C2b N2b 8_544 . . 37.8(6) ?
C2a C2b C2c 8_544 . 15_654 60.0(8) ?
Fe1b C2b N2c 1_655 . 15_654 137.3(10) ?
Fe1b C2b N2b 1_655 . . 175.1(7) ?
Fe1b C2b C2c 1_655 . 15_654 142.8(8) ?
N2c C2b N2b 15_654 . . 40.3(9) ?
N2c C2b C2c 15_654 . 15_654 79.3(11) ?
N2b C2b C2c . . 15_654 39.0(6) ?
Sr2a C1a Sr2a 16_654 . 17_434 114.50(17) ?
Sr2a C1a Sr2a 16_654 . 18_454 114.50(17) ?
Sr2a C1a Fe1a 16_654 . . 76.2(2) ?
Sr2a C1a Sr2c 16_654 . 4_664 102.24(18) ?
Sr2a C1a Sr2c 16_654 . 5_544 12.25(2) ?
Sr2a C1a Sr2c 16_654 . 6_454 122.9(3) ?
Sr2a C1a Sr2b 16_654 . 10_554 102.49(18) ?
Sr2a C1a Sr2b 16_654 . 11_444 122.6(3) ?
Sr2a C1a Sr2b 16_654 . 12_454 12.00(3) ?
Sr2a C1a N1a 16_654 . 16_554 103.8(2) ?
Sr2a C1a N3bc 16_654 . 4_554 103.8(2) ?
Sr2a C1a Sr2a 17_434 . 18_454 114.50(17) ?
Sr2a C1a Fe1a 17_434 . . 76.2(2) ?
Sr2a C1a Sr2c 17_434 . 4_664 122.9(3) ?
Sr2a C1a Sr2c 17_434 . 5_544 102.24(18) ?
Sr2a C1a Sr2c 17_434 . 6_454 12.25(4) ?
Sr2a C1a Sr2b 17_434 . 10_554 12.00(3) ?
Sr2a C1a Sr2b 17_434 . 11_444 102.49(18) ?
Sr2a C1a Sr2b 17_434 . 12_454 122.6(3) ?
Sr2a C1a N1a 17_434 . 16_554 103.8(2) ?
Sr2a C1a N3bc 17_434 . 4_554 103.8(2) ?
Sr2a C1a Fe1a 18_454 . . 76.2(2) ?
Sr2a C1a Sr2c 18_454 . 4_664 12.25(3) ?
Sr2a C1a Sr2c 18_454 . 5_544 122.9(3) ?
Sr2a C1a Sr2c 18_454 . 6_454 102.24(18) ?
Sr2a C1a Sr2b 18_454 . 10_554 122.6(3) ?
Sr2a C1a Sr2b 18_454 . 11_444 12.00(3) ?
Sr2a C1a Sr2b 18_454 . 12_454 102.49(18) ?
Sr2a C1a N1a 18_454 . 16_554 103.8(2) ?
Sr2a C1a N3bc 18_454 . 4_554 103.8(2) ?
Fe1a C1a Sr2c . . 4_664 71.9(3) ?
Fe1a C1a Sr2c . . 5_544 71.9(3) ?
Fe1a C1a Sr2c . . 6_454 71.9(3) ?
Fe1a C1a Sr2b . . 10_554 71.8(3) ?
Fe1a C1a Sr2b . . 11_444 71.8(3) ?
Fe1a C1a Sr2b . . 12_454 71.8(3) ?
Fe1a C1a N1a . . 16_554 180 ?
Fe1a C1a N3bc . . 4_554 180 ?
Sr2c C1a Sr2c 4_664 . 5_544 110.8(3) ?
Sr2c C1a Sr2c 4_664 . 6_454 110.8(3) ?
Sr2c C1a Sr2b 4_664 . 10_554 129.0(4) ?
Sr2c C1a Sr2b 4_664 . 11_444 22.39(5) ?
Sr2c C1a Sr2b 4_664 . 12_454 90.24(19) ?
Sr2c C1a N1a 4_664 . 16_554 108.1(3) ?
Sr2c C1a N3bc 4_664 . 4_554 108.1(3) ?
Sr2c C1a Sr2c 5_544 . 6_454 110.8(3) ?
Sr2c C1a Sr2b 5_544 . 10_554 90.24(19) ?
Sr2c C1a Sr2b 5_544 . 11_444 129.0(4) ?
Sr2c C1a Sr2b 5_544 . 12_454 22.39(5) ?
Sr2c C1a N1a 5_544 . 16_554 108.1(3) ?
Sr2c C1a N3bc 5_544 . 4_554 108.1(3) ?
Sr2c C1a Sr2b 6_454 . 10_554 22.39(5) ?
Sr2c C1a Sr2b 6_454 . 11_444 90.24(19) ?
Sr2c C1a Sr2b 6_454 . 12_454 129.0(4) ?
Sr2c C1a N1a 6_454 . 16_554 108.1(3) ?
Sr2c C1a N3bc 6_454 . 4_554 108.1(3) ?
Sr2b C1a Sr2b 10_554 . 11_444 110.7(3) ?
Sr2b C1a Sr2b 10_554 . 12_454 110.7(3) ?
Sr2b C1a N1a 10_554 . 16_554 108.2(3) ?
Sr2b C1a N3bc 10_554 . 4_554 108.2(3) ?
Sr2b C1a Sr2b 11_444 . 12_454 110.7(3) ?
Sr2b C1a N1a 11_444 . 16_554 108.2(3) ?
Sr2b C1a N3bc 11_444 . 4_554 108.2(3) ?
Sr2b C1a N1a 12_454 . 16_554 108.2(3) ?
Sr2b C1a N3bc 12_454 . 4_554 108.2(3) ?
N1a C1a N3bc 16_554 . 4_554 0 ?
Sr2a C1c Sr2a 10_554 . 11_444 110.7(3) ?
Sr2a C1c Sr2a 10_554 . 12_454 110.7(3) ?
Sr2a C1c Sr2c 10_554 . 16_655 102.49(18) ?
Sr2a C1c Sr2c 10_554 . 17_435 12.00(3) ?
Sr2a C1c Sr2c 10_554 . 18_455 122.6(3) ?
Sr2a C1c Sr2b 10_554 . 4_665 129.0(4) ?
Sr2a C1c Sr2b 10_554 . 5_545 90.24(19) ?
Sr2a C1c Sr2b 10_554 . 6_455 22.39(5) ?
Sr2a C1c Fe1c 10_554 . . 71.8(3) ?
Sr2a C1c N3ab 10_554 . 4_555 108.2(3) ?
Sr2a C1c N1c 10_554 . 16_555 108.2(3) ?
Sr2a C1c Sr2a 11_444 . 12_454 110.7(3) ?
Sr2a C1c Sr2c 11_444 . 16_655 122.6(3) ?
Sr2a C1c Sr2c 11_444 . 17_435 102.49(18) ?
Sr2a C1c Sr2c 11_444 . 18_455 12.00(3) ?
Sr2a C1c Sr2b 11_444 . 4_665 22.39(5) ?
Sr2a C1c Sr2b 11_444 . 5_545 129.0(4) ?
Sr2a C1c Sr2b 11_444 . 6_455 90.24(19) ?
Sr2a C1c Fe1c 11_444 . . 71.8(3) ?
Sr2a C1c N3ab 11_444 . 4_555 108.2(3) ?
Sr2a C1c N1c 11_444 . 16_555 108.2(3) ?
Sr2a C1c Sr2c 12_454 . 16_655 12.00(3) ?
Sr2a C1c Sr2c 12_454 . 17_435 122.6(3) ?
Sr2a C1c Sr2c 12_454 . 18_455 102.49(18) ?
Sr2a C1c Sr2b 12_454 . 4_665 90.24(19) ?
Sr2a C1c Sr2b 12_454 . 5_545 22.39(5) ?
Sr2a C1c Sr2b 12_454 . 6_455 129.0(4) ?
Sr2a C1c Fe1c 12_454 . . 71.8(3) ?
Sr2a C1c N3ab 12_454 . 4_555 108.2(3) ?
Sr2a C1c N1c 12_454 . 16_555 108.2(3) ?
Sr2c C1c Sr2c 16_655 . 17_435 114.50(17) ?
Sr2c C1c Sr2c 16_655 . 18_455 114.50(17) ?
Sr2c C1c Sr2b 16_655 . 4_665 102.24(18) ?
Sr2c C1c Sr2b 16_655 . 5_545 12.25(2) ?
Sr2c C1c Sr2b 16_655 . 6_455 122.9(3) ?
Sr2c C1c Fe1c 16_655 . . 76.2(2) ?
Sr2c C1c N3ab 16_655 . 4_555 103.8(2) ?
Sr2c C1c N1c 16_655 . 16_555 103.8(2) ?
Sr2c C1c Sr2c 17_435 . 18_455 114.50(17) ?
Sr2c C1c Sr2b 17_435 . 4_665 122.9(3) ?
Sr2c C1c Sr2b 17_435 . 5_545 102.24(18) ?
Sr2c C1c Sr2b 17_435 . 6_455 12.25(4) ?
Sr2c C1c Fe1c 17_435 . . 76.2(2) ?
Sr2c C1c N3ab 17_435 . 4_555 103.8(2) ?
Sr2c C1c N1c 17_435 . 16_555 103.8(2) ?
Sr2c C1c Sr2b 18_455 . 4_665 12.25(3) ?
Sr2c C1c Sr2b 18_455 . 5_545 122.9(3) ?
Sr2c C1c Sr2b 18_455 . 6_455 102.24(18) ?
Sr2c C1c Fe1c 18_455 . . 76.2(2) ?
Sr2c C1c N3ab 18_455 . 4_555 103.8(2) ?
Sr2c C1c N1c 18_455 . 16_555 103.8(2) ?
Sr2b C1c Sr2b 4_665 . 5_545 110.8(3) ?
Sr2b C1c Sr2b 4_665 . 6_455 110.8(3) ?
Sr2b C1c Fe1c 4_665 . . 71.9(3) ?
Sr2b C1c N3ab 4_665 . 4_555 108.1(3) ?
Sr2b C1c N1c 4_665 . 16_555 108.1(3) ?
Sr2b C1c Sr2b 5_545 . 6_455 110.8(3) ?
Sr2b C1c Fe1c 5_545 . . 71.9(3) ?
Sr2b C1c N3ab 5_545 . 4_555 108.1(3) ?
Sr2b C1c N1c 5_545 . 16_555 108.1(3) ?
Sr2b C1c Fe1c 6_455 . . 71.9(3) ?
Sr2b C1c N3ab 6_455 . 4_555 108.1(3) ?
Sr2b C1c N1c 6_455 . 16_555 108.1(3) ?
Fe1c C1c N3ab . . 4_555 180 ?
Fe1c C1c N1c . . 16_555 180 ?
N3ab C1c N1c 4_555 . 16_555 0 ?
Sr2a C1b Sr2a 4_664 . 5_544 110.8(3) ?
Sr2a C1b Sr2a 4_664 . 6_454 110.8(3) ?
Sr2a C1b Sr2c 4_664 . 10_554 129.0(4) ?
Sr2a C1b Sr2c 4_664 . 11_444 22.39(5) ?
Sr2a C1b Sr2c 4_664 . 12_454 90.24(19) ?
Sr2a C1b Sr2b 4_664 . 16_655 102.24(18) ?
Sr2a C1b Sr2b 4_664 . 17_435 122.9(3) ?
Sr2a C1b Sr2b 4_664 . 18_455 12.25(3) ?
Sr2a C1b N3ac 4_664 . 4_554 108.1(3) ?
Sr2a C1b Fe1b 4_664 . . 71.9(3) ?
Sr2a C1b N1b 4_664 . 16_555 108.1(3) ?
Sr2a C1b Sr2a 5_544 . 6_454 110.8(3) ?
Sr2a C1b Sr2c 5_544 . 10_554 90.24(19) ?
Sr2a C1b Sr2c 5_544 . 11_444 129.0(4) ?
Sr2a C1b Sr2c 5_544 . 12_454 22.39(5) ?
Sr2a C1b Sr2b 5_544 . 16_655 12.25(2) ?
Sr2a C1b Sr2b 5_544 . 17_435 102.24(18) ?
Sr2a C1b Sr2b 5_544 . 18_455 122.9(3) ?
Sr2a C1b N3ac 5_544 . 4_554 108.1(3) ?
Sr2a C1b Fe1b 5_544 . . 71.9(3) ?
Sr2a C1b N1b 5_544 . 16_555 108.1(3) ?
Sr2a C1b Sr2c 6_454 . 10_554 22.39(5) ?
Sr2a C1b Sr2c 6_454 . 11_444 90.24(19) ?
Sr2a C1b Sr2c 6_454 . 12_454 129.0(4) ?
Sr2a C1b Sr2b 6_454 . 16_655 122.9(3) ?
Sr2a C1b Sr2b 6_454 . 17_435 12.25(4) ?
Sr2a C1b Sr2b 6_454 . 18_455 102.24(18) ?
Sr2a C1b N3ac 6_454 . 4_554 108.1(3) ?
Sr2a C1b Fe1b 6_454 . . 71.9(3) ?
Sr2a C1b N1b 6_454 . 16_555 108.1(3) ?
Sr2c C1b Sr2c 10_554 . 11_444 110.7(3) ?
Sr2c C1b Sr2c 10_554 . 12_454 110.7(3) ?
Sr2c C1b Sr2b 10_554 . 16_655 102.49(18) ?
Sr2c C1b Sr2b 10_554 . 17_435 12.00(3) ?
Sr2c C1b Sr2b 10_554 . 18_455 122.6(3) ?
Sr2c C1b N3ac 10_554 . 4_554 108.2(3) ?
Sr2c C1b Fe1b 10_554 . . 71.8(3) ?
Sr2c C1b N1b 10_554 . 16_555 108.2(3) ?
Sr2c C1b Sr2c 11_444 . 12_454 110.7(3) ?
Sr2c C1b Sr2b 11_444 . 16_655 122.6(3) ?
Sr2c C1b Sr2b 11_444 . 17_435 102.49(18) ?
Sr2c C1b Sr2b 11_444 . 18_455 12.00(3) ?
Sr2c C1b N3ac 11_444 . 4_554 108.2(3) ?
Sr2c C1b Fe1b 11_444 . . 71.8(3) ?
Sr2c C1b N1b 11_444 . 16_555 108.2(3) ?
Sr2c C1b Sr2b 12_454 . 16_655 12.00(3) ?
Sr2c C1b Sr2b 12_454 . 17_435 122.6(3) ?
Sr2c C1b Sr2b 12_454 . 18_455 102.49(18) ?
Sr2c C1b N3ac 12_454 . 4_554 108.2(3) ?
Sr2c C1b Fe1b 12_454 . . 71.8(3) ?
Sr2c C1b N1b 12_454 . 16_555 108.2(3) ?
Sr2b C1b Sr2b 16_655 . 17_435 114.50(17) ?
Sr2b C1b Sr2b 16_655 . 18_455 114.50(17) ?
Sr2b C1b N3ac 16_655 . 4_554 103.8(2) ?
Sr2b C1b Fe1b 16_655 . . 76.2(2) ?
Sr2b C1b N1b 16_655 . 16_555 103.8(2) ?
Sr2b C1b Sr2b 17_435 . 18_455 114.50(17) ?
Sr2b C1b N3ac 17_435 . 4_554 103.8(2) ?
Sr2b C1b Fe1b 17_435 . . 76.2(2) ?
Sr2b C1b N1b 17_435 . 16_555 103.8(2) ?
Sr2b C1b N3ac 18_455 . 4_554 103.8(2) ?
Sr2b C1b Fe1b 18_455 . . 76.2(2) ?
Sr2b C1b N1b 18_455 . 16_555 103.8(2) ?
N3ac C1b Fe1b 4_554 . . 180 ?
N3ac C1b N1b 4_554 . 16_555 0 ?
Fe1b C1b N1b . . 16_555 180 ?




#=======================================================================

# 11. STRUCTURE-FACTOR LIST



_chemical_properties_physical    Air-sensitive,Moisture-sensitive
